 
data_manganoarrojadite-(KNa)
 
_audit_creation_method            'SHELXL-2018/3'
_shelx_SHELXL_version_number      '2018/3'
_chemical_name_systematic         'Potassium sodium manganese iron aluminium phosphate(V) hydroxide'
_chemical_name_common             'Manganoarrojadite-(KNa)'
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Al Ca0.12 H3.38 Fe9.10 K0.88 Mg1.10 Mn3.68 Na4.75 O50 P12' 
_chemical_formula_weight          2087.41

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mg'  'Mg'   0.0486   0.0363
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0645   0.0514
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K'  'K'   0.2009   0.2494
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.3463   0.8444
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            9
_space_group_name_H-M_alt         'C c'
_space_group_name_Hall            'C -2yc'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 'x, -y, z+1/2'
 'x+1/2, y+1/2, z'
 'x+1/2, -y+1/2, z+1/2'
loop_
_publ_author_name
'Lykova, I.'
'Rowe, R.'
'Poirier, G.'
'Helwig, K.'
'Friis, H.'
_cell_length_a                    16.5345(3)
_cell_length_b                    10.04057(19)
_cell_length_c                    24.6261(5)
_cell_angle_alpha                 90
_cell_angle_beta                  105.891(2)
_cell_angle_gamma                 90
_cell_volume                      3932.09(14)
_cell_formula_units_Z             4
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used   16682
_cell_measurement_theta_min     2.3870
_cell_measurement_theta_max     33.2990
 
_exptl_crystal_description        anhedral
_exptl_crystal_colour             'pale green'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     3.526          
_exptl_crystal_F_000              4038
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.058
_exptl_crystal_size_mid           0.040
_exptl_crystal_size_min           0.019
_exptl_absorpt_coefficient_mu     5.234
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type            gaussian
_exptl_absorpt_correction_T_min                     0.816
_exptl_absorpt_correction_T_max                     0.965
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.66a (Rigaku Oxford Diffraction, 2019)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source 'micro-focus sealed X-ray tube'
_diffrn_measurement_device_type 'Rigaku XtaLAB Synergy-S'
_diffrn_measurement_method        ?
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             21717
_diffrn_reflns_av_unetI/netI      0.0216
_diffrn_reflns_av_R_equivalents   0.0178
_diffrn_reflns_limit_h_min        -23
_diffrn_reflns_limit_h_max        25
_diffrn_reflns_limit_k_min        -14
_diffrn_reflns_limit_k_max        14
_diffrn_reflns_limit_l_min        -20
_diffrn_reflns_limit_l_max        35
_diffrn_reflns_theta_min          2.399
_diffrn_reflns_theta_max          33.389
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.881
_diffrn_measured_fraction_theta_full  0.998
_diffrn_reflns_Laue_measured_fraction_max    0.881
_diffrn_reflns_Laue_measured_fraction_full   0.998
_diffrn_reflns_point_group_measured_fraction_max   0.584
_diffrn_reflns_point_group_measured_fraction_full  0.722
_reflns_number_total              8918
_reflns_number_gt                 8515
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.325
_reflns_Friedel_fraction_max      0.287
_reflns_Friedel_fraction_full     0.446
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         ?
_computing_structure_solution     ?
_computing_structure_refinement 'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0380P)²+8.8751P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    .
_refine_ls_hydrogen_treatment     undef
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack    0.038(12)
_chemical_absolute_configuration  ?
_refine_ls_number_reflns          8918
_refine_ls_number_parameters      751
_refine_ls_number_restraints      2
_refine_ls_R_factor_all           0.0268
_refine_ls_R_factor_gt            0.0250
_refine_ls_wR_factor_ref          0.0655
_refine_ls_wR_factor_gt           0.0646
_refine_ls_goodness_of_fit_ref    1.029
_refine_ls_restrained_S_all       1.029
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
K1 K 0.99862(13) 0.50858(13) 0.24413(10) 0.0352(5) Uani 0.874(6) 1 d . . P . .
Na1 Na 0.0040(2) 0.9977(2) 0.99843(13) 0.0228(4) Uani 1 1 d . . . . .
Na2 Na 0.8736(3) 0.4867(2) 0.87784(12) 0.0443(9) Uani 1 1 d . . . . .
Na3 Na 0.29495(15) 0.4459(2) 0.04226(10) 0.0277(5) Uani 1 1 d . . . . .
Na4 Na 0.12151(18) 0.5116(2) 0.12095(10) 0.0221(5) Uani 1 1 d . . . . .
Na5 Na 0.02189(19) 0.8183(3) 0.77109(12) 0.0258(9) Uani 0.752(9) 1 d . . P . .
Mn Mn 0.23041(5) 0.78586(6) 0.97856(3) 0.01277(12) Uani 0.88 1 d . . P . .
Ca Ca 0.23041(5) 0.78586(6) 0.97856(3) 0.01277(12) Uani 0.12 1 d . . P . .
Fe1 Fe 0.22726(4) 0.11699(6) 0.97591(3) 0.01155(11) Uani 0.7 1 d . . P . .
Mn1 Mn 0.22726(4) 0.11699(6) 0.97591(3) 0.01155(11) Uani 0.3 1 d . . P . .
Fe2 Fe 0.28938(5) 0.51216(7) 0.22829(3) 0.01184(14) Uani 0.55 1 d . . P . .
Mn2 Mn 0.28938(5) 0.51216(7) 0.22829(3) 0.01184(14) Uani 0.3 1 d . . P . .
Mg2 Mg 0.28938(5) 0.51216(7) 0.22829(3) 0.01184(14) Uani 0.15 1 d . . P . .
Fe3 Fe 0.71499(5) 0.49329(7) 0.76594(3) 0.01128(13) Uani 0.7 1 d . . P . .
Mn3 Mn 0.71499(5) 0.49329(7) 0.76594(3) 0.01128(13) Uani 0.3 1 d . . P . .
Fe4 Fe 0.11254(5) 1.01474(8) 0.13706(4) 0.01063(15) Uani 0.7 1 d . . P . .
Mg4 Mg 0.11254(5) 1.01474(8) 0.13706(4) 0.01063(15) Uani 0.3 1 d . . P . .
Fe5 Fe 0.89613(6) 0.98862(8) 0.85777(4) 0.01060(15) Uani 0.7 1 d . . P . .
Mg5 Mg 0.89613(6) 0.98862(8) 0.85777(4) 0.01060(15) Uani 0.3 1 d . . P . .
Fe6 Fe 0.02154(4) 0.75148(7) 0.90041(3) 0.00914(13) Uani 0.9 1 d . . P . .
Mg6 Mg 0.02154(4) 0.75148(7) 0.90041(3) 0.00914(13) Uani 0.1 1 d . . P . .
Fe7 Fe 0.97754(4) 0.24724(7) 0.09333(3) 0.00769(13) Uani 0.85 1 d . . P . .
Mg7 Mg 0.97754(4) 0.24724(7) 0.09333(3) 0.00769(13) Uani 0.15 1 d . . P . .
Fe8 Fe 0.96960(4) 0.74714(6) 0.09624(3) 0.00800(12) Uani 1 1 d . . . . .
Fe9 Fe 0.03563(4) 0.26024(7) 0.89825(3) 0.00847(12) Uani 1 1 d . . . . .
Fe10 Fe 0.20642(4) 0.30592(7) 0.84961(3) 0.01099(13) Uani 0.6 1 d . . P . .
Mn10 Mn 0.20642(4) 0.30592(7) 0.84961(3) 0.01099(13) Uani 0.4 1 d . . P . .
Fe11 Fe 0.29818(5) 0.19937(8) 0.14574(3) 0.01431(15) Uani 0.4 1 d . . P . .
Mn11 Mn 0.29818(5) 0.19937(8) 0.14574(3) 0.01431(15) Uani 0.6 1 d . . P . .
Fe12 Fe 0.28452(4) 0.78871(7) 0.15165(3) 0.00970(13) Uani 0.6 1 d . . P . .
Mn12 Mn 0.28452(4) 0.78871(7) 0.15165(3) 0.00970(13) Uani 0.3 1 d . . P . .
Mg12 Mg 0.28452(4) 0.78871(7) 0.15165(3) 0.00970(13) Uani 0.1 1 d . . P . .
Fe13 Fe 0.22309(5) 0.29804(7) 0.34013(3) 0.01247(13) Uani 0.4 1 d . . P . .
Mn13 Mn 0.22309(5) 0.29804(7) 0.34013(3) 0.01247(13) Uani 0.6 1 d . . P . .
Al1 Al 0.00363(11) 0.50120(15) 0.99823(7) 0.00546(17) Uani 1 1 d . . . . .
P1 P 0.11752(7) 0.99477(9) 0.86640(5) 0.00653(17) Uani 1 1 d . . . . .
P2 P 0.42104(7) 0.49673(10) 0.16091(5) 0.00998(19) Uani 1 1 d . . . . .
P3 P 0.13261(7) 0.54033(12) 0.92281(5) 0.00668(18) Uani 1 1 d . . . . .
P4 P 0.87365(7) 0.46858(11) 0.07432(5) 0.00595(18) Uani 1 1 d . . . . .
P5 P 0.12924(7) 0.25278(11) 0.03774(5) 0.0063(2) Uani 1 1 d . . . . .
P6 P 0.37905(7) 0.25198(11) 0.96040(5) 0.0060(2) Uani 1 1 d . . . . .
P7 P 0.10895(7) 0.76482(11) 0.04545(5) 0.00644(19) Uani 1 1 d . . . . .
P8 P 0.90048(7) 0.23202(11) 0.95247(5) 0.00591(19) Uani 1 1 d . . . . .
P9 P 0.87083(7) 0.27580(12) 0.78599(5) 0.0077(2) Uani 1 1 d . . . . .
P10 P 0.13229(7) 0.72527(12) 0.20905(5) 0.00690(19) Uani 1 1 d . . . . .
P11 P 0.85859(8) 0.70521(12) 0.79109(5) 0.0097(2) Uani 1 1 d . . . . .
P12 P 0.14301(8) 0.29528(12) 0.20257(5) 0.0090(2) Uani 1 1 d . . . . .
O1 O 0.4803(2) 0.5613(3) 0.13091(15) 0.0136(6) Uani 1 1 d . . . . .
O2 O 1.0295(2) 0.9407(3) 0.86616(14) 0.0105(6) Uani 1 1 d . . . . .
O3 O 0.3893(2) 0.3646(3) 0.13296(14) 0.0105(6) Uani 1 1 d . . . . .
O4 O 0.1140(2) 0.1472(3) 0.86031(14) 0.0110(6) Uani 1 1 d . . . . .
O5 O 0.6452(2) 0.4262(3) 0.81890(14) 0.0146(7) Uani 1 1 d . . . . .
O6 O 0.1826(2) 0.9606(3) 0.92221(13) 0.0131(6) Uani 1 1 d . . . . .
O7 O 0.4773(3) 0.4732(4) 0.22429(16) 0.0313(10) Uani 1 1 d . . . . .
O8 O 0.3488(3) 0.5824(4) 0.1651(2) 0.0297(10) Uani 1 1 d . . . . .
O9 O 0.0509(2) 0.5586(3) 0.94200(13) 0.0078(5) Uani 1 1 d . . . . .
O10 O 0.95251(19) 0.4458(3) 0.05341(13) 0.0080(5) Uani 1 1 d . . . . .
O11 O 0.1263(2) 0.4060(3) 0.89316(14) 0.0113(6) Uani 1 1 d . . . . .
O12 O 0.8824(2) 0.5997(3) 0.10541(14) 0.0110(6) Uani 1 1 d . . . . .
O13 O 0.1288(2) 0.6612(3) 0.88252(14) 0.0112(6) Uani 1 1 d . . . . .
O14 O 0.3747(2) 0.8468(3) 0.11179(13) 0.0100(6) Uani 1 1 d . . . . .
O15 O 0.2119(2) 0.5599(4) 0.97063(14) 0.0141(6) Uani 1 1 d . . . . .
O16 O 0.2923(2) 0.9669(3) 0.02541(14) 0.0108(6) Uani 1 1 d . . . . .
O17 O 0.0849(2) 0.1664(3) 0.07187(14) 0.0123(6) Uani 1 1 d . . . . .
O18 O 0.4181(2) 0.3335(3) 0.92143(14) 0.0095(6) Uani 1 1 d . . . . .
O19 O 0.0989(2) 0.3975(3) 0.03522(13) 0.0091(6) Uani 1 1 d . . . . .
O20 O 0.90897(19) 0.6075(3) 0.96329(13) 0.0075(5) Uani 1 1 d . . . . .
O21 O 0.1116(2) 0.1916(3) 0.97755(14) 0.0128(6) Uani 1 1 d . . . . .
O22 O 0.4003(2) 0.3166(3) 1.01864(13) 0.0112(6) Uani 1 1 d . . . . .
O23 O 0.2248(2) 0.2470(3) 0.06207(15) 0.0135(7) Uani 1 1 d . . . . .
O24 O 0.2819(2) 0.2484(3) 0.93595(14) 0.0115(6) Uani 1 1 d . . . . .
O25 O 0.0528(2) 0.6420(3) 0.04699(13) 0.0081(6) Uani 1 1 d . . . . .
O26 O 0.9564(2) 0.3560(3) 0.95192(13) 0.0070(5) Uani 1 1 d . . . . .
O27 O 0.0745(2) 0.8701(3) 0.07879(13) 0.0102(6) Uani 1 1 d . . . . .
O28 O 0.9378(2) 0.1291(3) 0.91995(14) 0.0094(6) Uani 1 1 d . . . . .
O29 O 0.0971(2) 0.8141(3) 0.98479(13) 0.0106(6) Uani 1 1 d . . . . .
O30 O 0.9052(2) 0.1836(3) 1.01178(14) 0.0128(6) Uani 1 1 d . . . . .
O31 O 0.2019(2) 0.7353(4) 0.07080(14) 0.0123(6) Uani 1 1 d . . . . .
O32 O 0.8096(2) 0.2666(3) 0.92154(15) 0.0132(6) Uani 1 1 d . . . . .
O33 O 0.9527(2) 0.3219(4) 0.82734(14) 0.0145(7) Uani 1 1 d . . . . .
O34 O 0.0505(2) 0.6792(3) 0.16745(13) 0.0117(6) Uani 1 1 d . . . . .
O35 O 0.8683(2) 0.6791(4) 0.22681(14) 0.0159(7) Uani 1 1 d . . . . .
O36 O 0.1381(2) 0.6721(4) 0.26732(14) 0.0157(7) Uani 1 1 d . . . . .
O37 O 0.8621(3) 0.1233(4) 0.78913(16) 0.0228(8) Uani 1 1 d . . . . .
O38 O 0.1363(2) 0.8793(3) 0.20893(15) 0.0162(7) Uani 1 1 d . . . . .
O39 O 0.7967(2) 0.3383(4) 0.80454(15) 0.0155(7) Uani 1 1 d . . . . .
O40 O 0.2055(2) 0.6687(4) 0.18801(15) 0.0156(7) Uani 1 1 d . . . . .
O41 O 0.9456(2) 0.6661(4) 0.82875(15) 0.0159(7) Uani 1 1 d . . . . .
O42 O 0.0599(2) 0.3371(3) 0.16176(14) 0.0125(6) Uani 1 1 d . . . . .
O43 O 0.8481(3) 0.3492(5) 0.23286(17) 0.0396(14) Uani 1 1 d . . . . .
O44 O 0.1450(3) 0.3426(4) 0.26156(15) 0.0268(10) Uani 1 1 d . . . . .
O45 O 0.8525(2) 0.8585(3) 0.79108(15) 0.0138(7) Uani 1 1 d . . . . .
O46 O 0.1531(2) 0.1436(3) 0.20252(14) 0.0139(7) Uani 1 1 d . . . . .
O47 O 0.7882(2) 0.6482(4) 0.81551(18) 0.0230(8) Uani 1 1 d . . . . .
O48 O 0.2159(2) 0.3596(4) 0.18281(17) 0.0209(8) Uani 1 1 d . . . . .
O49 O 0.2352(2) 0.9957(4) 0.13510(17) 0.0190(8) Uani 1 1 d . . . . .
O50 O 0.2727(2) 0.5013(3) 0.86372(15) 0.0116(6) Uani 1 1 d . . . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
K1 O35 2.693(4) . ?
K1 O36 2.760(4) 1_655 ?
K1 O34 2.850(4) 1_655 ?
K1 O44 2.873(4) 1_655 ?
K1 O43 2.908(5) . ?
K1 O33 2.919(4) 2_564 ?
K1 O41 3.031(4) 2_564 ?
K1 O42 3.039(4) 1_655 ?
K1 Na5 3.350(3) 2_664 ?
K1 P9 3.377(2) 2_564 ?
K1 P10 3.378(2) 1_655 ?
K1 P12 3.560(2) 1_655 ?
Na1 O28 2.349(4) 1_465 ?
Na1 O27 2.378(4) 1_556 ?
Na1 O29 2.482(4) . ?
Na1 O30 2.561(5) 1_465 ?
Na1 O17 2.569(5) 1_566 ?
Na1 O18 2.619(4) 3_455 ?
Na1 O22 2.639(5) 3_455 ?
Na1 O21 2.778(5) 1_565 ?
Na1 P8 2.947(3) 1_465 ?
Na1 P7 2.953(3) 1_556 ?
Na1 P6 3.190(3) 3_455 ?
Na1 P5 3.268(3) 1_566 ?
Na2 O26 2.358(4) . ?
Na2 O20 2.359(4) . ?
Na2 O47 2.407(5) . ?
Na2 O39 2.417(5) . ?
Na2 O33 2.624(5) . ?
Na2 O41 2.628(5) . ?
Na2 O32 2.792(5) . ?
Na2 O9 3.011(5) 1_655 ?
Na2 P11 3.024(3) . ?
Na2 P9 3.090(3) . ?
Na2 P8 3.110(3) . ?
Na2 Al1 3.153(3) 1_655 ?
Na3 O15 2.232(4) 1_554 ?
Na3 O22 2.369(4) 1_554 ?
Na3 O23 2.424(4) . ?
Na3 O3 2.486(4) . ?
Na3 P2 3.132(3) . ?
Na3 O30 3.215(4) 3_454 ?
Na3 O8 3.217(5) . ?
Na3 O19 3.235(4) . ?
Na3 O24 3.244(4) 1_554 ?
Na3 P5 3.333(3) . ?
Na3 P6 3.365(3) 1_554 ?
Na3 O1 3.440(4) . ?
Na3 O31 3.449(4) . ?
Na3 Fe8 3.462(2) 3_445 ?
Na3 P3 3.526(2) 1_554 ?
Na4 O25 2.278(4) . ?
Na4 O19 2.341(4) . ?
Na4 O42 2.383(4) . ?
Na4 O48 2.405(4) . ?
Na4 O40 2.426(4) . ?
Na4 O34 2.502(4) . ?
Na4 O10 2.910(4) 1_455 ?
Na4 P12 2.914(3) . ?
Na4 P10 3.021(2) . ?
Na4 O31 3.039(4) . ?
Na4 Al1 3.117(3) 1_554 ?
Na4 P7 3.123(2) . ?
Na5 O5 2.325(5) 3_455 ?
Na5 O7 2.406(5) 4_465 ?
Na5 O2 2.616(4) 1_455 ?
Na5 O41 2.631(5) 1_455 ?
Na5 O44 2.659(6) 2_565 ?
Na5 O45 3.001(5) 1_455 ?
Na5 P1 3.019(3) . ?
Na5 P11 3.091(3) 1_455 ?
Na5 P12 3.164(3) 2_565 ?
Na5 Fe6 3.256(3) . ?
Na5 P2 3.334(3) 4_465 ?
Mn O32 2.174(4) 3_455 ?
Mn O6 2.242(3) . ?
Mn O16 2.244(3) 1_556 ?
Mn O29 2.269(4) . ?
Mn O15 2.291(4) . ?
Mn O31 2.495(4) 1_556 ?
Mn P7 2.9332(14) 1_556 ?
Mn O30 2.963(4) 3_455 ?
Mn Fe1 3.3254(9) 1_565 ?
Mn Fe13 3.4814(10) 2_565 ?
Fe1 O24 2.003(3) . ?
Fe1 O16 2.048(3) 1_546 ?
Fe1 O6 2.056(3) 1_545 ?
Fe1 O21 2.064(4) . ?
Fe1 O23 2.501(4) 1_556 ?
Fe1 P5 2.8559(13) 1_556 ?
Fe1 O4 2.964(4) . ?
Fe1 P6 2.9676(13) . ?
Fe1 P1 3.0645(13) 1_545 ?
Fe1 O20 3.105(3) 3_445 ?
Fe1 P4 3.2772(13) 3_446 ?
Fe1 O22 3.415(4) . ?
Fe1 O12 3.507(3) 3_446 ?
Fe1 Fe9 3.5282(9) . ?
Fe1 Fe10 3.5784(9) . ?
Fe2 O45 2.070(3) 4_464 ?
Fe2 O48 2.081(4) . ?
Fe2 O37 2.134(4) 4_454 ?
Fe2 O40 2.151(4) . ?
Fe2 O8 2.172(4) . ?
Fe2 P2 3.0814(13) . ?
Fe2 O7 3.160(5) . ?
Fe2 P12 3.1877(15) . ?
Fe2 Fe5 3.1938(11) 4_464 ?
Fe2 O44 3.215(5) . ?
Fe2 P11 3.2840(14) 4_464 ?
Fe2 P10 3.2979(14) . ?
Fe2 O36 3.328(4) . ?
Fe2 P9 3.3383(14) 4_454 ?
Fe2 Fe12 3.3461(10) . ?
Fe3 O38 2.074(3) 4_565 ?
Fe3 O5 2.076(3) . ?
Fe3 O39 2.109(4) . ?
Fe3 O46 2.121(3) 4 ?
Fe3 O47 2.137(4) . ?
Fe3 O43 2.998(6) 2_565 ?
Fe3 P11 3.1214(15) . ?
Fe3 Fe4 3.1631(11) 4_565 ?
Fe3 P10 3.2817(14) 4_565 ?
Fe3 P1 3.3017(12) 3_545 ?
Fe3 P9 3.3099(14) . ?
Fe3 O49 3.331(4) 4_565 ?
Fe3 P12 3.3511(14) 4 ?
Fe3 O35 3.419(4) 2_565 ?
Fe3 Fe13 3.4319(10) 4 ?
Fe4 O27 2.017(3) . ?
Fe4 O46 2.033(3) 1_565 ?
Fe4 O49 2.050(4) . ?
Fe4 O17 2.168(3) 1_565 ?
Fe4 O38 2.181(4) . ?
Fe4 O1 2.201(3) 3_455 ?
Fe4 Fe11 3.5416(12) 1_565 ?
Fe4 O31 3.747(4) . ?
Fe4 O30 4.284(4) 1_464 ?
Fe5 O28 2.057(3) 1_565 ?
Fe5 O45 2.068(3) . ?
Fe5 O50 2.090(4) 3 ?
Fe5 O37 2.117(4) 1_565 ?
Fe5 O18 2.169(3) 3 ?
Fe5 O2 2.211(3) . ?
Fe5 Fe13 3.5046(12) 4_565 ?
Fe5 O30 4.234(3) 1_565 ?
Fe6 O41 2.052(4) 1_455 ?
Fe6 O18 2.088(3) 3_455 ?
Fe6 O2 2.098(3) 1_455 ?
Fe6 O13 2.143(3) . ?
Fe6 O9 2.182(3) . ?
Fe6 O29 2.203(3) . ?
Fe6 P3 2.7599(14) . ?
Fe6 Fe13 4.0331(10) 2_565 ?
Fe7 O42 2.062(3) 1_655 ?
Fe7 O1 2.079(4) 3_545 ?
Fe7 O14 2.127(3) 3_545 ?
Fe7 O30 2.135(3) 1_554 ?
Fe7 O17 2.145(3) 1_655 ?
Fe7 O10 2.211(3) . ?
Fe7 P4 2.7692(13) . ?
Fe7 O31 4.439(3) 3_545 ?
Fe8 O34 2.011(3) 1_655 ?
Fe8 O22 2.062(3) 3_554 ?
Fe8 O12 2.121(3) . ?
Fe8 O3 2.151(3) 3 ?
Fe8 O27 2.264(3) 1_655 ?
Fe8 O25 2.322(3) 1_655 ?
Fe8 Fe11 3.4122(10) 3 ?
Fe8 O31 4.060(3) 1_655 ?
Fe9 O33 2.001(3) 1_455 ?
Fe9 O4 2.122(3) . ?
Fe9 O11 2.122(3) . ?
Fe9 O21 2.127(3) . ?
Fe9 O28 2.261(3) 1_455 ?
Fe9 O26 2.309(3) 1_455 ?
Fe9 O30 4.045(3) 1_455 ?
Fe10 O36 2.044(3) 2_565 ?
Fe10 O11 2.167(3) . ?
Fe10 O50 2.227(3) . ?
Fe10 O24 2.227(3) . ?
Fe10 O4 2.273(3) . ?
Fe10 O47 2.380(4) 3_445 ?
Fe10 Fe13 3.9973(10) 2_565 ?
Fe11 O35 2.026(4) 3_445 ?
Fe11 O23 2.139(3) . ?
Fe11 O12 2.164(3) 3_445 ?
Fe11 O49 2.277(4) 1_545 ?
Fe11 O3 2.319(3) . ?
Fe11 O48 2.440(4) . ?
Fe11 O46 3.140(4) . ?
Fe11 P5 3.3311(14) . ?
Fe11 P9 3.3408(13) 4_454 ?
Fe11 P4 3.3499(13) 3_445 ?
Fe11 P12 3.3815(14) . ?
Fe11 O17 3.513(4) . ?
Fe11 P2 3.5729(13) . ?
Fe12 O43 2.079(4) 3_455 ?
Fe12 O14 2.080(3) . ?
Fe12 O40 2.145(4) . ?
Fe12 O31 2.151(3) . ?
Fe12 O49 2.229(4) . ?
Fe12 O8 2.311(4) . ?
Fe12 O30 4.552(3) 3_454 ?
Fe13 O44 2.059(4) . ?
Fe13 O13 2.139(3) 2_564 ?
Fe13 O39 2.170(4) 4_454 ?
Fe13 O50 2.193(3) 2_564 ?
Fe13 O32 2.217(3) 4_454 ?
Fe13 O5 2.575(4) 4_454 ?
Fe13 O37 3.010(5) 4_454 ?
Fe13 P9 3.1747(13) 4_454 ?
Fe13 P3 3.2689(13) 2_564 ?
Fe13 P12 3.2822(13) . ?
Fe13 P8 3.4504(14) 4_454 ?
Fe13 O6 3.466(3) 2_564 ?
Al1 O9 1.858(3) . ?
Al1 O10 1.870(3) 1_456 ?
Al1 O26 1.884(3) 1_455 ?
Al1 O25 1.888(3) 1_556 ?
Al1 O20 1.895(3) 1_455 ?
Al1 O19 1.900(4) 1_556 ?
Al1 O30 3.637(4) 1_455 ?
Al1 O31 4.032(4) 1_556 ?
P1 O5 1.532(3) 3_455 ?
P1 O6 1.535(3) . ?
P1 O4 1.537(3) 1_565 ?
P1 O2 1.551(3) 1_455 ?
P2 O8 1.498(4) . ?
P2 O3 1.521(3) . ?
P2 O1 1.523(3) . ?
P2 O7 1.601(4) . ?
P2 O30 4.068(3) 3_454 ?
P2 O31 4.403(4) . ?
P3 O15 1.517(3) . ?
P3 O11 1.524(3) . ?
P3 O13 1.558(3) . ?
P3 O9 1.560(3) . ?
P3 O31 4.017(4) 1_556 ?
P4 O12 1.510(3) . ?
P4 O14 1.529(3) 3_545 ?
P4 O16 1.541(3) 3_545 ?
P4 O10 1.545(3) . ?
P4 O30 3.357(4) 1_554 ?
P4 O31 3.663(4) 3_545 ?
P5 O17 1.528(3) . ?
P5 O23 1.531(4) . ?
P5 O19 1.533(3) . ?
P5 O21 1.557(3) 1_554 ?
P5 O30 3.649(4) 1_454 ?
P6 O22 1.525(3) . ?
P6 O20 1.528(3) 3_445 ?
P6 O18 1.532(3) . ?
P6 O24 1.553(4) . ?
P6 O30 4.503(4) 3_455 ?
P7 O31 1.522(3) . ?
P7 O29 1.534(3) 1_554 ?
P7 O27 1.540(3) . ?
P7 O25 1.551(3) . ?
P8 O30 1.521(3) . ?
P8 O32 1.528(4) . ?
P8 O28 1.536(3) . ?
P8 O26 1.553(3) . ?
P9 O35 1.516(4) 2_565 ?
P9 O33 1.526(4) . ?
P9 O37 1.542(4) . ?
P9 O39 1.553(4) . ?
P10 O36 1.509(3) . ?
P10 O34 1.528(3) . ?
P10 O38 1.548(4) . ?
P10 O40 1.549(4) . ?
P10 O31 3.883(4) . ?
P11 O43 1.500(4) 2_565 ?
P11 O41 1.534(4) . ?
P11 O45 1.542(3) . ?
P11 O47 1.557(4) . ?
P12 O44 1.520(4) . ?
P12 O42 1.522(4) . ?
P12 O46 1.532(4) . ?
P12 O48 1.558(4) . ?
O1 O30 3.109(5) 3_454 ?
O8 O31 3.250(6) . ?
O9 O31 3.887(5) 1_556 ?
O10 O30 2.855(5) 1_554 ?
O14 O31 2.975(5) . ?
O14 O30 3.112(5) 3_454 ?
O15 O31 3.072(5) 1_556 ?
O15 O30 3.318(5) 3_455 ?
O16 O31 3.131(5) . ?
O16 O30 3.469(5) 3_454 ?
O17 O30 2.939(5) 1_454 ?
O19 O30 3.767(5) 1_454 ?
O19 O31 3.789(5) . ?
O21 O30 3.734(5) 1_455 ?
O22 O30 3.691(5) 3_455 ?
O25 O31 2.552(5) . ?
O26 O30 2.563(4) . ?
O27 O31 2.557(5) . ?
O28 O30 2.524(5) . ?
O29 O31 2.471(5) 1_556 ?
O30 O32 2.492(5) . ?
O31 O40 2.948(5) . ?
O31 O49 3.028(5) . ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O35 K1 O36 103.97(10) . 1_655 ?
O35 K1 O34 83.43(11) . 1_655 ?
O36 K1 O34 52.68(10) 1_655 1_655 ?
O35 K1 O44 175.86(15) . 1_655 ?
O36 K1 O44 72.07(14) 1_655 1_655 ?
O34 K1 O44 93.08(13) 1_655 1_655 ?
O35 K1 O43 73.03(16) . . ?
O36 K1 O43 172.74(16) 1_655 . ?
O34 K1 O43 132.25(14) 1_655 . ?
O44 K1 O43 111.05(13) 1_655 . ?
O35 K1 O33 52.41(10) . 2_564 ?
O36 K1 O33 82.60(12) 1_655 2_564 ?
O34 K1 O33 107.34(9) 1_655 2_564 ?
O44 K1 O33 127.14(13) 1_655 2_564 ?
O43 K1 O33 90.43(14) . 2_564 ?
O35 K1 O41 96.17(12) . 2_564 ?
O36 K1 O41 125.77(13) 1_655 2_564 ?
O34 K1 O41 178.11(13) 1_655 2_564 ?
O44 K1 O41 87.25(13) 1_655 2_564 ?
O43 K1 O41 49.16(10) . 2_564 ?
O33 K1 O41 71.04(12) 2_564 2_564 ?
O35 K1 O42 130.78(13) . 1_655 ?
O36 K1 O42 93.59(12) 1_655 1_655 ?
O34 K1 O42 71.47(11) 1_655 1_655 ?
O44 K1 O42 49.42(10) 1_655 1_655 ?
O43 K1 O42 93.31(14) . 1_655 ?
O33 K1 O42 175.76(13) 2_564 1_655 ?
O41 K1 O42 110.07(9) 2_564 1_655 ?
O35 K1 Na5 134.26(12) . 2_664 ?
O36 K1 Na5 119.85(12) 1_655 2_664 ?
O34 K1 Na5 132.93(11) 1_655 2_664 ?
O44 K1 Na5 49.88(11) 1_655 2_664 ?
O43 K1 Na5 61.87(12) . 2_664 ?
O33 K1 Na5 118.03(11) 2_564 2_664 ?
O41 K1 Na5 48.39(9) 2_564 2_664 ?
O42 K1 Na5 62.35(9) 1_655 2_664 ?
O35 K1 P9 25.92(8) . 2_564 ?
O36 K1 P9 96.47(10) 1_655 2_564 ?
O34 K1 P9 98.27(8) 1_655 2_564 ?
O44 K1 P9 153.93(12) 1_655 2_564 ?
O43 K1 P9 77.95(13) . 2_564 ?
O33 K1 P9 26.80(7) 2_564 2_564 ?
O41 K1 P9 80.69(9) 2_564 2_564 ?
O42 K1 P9 156.63(11) 1_655 2_564 ?
Na5 K1 P9 127.96(8) 2_664 2_564 ?
O35 K1 P10 95.80(9) . 1_655 ?
O36 K1 P10 26.07(7) 1_655 1_655 ?
O34 K1 P10 26.72(7) 1_655 1_655 ?
O44 K1 P10 80.11(11) 1_655 1_655 ?
O43 K1 P10 158.90(12) . 1_655 ?
O33 K1 P10 96.79(9) 2_564 1_655 ?
O41 K1 P10 151.79(11) 2_564 1_655 ?
O42 K1 P10 80.38(8) 1_655 1_655 ?
Na5 K1 P10 129.35(8) 2_664 1_655 ?
P9 K1 P10 99.96(4) 2_564 1_655 ?
O35 K1 P12 155.15(12) . 1_655 ?
O36 K1 P12 80.17(10) 1_655 1_655 ?
O34 K1 P12 79.86(9) 1_655 1_655 ?
O44 K1 P12 24.48(7) 1_655 1_655 ?
O43 K1 P12 105.39(13) . 1_655 ?
O33 K1 P12 151.20(11) 2_564 1_655 ?
O41 K1 P12 101.10(9) 2_564 1_655 ?
O42 K1 P12 25.11(7) 1_655 1_655 ?
Na5 K1 P12 54.40(6) 2_664 1_655 ?
P9 K1 P12 176.63(7) 2_564 1_655 ?
P10 K1 P12 77.09(5) 1_655 1_655 ?
O28 Na1 O27 178.2(2) 1_465 1_556 ?
O28 Na1 O29 118.20(17) 1_465 . ?
O27 Na1 O29 62.08(12) 1_556 . ?
O28 Na1 O30 61.70(12) 1_465 1_465 ?
O27 Na1 O30 118.06(17) 1_556 1_465 ?
O29 Na1 O30 178.70(19) . 1_465 ?
O28 Na1 O17 104.17(14) 1_465 1_566 ?
O27 Na1 O17 74.18(14) 1_556 1_566 ?
O29 Na1 O17 111.26(16) . 1_566 ?
O30 Na1 O17 69.91(13) 1_465 1_566 ?
O28 Na1 O18 73.69(14) 1_465 3_455 ?
O27 Na1 O18 107.97(13) 1_556 3_455 ?
O29 Na1 O18 70.61(13) . 3_455 ?
O30 Na1 O18 108.23(15) 1_465 3_455 ?
O17 Na1 O18 177.75(17) 1_566 3_455 ?
O28 Na1 O22 111.18(16) 1_465 3_455 ?
O27 Na1 O22 70.56(13) 1_556 3_455 ?
O29 Na1 O22 88.42(13) . 3_455 ?
O30 Na1 O22 90.43(15) 1_465 3_455 ?
O17 Na1 O22 124.13(16) 1_566 3_455 ?
O18 Na1 O22 56.69(11) 3_455 3_455 ?
O28 Na1 O21 68.43(13) 1_465 1_565 ?
O27 Na1 O21 109.82(16) 1_556 1_565 ?
O29 Na1 O21 92.50(15) . 1_565 ?
O30 Na1 O21 88.65(13) 1_465 1_565 ?
O17 Na1 O21 55.42(11) 1_566 1_565 ?
O18 Na1 O21 123.72(15) 3_455 1_565 ?
O22 Na1 O21 179.07(18) 3_455 1_565 ?
O28 Na1 P8 31.20(9) 1_465 1_465 ?
O27 Na1 P8 148.27(15) 1_556 1_465 ?
O29 Na1 P8 149.03(15) . 1_465 ?
O30 Na1 P8 31.06(8) 1_465 1_465 ?
O17 Na1 P8 83.10(10) 1_566 1_465 ?
O18 Na1 P8 94.67(12) 3_455 1_465 ?
O22 Na1 P8 106.45(13) 3_455 1_465 ?
O21 Na1 P8 72.76(10) 1_565 1_465 ?
O28 Na1 P7 149.22(16) 1_465 1_556 ?
O27 Na1 P7 31.28(9) 1_556 1_556 ?
O29 Na1 P7 31.30(8) . 1_556 ?
O30 Na1 P7 148.65(15) 1_465 1_556 ?
O17 Na1 P7 96.28(12) 1_566 1_556 ?
O18 Na1 P7 85.96(10) 3_455 1_556 ?
O22 Na1 P7 73.89(10) 3_455 1_556 ?
O21 Na1 P7 106.89(13) 1_565 1_556 ?
P8 Na1 P7 179.37(13) 1_465 1_556 ?
O28 Na1 P6 94.24(13) 1_465 3_455 ?
O27 Na1 P6 87.58(11) 1_556 3_455 ?
O29 Na1 P6 76.20(10) . 3_455 ?
O30 Na1 P6 102.50(13) 1_465 3_455 ?
O17 Na1 P6 152.47(15) 1_566 3_455 ?
O18 Na1 P6 28.47(8) 3_455 3_455 ?
O22 Na1 P6 28.37(8) 3_455 3_455 ?
O21 Na1 P6 152.10(14) 1_565 3_455 ?
P8 Na1 P6 104.07(10) 1_465 3_455 ?
P7 Na1 P6 76.49(6) 1_556 3_455 ?
O28 Na1 P5 85.34(11) 1_465 1_566 ?
O27 Na1 P5 92.84(12) 1_556 1_566 ?
O29 Na1 P5 104.86(13) . 1_566 ?
O30 Na1 P5 76.44(10) 1_465 1_566 ?
O17 Na1 P5 27.11(8) 1_566 1_566 ?
O18 Na1 P5 151.87(14) 3_455 1_566 ?
O22 Na1 P5 151.12(14) 3_455 1_566 ?
O21 Na1 P5 28.38(7) 1_565 1_566 ?
P8 Na1 P5 75.08(6) 1_465 1_566 ?
P7 Na1 P5 104.36(9) 1_556 1_566 ?
P6 Na1 P5 178.94(11) 3_455 1_566 ?
O26 Na2 O20 69.29(13) . . ?
O26 Na2 O47 169.63(18) . . ?
O20 Na2 O47 100.45(16) . . ?
O26 Na2 O39 108.06(15) . . ?
O20 Na2 O39 159.1(2) . . ?
O47 Na2 O39 80.91(16) . . ?
O26 Na2 O33 75.91(14) . . ?
O20 Na2 O33 135.49(19) . . ?
O47 Na2 O33 113.84(17) . . ?
O39 Na2 O33 59.04(13) . . ?
O26 Na2 O41 119.8(2) . . ?
O20 Na2 O41 91.46(15) . . ?
O47 Na2 O41 60.36(14) . . ?
O39 Na2 O41 106.92(16) . . ?
O33 Na2 O41 82.37(16) . . ?
O26 Na2 O32 57.45(12) . . ?
O20 Na2 O32 95.19(15) . . ?
O47 Na2 O32 124.1(2) . . ?
O39 Na2 O32 67.79(13) . . ?
O33 Na2 O32 88.52(13) . . ?
O41 Na2 O32 170.90(17) . . ?
O26 Na2 O9 56.77(12) . 1_655 ?
O20 Na2 O9 56.02(12) . 1_655 ?
O47 Na2 O9 119.34(16) . 1_655 ?
O39 Na2 O9 141.02(18) . 1_655 ?
O33 Na2 O9 81.98(15) . 1_655 ?
O41 Na2 O9 65.11(13) . 1_655 ?
O32 Na2 O9 113.90(13) . 1_655 ?
O26 Na2 P11 150.29(19) . . ?
O20 Na2 P11 102.11(12) . . ?
O47 Na2 P11 30.73(10) . . ?
O39 Na2 P11 89.71(12) . . ?
O33 Na2 P11 94.47(13) . . ?
O41 Na2 P11 30.47(8) . . ?
O32 Na2 P11 151.67(15) . . ?
O9 Na2 P11 94.41(12) 1_655 . ?
O26 Na2 P9 94.24(11) . . ?
O20 Na2 P9 162.87(15) . . ?
O47 Na2 P9 96.10(13) . . ?
O39 Na2 P9 29.67(9) . . ?
O33 Na2 P9 29.57(8) . . ?
O41 Na2 P9 92.92(13) . . ?
O32 Na2 P9 78.94(10) . . ?
O9 Na2 P9 111.46(14) 1_655 . ?
P11 Na2 P9 89.90(9) . . ?
O26 Na2 P8 29.07(9) . . ?
O20 Na2 P8 86.27(11) . . ?
O47 Na2 P8 153.49(19) . . ?
O39 Na2 P8 83.98(12) . . ?
O33 Na2 P8 75.67(10) . . ?
O41 Na2 P8 145.71(17) . . ?
O32 Na2 P8 29.38(8) . . ?
O9 Na2 P8 85.76(10) 1_655 . ?
P11 Na2 P8 170.03(12) . . ?
P9 Na2 P8 80.79(6) . . ?
O26 Na2 Al1 36.50(9) . 1_655 ?
O20 Na2 Al1 36.78(9) . 1_655 ?
O47 Na2 Al1 134.31(14) . 1_655 ?
O39 Na2 Al1 144.56(13) . 1_655 ?
O33 Na2 Al1 100.08(13) . 1_655 ?
O41 Na2 Al1 97.07(14) . 1_655 ?
O32 Na2 Al1 84.66(10) . 1_655 ?
O9 Na2 Al1 34.99(7) 1_655 1_655 ?
P11 Na2 Al1 122.27(11) . 1_655 ?
P9 Na2 Al1 126.13(11) . 1_655 ?
P8 Na2 Al1 62.09(6) . 1_655 ?
O15 Na3 O22 114.93(15) 1_554 1_554 ?
O15 Na3 O23 110.91(15) 1_554 . ?
O22 Na3 O23 91.29(15) 1_554 . ?
O15 Na3 O3 167.80(16) 1_554 . ?
O22 Na3 O3 73.62(13) 1_554 . ?
O23 Na3 O3 76.45(13) . . ?
O15 Na3 P2 139.65(14) 1_554 . ?
O22 Na3 P2 88.39(11) 1_554 . ?
O23 Na3 P2 100.33(11) . . ?
O3 Na3 P2 28.57(8) . . ?
O15 Na3 O30 72.53(12) 1_554 3_454 ?
O22 Na3 O30 81.23(13) 1_554 3_454 ?
O23 Na3 O30 172.51(15) . 3_454 ?
O3 Na3 O30 101.38(12) . 3_454 ?
P2 Na3 O30 79.72(9) . 3_454 ?
O15 Na3 O8 118.48(15) 1_554 . ?
O22 Na3 O8 115.56(14) 1_554 . ?
O23 Na3 O8 100.73(13) . . ?
O3 Na3 O8 49.53(11) . . ?
P2 Na3 O8 27.25(8) . . ?
O30 Na3 O8 82.79(11) 3_454 . ?
O15 Na3 O19 69.16(12) 1_554 . ?
O22 Na3 O19 134.26(14) 1_554 . ?
O23 Na3 O19 50.19(11) . . ?
O3 Na3 O19 111.82(13) . . ?
P2 Na3 O19 118.41(9) . . ?
O30 Na3 O19 136.29(11) 3_454 . ?
O8 Na3 O19 97.45(11) . . ?
O15 Na3 O24 77.59(12) 1_554 1_554 ?
O22 Na3 O24 50.04(11) 1_554 1_554 ?
O23 Na3 O24 74.29(12) . 1_554 ?
O3 Na3 O24 114.27(12) . 1_554 ?
P2 Na3 O24 137.11(10) . 1_554 ?
O30 Na3 O24 100.49(10) 3_454 1_554 ?
O8 Na3 O24 163.63(12) . 1_554 ?
O19 Na3 O24 91.19(10) . 1_554 ?
O15 Na3 P5 87.13(11) 1_554 . ?
O22 Na3 P5 109.04(12) 1_554 . ?
O23 Na3 P5 25.02(8) . . ?
O3 Na3 P5 98.44(11) . . ?
P2 Na3 P5 117.20(7) . . ?
O30 Na3 P5 159.64(10) 3_454 . ?
O8 Na3 P5 107.01(10) . . ?
O19 Na3 P5 26.93(6) . . ?
O24 Na3 P5 75.24(8) 1_554 . ?
O15 Na3 P6 95.10(12) 1_554 1_554 ?
O22 Na3 P6 23.61(9) 1_554 1_554 ?
O23 Na3 P6 86.72(11) . 1_554 ?
O3 Na3 P6 95.03(10) . 1_554 ?
P2 Na3 P6 111.99(7) . 1_554 ?
O30 Na3 P6 86.33(9) 3_454 1_554 ?
O8 Na3 P6 139.15(11) . 1_554 ?
O19 Na3 P6 116.96(10) . 1_554 ?
O24 Na3 P6 27.11(6) 1_554 1_554 ?
P5 Na3 P6 96.56(7) . 1_554 ?
O15 Na3 O1 125.25(14) 1_554 . ?
O22 Na3 O1 75.71(12) 1_554 . ?
O23 Na3 O1 122.79(12) . . ?
O3 Na3 O1 46.35(10) . . ?
P2 Na3 O1 26.27(6) . . ?
O30 Na3 O1 55.57(9) 3_454 . ?
O8 Na3 O1 44.81(10) . . ?
O19 Na3 O1 142.18(11) . . ?
O24 Na3 O1 124.66(11) 1_554 . ?
P5 Na3 O1 142.96(9) . . ?
P6 Na3 O1 97.62(9) 1_554 . ?
O15 Na3 O31 61.11(12) 1_554 . ?
O22 Na3 O31 155.58(14) 1_554 . ?
O23 Na3 O31 112.85(13) . . ?
O3 Na3 O31 107.38(12) . . ?
P2 Na3 O31 83.83(8) . . ?
O30 Na3 O31 74.62(10) 3_454 . ?
O8 Na3 O31 58.23(10) . . ?
O19 Na3 O31 68.98(9) . . ?
O24 Na3 O31 138.14(11) 1_554 . ?
P5 Na3 O31 95.08(8) . . ?
P6 Na3 O31 152.88(10) 1_554 . ?
O1 Na3 O31 87.50(10) . . ?
O15 Na3 Fe8 150.11(13) 1_554 3_445 ?
O22 Na3 Fe8 35.55(8) 1_554 3_445 ?
O23 Na3 Fe8 80.94(10) . 3_445 ?
O3 Na3 Fe8 38.15(8) . 3_445 ?
P2 Na3 Fe8 57.56(4) . 3_445 ?
O30 Na3 Fe8 92.93(9) 3_454 3_445 ?
O8 Na3 Fe8 84.11(9) . 3_445 ?
O19 Na3 Fe8 130.71(10) . 3_445 ?
O24 Na3 Fe8 79.72(8) 1_554 3_445 ?
P5 Na3 Fe8 105.62(7) . 3_445 ?
P6 Na3 Fe8 57.21(4) 1_554 3_445 ?
O1 Na3 Fe8 56.36(7) . 3_445 ?
O31 Na3 Fe8 141.17(9) . 3_445 ?
O15 Na3 P3 16.19(9) 1_554 1_554 ?
O22 Na3 P3 112.68(11) 1_554 1_554 ?
O23 Na3 P3 95.32(11) . 1_554 ?
O3 Na3 P3 170.02(13) . 1_554 ?
P2 Na3 P3 153.46(9) . 1_554 ?
O30 Na3 P3 87.49(8) 3_454 1_554 ?
O8 Na3 P3 128.42(11) . 1_554 ?
O19 Na3 P3 58.20(7) . 1_554 ?
O24 Na3 P3 67.92(8) 1_554 1_554 ?
P5 Na3 P3 72.40(5) . 1_554 ?
P6 Na3 P3 90.05(6) 1_554 1_554 ?
O1 Na3 P3 141.37(10) . 1_554 ?
O31 Na3 P3 70.32(7) . 1_554 ?
Fe8 Na3 P3 147.11(8) 3_445 1_554 ?
O25 Na4 O19 68.82(13) . . ?
O25 Na4 O42 125.63(17) . . ?
O19 Na4 O42 92.24(14) . . ?
O25 Na4 O48 165.09(18) . . ?
O19 Na4 O48 100.15(15) . . ?
O42 Na4 O48 62.88(13) . . ?
O25 Na4 O40 103.77(14) . . ?
O19 Na4 O40 148.49(18) . . ?
O42 Na4 O40 114.96(15) . . ?
O48 Na4 O40 80.22(16) . . ?
O25 Na4 O34 77.62(13) . . ?
O19 Na4 O34 139.74(16) . . ?
O42 Na4 O34 89.60(15) . . ?
O48 Na4 O34 116.19(16) . . ?
O40 Na4 O34 60.29(12) . . ?
O25 Na4 O10 58.84(12) . 1_455 ?
O19 Na4 O10 58.79(11) . 1_455 ?
O42 Na4 O10 67.64(12) . 1_455 ?
O48 Na4 O10 124.95(14) . 1_455 ?
O40 Na4 O10 144.87(15) . 1_455 ?
O34 Na4 O10 85.21(13) . 1_455 ?
O25 Na4 P12 156.87(15) . . ?
O19 Na4 P12 102.49(11) . . ?
O42 Na4 P12 31.40(9) . . ?
O48 Na4 P12 32.29(10) . . ?
O40 Na4 P12 94.36(12) . . ?
O34 Na4 P12 99.75(11) . . ?
O10 Na4 P12 98.14(10) 1_455 . ?
O25 Na4 P10 94.85(11) . . ?
O19 Na4 P10 163.50(13) . . ?
O42 Na4 P10 99.63(12) . . ?
O48 Na4 P10 95.47(13) . . ?
O40 Na4 P10 30.63(9) . . ?
O34 Na4 P10 30.30(8) . . ?
O10 Na4 P10 115.49(11) 1_455 . ?
P12 Na4 P10 93.55(7) . . ?
O25 Na4 O31 55.15(11) . . ?
O19 Na4 O31 88.56(13) . . ?
O42 Na4 O31 179.07(15) . . ?
O48 Na4 O31 116.50(15) . . ?
O40 Na4 O31 64.14(12) . . ?
O34 Na4 O31 90.11(12) . . ?
O10 Na4 O31 113.21(11) 1_455 . ?
P12 Na4 O31 147.86(12) . . ?
P10 Na4 O31 79.68(9) . . ?
O25 Na4 Al1 37.01(9) . 1_554 ?
O19 Na4 Al1 37.44(9) . 1_554 ?
O42 Na4 Al1 99.10(12) . 1_554 ?
O48 Na4 Al1 135.88(13) . 1_554 ?
O40 Na4 Al1 140.45(13) . 1_554 ?
O34 Na4 Al1 102.65(11) . 1_554 ?
O10 Na4 Al1 35.95(7) 1_455 1_554 ?
P12 Na4 Al1 124.71(9) . 1_554 ?
P10 Na4 Al1 128.19(9) . 1_554 ?
O31 Na4 Al1 81.83(9) . 1_554 ?
O25 Na4 P7 28.22(9) . . ?
O19 Na4 P7 83.88(11) . . ?
O42 Na4 P7 152.05(14) . . ?
O48 Na4 P7 145.05(15) . . ?
O40 Na4 P7 78.96(11) . . ?
O34 Na4 P7 76.24(9) . . ?
O10 Na4 P7 87.00(9) 1_455 . ?
P12 Na4 P7 173.26(9) . . ?
P10 Na4 P7 80.26(6) . . ?
O31 Na4 P7 28.56(7) . . ?
Al1 Na4 P7 61.84(5) 1_554 . ?
O5 Na5 O7 87.03(17) 3_455 4_465 ?
O5 Na5 O2 60.47(12) 3_455 1_455 ?
O7 Na5 O2 87.32(15) 4_465 1_455 ?
O5 Na5 O41 118.76(16) 3_455 1_455 ?
O7 Na5 O41 129.38(19) 4_465 1_455 ?
O2 Na5 O41 72.71(13) 1_455 1_455 ?
O5 Na5 O44 75.00(15) 3_455 2_565 ?
O7 Na5 O44 128.90(18) 4_465 2_565 ?
O2 Na5 O44 120.91(15) 1_455 2_565 ?
O41 Na5 O44 100.75(15) 1_455 2_565 ?
O5 Na5 O45 125.67(15) 3_455 1_455 ?
O7 Na5 O45 77.55(16) 4_465 1_455 ?
O2 Na5 O45 66.97(12) 1_455 1_455 ?
O41 Na5 O45 51.87(11) 1_455 1_455 ?
O44 Na5 O45 150.18(15) 2_565 1_455 ?
O5 Na5 P1 29.86(9) 3_455 . ?
O7 Na5 P1 83.59(13) 4_465 . ?
O2 Na5 P1 30.91(8) 1_455 . ?
O41 Na5 P1 98.49(12) 1_455 . ?
O44 Na5 P1 100.04(13) 2_565 . ?
O45 Na5 P1 96.16(11) 1_455 . ?
O5 Na5 P11 140.73(14) 3_455 1_455 ?
O7 Na5 P11 103.27(16) 4_465 1_455 ?
O2 Na5 P11 81.97(11) 1_455 1_455 ?
O41 Na5 P11 29.74(8) 1_455 1_455 ?
O44 Na5 P11 120.95(13) 2_565 1_455 ?
O45 Na5 P11 29.28(7) 1_455 1_455 ?
P1 Na5 P11 112.72(10) . 1_455 ?
O5 Na5 P12 80.94(12) 3_455 2_565 ?
O7 Na5 P12 102.35(14) 4_465 2_565 ?
O2 Na5 P12 139.82(13) 1_455 2_565 ?
O41 Na5 P12 123.06(13) 1_455 2_565 ?
O44 Na5 P12 28.62(8) 2_565 2_565 ?
O45 Na5 P12 153.06(13) 1_455 2_565 ?
P1 Na5 P12 110.67(10) . 2_565 ?
P11 Na5 P12 131.36(10) 1_455 2_565 ?
O5 Na5 Fe6 80.62(12) 3_455 . ?
O7 Na5 Fe6 124.43(14) 4_465 . ?
O2 Na5 Fe6 40.02(8) 1_455 . ?
O41 Na5 Fe6 39.02(9) 1_455 . ?
O44 Na5 Fe6 99.64(12) 2_565 . ?
O45 Na5 Fe6 67.39(9) 1_455 . ?
P1 Na5 Fe6 60.09(6) . . ?
P11 Na5 Fe6 62.15(6) 1_455 . ?
P12 Na5 Fe6 128.19(10) 2_565 . ?
O5 Na5 P2 109.05(14) 3_455 4_465 ?
O7 Na5 P2 26.64(11) 4_465 4_465 ?
O2 Na5 P2 110.95(12) 1_455 4_465 ?
O41 Na5 P2 123.77(13) 1_455 4_465 ?
O44 Na5 P2 119.41(13) 2_565 4_465 ?
O45 Na5 P2 77.14(10) 1_455 4_465 ?
P1 Na5 P2 110.16(9) . 4_465 ?
P11 Na5 P2 94.03(9) 1_455 4_465 ?
P12 Na5 P2 90.87(8) 2_565 4_465 ?
Fe6 Na5 P2 140.93(11) . 4_465 ?
O32 Mn O6 80.94(12) 3_455 . ?
O32 Mn O16 97.70(13) 3_455 1_556 ?
O6 Mn O16 73.63(11) . 1_556 ?
O32 Mn O29 145.33(13) 3_455 . ?
O6 Mn O29 76.10(12) . . ?
O16 Mn O29 100.28(12) 1_556 . ?
O32 Mn O15 86.94(13) 3_455 . ?
O6 Mn O15 134.91(12) . . ?
O16 Mn O15 151.37(13) 1_556 . ?
O29 Mn O15 91.15(12) . . ?
O32 Mn O31 150.08(14) 3_455 1_556 ?
O6 Mn O31 126.89(12) . 1_556 ?
O16 Mn O31 82.53(12) 1_556 1_556 ?
O29 Mn O31 62.28(11) . 1_556 ?
O15 Mn O31 79.74(12) . 1_556 ?
O32 Mn P7 169.10(10) 3_455 1_556 ?
O6 Mn P7 102.96(9) . 1_556 ?
O16 Mn P7 93.17(9) 1_556 1_556 ?
O29 Mn P7 31.10(8) . 1_556 ?
O15 Mn P7 83.15(9) . 1_556 ?
O31 Mn P7 31.25(8) 1_556 1_556 ?
O32 Mn O30 55.49(11) 3_455 3_455 ?
O6 Mn O30 126.43(11) . 3_455 ?
O16 Mn O30 82.30(11) 1_556 3_455 ?
O29 Mn O30 156.45(12) . 3_455 ?
O15 Mn O30 77.15(11) . 3_455 ?
O31 Mn O30 95.22(10) 1_556 3_455 ?
P7 Mn O30 125.87(7) 1_556 3_455 ?
O32 Mn Fe1 94.89(10) 3_455 1_565 ?
O6 Mn Fe1 37.32(8) . 1_565 ?
O16 Mn Fe1 37.11(8) 1_556 1_565 ?
O29 Mn Fe1 82.31(8) . 1_565 ?
O15 Mn Fe1 170.98(9) . 1_565 ?
O31 Mn Fe1 102.45(8) 1_556 1_565 ?
P7 Mn Fe1 94.22(3) 1_556 1_565 ?
O30 Mn Fe1 111.14(7) 3_455 1_565 ?
O32 Mn Fe13 37.99(9) 3_455 2_565 ?
O6 Mn Fe13 70.82(8) . 2_565 ?
O16 Mn Fe13 126.03(9) 1_556 2_565 ?
O29 Mn Fe13 108.81(9) . 2_565 ?
O15 Mn Fe13 73.07(9) . 2_565 ?
O31 Mn Fe13 151.35(8) 1_556 2_565 ?
P7 Mn Fe13 133.39(4) 1_556 2_565 ?
O30 Mn Fe13 87.50(7) 3_455 2_565 ?
Fe1 Mn Fe13 103.10(3) 1_565 2_565 ?
O32 Mn Na3 92.07(10) 3_455 1_556 ?
O6 Mn Na3 166.76(9) . 1_556 ?
O16 Mn Na3 118.71(9) 1_556 1_556 ?
O29 Mn Na3 104.68(9) . 1_556 ?
O15 Mn Na3 32.66(9) . 1_556 ?
O31 Mn Na3 62.70(9) 1_556 1_556 ?
P7 Mn Na3 82.01(5) 1_556 1_556 ?
O30 Mn Na3 55.27(7) 3_455 1_556 ?
Fe1 Mn Na3 155.59(5) 1_565 1_556 ?
Fe13 Mn Na3 96.77(4) 2_565 1_556 ?
O24 Fe1 O16 122.89(14) . 1_546 ?
O24 Fe1 O6 108.55(14) . 1_545 ?
O16 Fe1 O6 81.86(12) 1_546 1_545 ?
O24 Fe1 O21 108.39(14) . . ?
O16 Fe1 O21 126.40(14) 1_546 . ?
O6 Fe1 O21 96.80(14) 1_545 . ?
O24 Fe1 O23 100.79(13) . 1_556 ?
O16 Fe1 O23 90.39(12) 1_546 1_556 ?
O6 Fe1 O23 149.12(12) 1_545 1_556 ?
O21 Fe1 O23 64.14(12) . 1_556 ?
O24 Fe1 P5 110.23(10) . 1_556 ?
O16 Fe1 P5 108.41(10) 1_546 1_556 ?
O6 Fe1 P5 123.46(10) 1_545 1_556 ?
O21 Fe1 P5 32.04(10) . 1_556 ?
O23 Fe1 P5 32.35(8) 1_556 1_556 ?
O24 Fe1 O4 73.27(12) . . ?
O16 Fe1 O4 137.53(12) 1_546 . ?
O6 Fe1 O4 55.88(11) 1_545 . ?
O21 Fe1 O4 68.69(11) . . ?
O23 Fe1 O4 127.51(10) 1_556 . ?
P5 Fe1 O4 99.31(7) 1_556 . ?
O24 Fe1 P6 28.92(10) . . ?
O16 Fe1 P6 95.06(10) 1_546 . ?
O6 Fe1 P6 115.70(10) 1_545 . ?
O21 Fe1 P6 131.09(11) . . ?
O23 Fe1 P6 94.67(8) 1_556 . ?
P5 Fe1 P6 118.30(4) 1_556 . ?
O4 Fe1 P6 99.43(7) . . ?
O24 Fe1 P1 93.99(10) . 1_545 ?
O16 Fe1 P1 108.48(10) 1_546 1_545 ?
O6 Fe1 P1 26.64(9) 1_545 1_545 ?
O21 Fe1 P1 80.45(10) . 1_545 ?
O23 Fe1 P1 144.34(8) 1_556 1_545 ?
P5 Fe1 P1 112.00(4) 1_556 1_545 ?
O4 Fe1 P1 29.49(7) . 1_545 ?
P6 Fe1 P1 112.80(4) . 1_545 ?
O24 Fe1 O20 52.56(11) . 3_445 ?
O16 Fe1 O20 70.88(11) 1_546 3_445 ?
O6 Fe1 O20 95.69(11) 1_545 3_445 ?
O21 Fe1 O20 160.02(12) . 3_445 ?
O23 Fe1 O20 109.98(10) 1_556 3_445 ?
P5 Fe1 O20 140.71(7) 1_556 3_445 ?
O4 Fe1 O20 106.33(9) . 3_445 ?
P6 Fe1 O20 29.04(6) . 3_445 ?
P1 Fe1 O20 104.81(6) 1_545 3_445 ?
O24 Fe1 P4 108.75(10) . 3_446 ?
O16 Fe1 P4 20.66(9) 1_546 3_446 ?
O6 Fe1 P4 101.00(9) 1_545 3_446 ?
O21 Fe1 P4 130.62(10) . 3_446 ?
O23 Fe1 P4 77.88(8) 1_556 3_446 ?
P5 Fe1 P4 103.58(4) 1_556 3_446 ?
O4 Fe1 P4 154.33(7) . 3_446 ?
P6 Fe1 P4 79.83(3) . 3_446 ?
P1 Fe1 P4 127.46(3) 1_545 3_446 ?
O20 Fe1 P4 61.39(6) 3_445 3_446 ?
O24 Fe1 Mn 131.40(10) . 1_545 ?
O16 Fe1 Mn 41.40(9) 1_546 1_545 ?
O6 Fe1 Mn 41.39(9) 1_545 1_545 ?
O21 Fe1 Mn 111.85(10) . 1_545 ?
O23 Fe1 Mn 120.60(8) 1_556 1_545 ?
P5 Fe1 Mn 118.36(3) 1_556 1_545 ?
O4 Fe1 Mn 97.09(7) . 1_545 ?
P6 Fe1 Mn 116.74(3) . 1_545 ?
P1 Fe1 Mn 67.62(3) 1_545 1_545 ?
O20 Fe1 Mn 87.76(6) 3_445 1_545 ?
P4 Fe1 Mn 61.74(3) 3_446 1_545 ?
O24 Fe1 O22 46.54(11) . . ?
O16 Fe1 O22 89.40(11) 1_546 . ?
O6 Fe1 O22 140.33(11) 1_545 . ?
O21 Fe1 O22 118.90(13) . . ?
O23 Fe1 O22 68.83(10) 1_556 . ?
P5 Fe1 O22 96.05(6) 1_556 . ?
O4 Fe1 O22 119.45(9) . . ?
P6 Fe1 O22 26.47(6) . . ?
P1 Fe1 O22 138.63(6) 1_545 . ?
O20 Fe1 O22 45.33(8) 3_445 . ?
P4 Fe1 O22 69.65(6) 3_446 . ?
Mn Fe1 O22 124.99(6) 1_545 . ?
O24 Fe1 O12 99.40(11) . 3_446 ?
O16 Fe1 O12 44.64(11) 1_546 3_446 ?
O6 Fe1 O12 126.28(11) 1_545 3_446 ?
O21 Fe1 O12 116.80(11) . 3_446 ?
O23 Fe1 O12 55.38(9) 1_556 3_446 ?
P5 Fe1 O12 85.37(6) 1_556 3_446 ?
O4 Fe1 O12 172.28(9) . 3_446 ?
P6 Fe1 O12 72.90(6) . 3_446 ?
P1 Fe1 O12 152.85(6) 1_545 3_446 ?
O20 Fe1 O12 66.60(7) 3_445 3_446 ?
P4 Fe1 O12 25.44(6) 3_446 3_446 ?
Mn Fe1 O12 85.94(6) 1_545 3_446 ?
O22 Fe1 O12 53.59(8) . 3_446 ?
O24 Fe1 Fe9 85.66(10) . . ?
O16 Fe1 Fe9 150.42(10) 1_546 . ?
O6 Fe1 Fe9 81.47(9) 1_545 . ?
O21 Fe1 Fe9 33.22(9) . . ?
O23 Fe1 Fe9 91.51(8) 1_556 . ?
P5 Fe1 Fe9 62.47(3) 1_556 . ?
O4 Fe1 Fe9 36.88(6) . . ?
P6 Fe1 Fe9 114.18(3) . . ?
P1 Fe1 Fe9 57.23(2) 1_545 . ?
O20 Fe1 Fe9 135.08(6) 3_445 . ?
P4 Fe1 Fe9 163.35(3) 3_446 . ?
Mn Fe1 Fe9 115.16(3) 1_545 . ?
O22 Fe1 Fe9 118.69(6) . . ?
O12 Fe1 Fe9 146.90(6) 3_446 . ?
O24 Fe1 Fe10 34.20(10) . . ?
O16 Fe1 Fe10 144.83(10) 1_546 . ?
O6 Fe1 Fe10 85.05(9) 1_545 . ?
O21 Fe1 Fe10 87.43(10) . . ?
O23 Fe1 Fe10 116.14(8) 1_556 . ?
P5 Fe1 Fe10 106.06(3) 1_556 . ?
O4 Fe1 Fe10 39.26(6) . . ?
P6 Fe1 Fe10 61.94(3) . . ?
P1 Fe1 Fe10 63.54(2) 1_545 . ?
O20 Fe1 Fe10 78.16(6) 3_445 . ?
P4 Fe1 Fe10 139.44(3) 3_446 . ?
Mn Fe1 Fe10 122.98(3) 1_545 . ?
O22 Fe1 Fe10 80.21(6) . . ?
O12 Fe1 Fe10 133.55(6) 3_446 . ?
Fe9 Fe1 Fe10 56.922(19) . . ?
O45 Fe2 O48 164.70(15) 4_464 . ?
O45 Fe2 O37 78.69(14) 4_464 4_454 ?
O48 Fe2 O37 92.43(15) . 4_454 ?
O45 Fe2 O40 90.88(14) 4_464 . ?
O48 Fe2 O40 94.69(16) . . ?
O37 Fe2 O40 163.32(15) 4_454 . ?
O45 Fe2 O8 95.56(16) 4_464 . ?
O48 Fe2 O8 99.52(16) . . ?
O37 Fe2 O8 115.55(18) 4_454 . ?
O40 Fe2 O8 78.09(15) . . ?
O45 Fe2 P2 98.51(11) 4_464 . ?
O48 Fe2 P2 93.88(12) . . ?
O37 Fe2 P2 90.05(13) 4_454 . ?
O40 Fe2 P2 104.47(10) . . ?
O8 Fe2 P2 26.61(11) . . ?
O45 Fe2 O7 78.60(13) 4_464 . ?
O48 Fe2 O7 109.04(14) . . ?
O37 Fe2 O7 64.74(14) 4_454 . ?
O40 Fe2 O7 126.28(13) . . ?
O8 Fe2 O7 51.42(14) . . ?
P2 Fe2 O7 29.69(7) . . ?
O45 Fe2 P12 141.00(11) 4_464 . ?
O48 Fe2 P12 24.59(11) . . ?
O37 Fe2 P12 87.43(12) 4_454 . ?
O40 Fe2 P12 92.81(11) . . ?
O8 Fe2 P12 123.17(13) . . ?
P2 Fe2 P12 117.94(4) . . ?
O7 Fe2 P12 127.50(8) . . ?
O45 Fe2 Fe5 39.46(9) 4_464 4_464 ?
O48 Fe2 Fe5 128.11(11) . 4_464 ?
O37 Fe2 Fe5 41.10(10) 4_454 4_464 ?
O40 Fe2 Fe5 124.93(10) . 4_464 ?
O8 Fe2 Fe5 118.75(13) . 4_464 ?
P2 Fe2 Fe5 105.00(4) . 4_464 ?
O7 Fe2 Fe5 75.61(7) . 4_464 ?
P12 Fe2 Fe5 112.25(3) . 4_464 ?
O45 Fe2 O44 113.54(12) 4_464 . ?
O48 Fe2 O44 51.88(13) . . ?
O37 Fe2 O44 78.36(14) 4_454 . ?
O40 Fe2 O44 94.28(13) . . ?
O8 Fe2 O44 150.14(15) . . ?
P2 Fe2 O44 142.54(7) . . ?
O7 Fe2 O44 138.35(11) . . ?
P12 Fe2 O44 27.46(7) . . ?
Fe5 Fe2 O44 89.44(7) 4_464 . ?
O45 Fe2 Na4 138.44(11) 4_464 . ?
O48 Fe2 Na4 47.30(11) . . ?
O37 Fe2 Na4 139.24(12) 4_454 . ?
O40 Fe2 Na4 47.95(10) . . ?
O8 Fe2 Na4 82.64(14) . . ?
P2 Fe2 Na4 97.65(6) . . ?
O7 Fe2 Na4 126.83(9) . . ?
P12 Fe2 Na4 53.66(5) . . ?
Fe5 Fe2 Na4 157.31(6) 4_464 . ?
O44 Fe2 Na4 71.33(8) . . ?
O45 Fe2 P11 21.00(9) 4_464 4_464 ?
O48 Fe2 P11 165.04(12) . 4_464 ?
O37 Fe2 P11 99.42(11) 4_454 4_464 ?
O40 Fe2 P11 71.53(10) . 4_464 ?
O8 Fe2 P11 83.64(12) . 4_464 ?
P2 Fe2 P11 95.20(4) . 4_464 ?
O7 Fe2 P11 84.43(8) . 4_464 ?
P12 Fe2 P11 146.26(5) . 4_464 ?
Fe5 Fe2 P11 60.39(3) 4_464 4_464 ?
O44 Fe2 P11 121.66(7) . 4_464 ?
Na4 Fe2 P11 119.45(5) . 4_464 ?
O45 Fe2 P10 85.19(11) 4_464 . ?
O48 Fe2 P10 94.54(12) . . ?
O37 Fe2 P10 141.68(12) 4_454 . ?
O40 Fe2 P10 22.54(10) . . ?
O8 Fe2 P10 100.34(12) . . ?
P2 Fe2 P10 126.87(4) . . ?
O7 Fe2 P10 144.93(8) . . ?
P12 Fe2 P10 83.65(4) . . ?
Fe5 Fe2 P10 110.08(3) 4_464 . ?
O44 Fe2 P10 76.69(8) . . ?
Na4 Fe2 P10 54.80(5) . . ?
P11 Fe2 P10 70.50(3) 4_464 . ?
O45 Fe2 O36 75.31(12) 4_464 . ?
O48 Fe2 O36 97.82(13) . . ?
O37 Fe2 O36 115.36(13) 4_454 . ?
O40 Fe2 O36 48.68(11) . . ?
O8 Fe2 O36 124.99(12) . . ?
P2 Fe2 O36 151.34(7) . . ?
O7 Fe2 O36 153.13(10) . . ?
P12 Fe2 O36 78.29(7) . . ?
Fe5 Fe2 O36 88.08(6) 4_464 . ?
O44 Fe2 O36 60.84(10) . . ?
Na4 Fe2 O36 72.25(7) . . ?
P11 Fe2 O36 68.88(7) 4_464 . ?
P10 Fe2 O36 26.33(6) . . ?
O45 Fe2 P9 99.42(10) 4_464 4_454 ?
O48 Fe2 P9 72.53(11) . 4_454 ?
O37 Fe2 P9 20.77(10) 4_454 4_454 ?
O40 Fe2 P9 164.45(11) . 4_454 ?
O8 Fe2 P9 112.14(11) . 4_454 ?
P2 Fe2 P9 85.61(3) . 4_454 ?
O7 Fe2 P9 67.69(8) . 4_454 ?
P12 Fe2 P9 71.87(3) . 4_454 ?
Fe5 Fe2 P9 61.62(3) 4_464 4_454 ?
O44 Fe2 P9 70.98(7) . 4_454 ?
Na4 Fe2 P9 119.82(5) . 4_454 ?
P11 Fe2 P9 120.00(4) 4_464 4_454 ?
P10 Fe2 P9 146.43(4) . 4_454 ?
O36 Fe2 P9 122.85(7) . 4_454 ?
O45 Fe2 Fe12 80.20(9) 4_464 . ?
O48 Fe2 Fe12 112.75(11) . . ?
O37 Fe2 Fe12 147.88(12) 4_454 . ?
O40 Fe2 Fe12 38.78(10) . . ?
O8 Fe2 Fe12 43.32(11) . . ?
P2 Fe2 Fe12 69.47(3) . . ?
O7 Fe2 Fe12 87.55(8) . . ?
P12 Fe2 Fe12 123.72(4) . . ?
Fe5 Fe2 Fe12 119.11(3) 4_464 . ?
O44 Fe2 Fe12 132.71(8) . . ?
Na4 Fe2 Fe12 70.19(5) . . ?
P11 Fe2 Fe12 60.00(3) 4_464 . ?
P10 Fe2 Fe12 58.95(3) . . ?
O36 Fe2 Fe12 81.88(6) . . ?
P9 Fe2 Fe12 154.61(4) 4_454 . ?
O38 Fe3 O5 105.77(16) 4_565 . ?
O38 Fe3 O39 165.07(14) 4_565 . ?
O5 Fe3 O39 82.83(14) . . ?
O38 Fe3 O46 79.32(14) 4_565 4 ?
O5 Fe3 O46 90.77(14) . 4 ?
O39 Fe3 O46 88.52(14) . 4 ?
O38 Fe3 O47 95.16(15) 4_565 . ?
O5 Fe3 O47 101.69(15) . . ?
O39 Fe3 O47 94.97(16) . . ?
O46 Fe3 O47 167.38(15) 4 . ?
O38 Fe3 O43 82.06(14) 4_565 2_565 ?
O5 Fe3 O43 156.54(13) . 2_565 ?
O39 Fe3 O43 94.84(13) . 2_565 ?
O46 Fe3 O43 112.56(13) 4 2_565 ?
O47 Fe3 O43 55.11(14) . 2_565 ?
O38 Fe3 P11 90.92(11) 4_565 . ?
O5 Fe3 P11 128.30(10) . . ?
O39 Fe3 P11 93.14(11) . . ?
O46 Fe3 P11 140.81(11) 4 . ?
O47 Fe3 P11 27.02(12) . . ?
O43 Fe3 P11 28.28(8) 2_565 . ?
O38 Fe3 Fe4 43.29(10) 4_565 4_565 ?
O5 Fe3 Fe4 112.65(10) . 4_565 ?
O39 Fe3 Fe4 122.31(10) . 4_565 ?
O46 Fe3 Fe4 39.37(9) 4 4_565 ?
O47 Fe3 Fe4 130.98(11) . 4_565 ?
O43 Fe3 Fe4 88.40(8) 2_565 4_565 ?
P11 Fe3 Fe4 112.69(4) . 4_565 ?
O38 Fe3 Na2 143.05(11) 4_565 . ?
O5 Fe3 Na2 85.35(13) . . ?
O39 Fe3 Na2 48.14(11) . . ?
O46 Fe3 Na2 136.65(11) 4 . ?
O47 Fe3 Na2 47.89(11) . . ?
O43 Fe3 Na2 76.03(10) 2_565 . ?
P11 Fe3 Na2 56.70(6) . . ?
Fe4 Fe3 Na2 159.77(8) 4_565 . ?
O38 Fe3 P10 21.38(10) 4_565 4_565 ?
O5 Fe3 P10 108.01(11) . 4_565 ?
O39 Fe3 P10 165.58(11) . 4_565 ?
O46 Fe3 P10 100.55(10) 4 4_565 ?
O47 Fe3 P10 73.84(11) . 4_565 ?
O43 Fe3 P10 71.38(8) 2_565 4_565 ?
P11 Fe3 P10 72.73(3) . 4_565 ?
Fe4 Fe3 P10 63.10(3) 4_565 4_565 ?
Na2 Fe3 P10 121.71(5) . 4_565 ?
O38 Fe3 P1 99.20(11) 4_565 3_545 ?
O5 Fe3 P1 20.19(9) . 3_545 ?
O39 Fe3 P1 92.84(10) . 3_545 ?
O46 Fe3 P1 108.58(11) 4 3_545 ?
O47 Fe3 P1 83.41(12) . 3_545 ?
O43 Fe3 P1 138.27(8) 2_565 3_545 ?
P11 Fe3 P1 110.43(4) . 3_545 ?
Fe4 Fe3 P1 120.99(3) 4_565 3_545 ?
Na2 Fe3 P1 79.08(8) . 3_545 ?
P10 Fe3 P1 94.83(3) 4_565 3_545 ?
O38 Fe3 P9 145.75(11) 4_565 . ?
O5 Fe3 P9 103.66(11) . . ?
O39 Fe3 P9 21.47(10) . . ?
O46 Fe3 P9 83.17(10) 4 . ?
O47 Fe3 P9 95.67(11) . . ?
O43 Fe3 P9 77.84(8) 2_565 . ?
P11 Fe3 P9 84.34(4) . . ?
Fe4 Fe3 P9 108.30(3) 4_565 . ?
Na2 Fe3 P9 56.25(6) . . ?
P10 Fe3 P9 148.01(4) 4_565 . ?
P1 Fe3 P9 114.27(3) 3_545 . ?
O38 Fe3 O49 62.31(13) 4_565 4_565 ?
O5 Fe3 O49 147.00(12) . 4_565 ?
O39 Fe3 O49 103.83(12) . 4_565 ?
O46 Fe3 O49 57.67(12) 4 4_565 ?
O47 Fe3 O49 109.71(13) . 4_565 ?
O43 Fe3 O49 56.24(10) 2_565 4_565 ?
P11 Fe3 O49 84.09(7) . 4_565 ?
Fe4 Fe3 O49 36.70(7) 4_565 4_565 ?
Na2 Fe3 O49 123.41(10) . 4_565 ?
P10 Fe3 O49 72.47(7) 4_565 4_565 ?
P1 Fe3 O49 157.44(7) 3_545 4_565 ?
P9 Fe3 O49 83.46(7) . 4_565 ?
O38 Fe3 P12 98.12(10) 4_565 4 ?
O5 Fe3 P12 79.89(10) . 4 ?
O39 Fe3 P12 70.98(11) . 4 ?
O46 Fe3 P12 19.73(9) 4 4 ?
O47 Fe3 P12 165.66(11) . 4 ?
O43 Fe3 P12 121.54(8) 2_565 4 ?
P11 Fe3 P12 146.69(5) . 4 ?
Fe4 Fe3 P12 59.09(3) 4_565 4 ?
Na2 Fe3 P12 118.66(5) . 4 ?
P10 Fe3 P12 119.50(4) 4_565 4 ?
P1 Fe3 P12 99.72(3) 3_545 4 ?
P9 Fe3 P12 70.23(3) . 4 ?
O49 Fe3 P12 72.25(7) 4_565 4 ?
O38 Fe3 O35 119.86(13) 4_565 2_565 ?
O5 Fe3 O35 126.55(12) . 2_565 ?
O39 Fe3 O35 47.19(11) . 2_565 ?
O46 Fe3 O35 73.13(12) 4 2_565 ?
O47 Fe3 O35 100.46(13) . 2_565 ?
O43 Fe3 O35 62.25(11) 2_565 2_565 ?
P11 Fe3 O35 79.54(7) . 2_565 ?
Fe4 Fe3 O35 86.50(6) 4_565 2_565 ?
Na2 Fe3 O35 74.90(9) . 2_565 ?
P10 Fe3 O35 124.75(7) 4_565 2_565 ?
P1 Fe3 O35 139.93(6) 3_545 2_565 ?
P9 Fe3 O35 25.97(6) . 2_565 ?
O49 Fe3 O35 57.71(9) 4_565 2_565 ?
P12 Fe3 O35 68.12(7) 4 2_565 ?
O38 Fe3 Fe13 144.29(11) 4_565 4 ?
O5 Fe3 Fe13 48.43(10) . 4 ?
O39 Fe3 Fe13 37.29(10) . 4 ?
O46 Fe3 Fe13 77.31(9) 4 4 ?
O47 Fe3 Fe13 112.51(11) . 4 ?
O43 Fe3 Fe13 132.05(9) 2_565 4 ?
P11 Fe3 Fe13 123.97(3) . 4 ?
Fe4 Fe3 Fe13 116.39(3) 4_565 4 ?
Na2 Fe3 Fe13 68.03(6) . 4 ?
P10 Fe3 Fe13 155.81(4) 4_565 4 ?
P1 Fe3 Fe13 63.95(3) 3_545 4 ?
P9 Fe3 Fe13 56.15(3) . 4 ?
O49 Fe3 Fe13 122.93(7) 4_565 4 ?
P12 Fe3 Fe13 57.87(3) 4 4 ?
O35 Fe3 Fe13 78.16(6) 2_565 4 ?
O27 Fe4 O46 173.42(14) . 1_565 ?
O27 Fe4 O49 91.94(15) . . ?
O46 Fe4 O49 87.95(15) 1_565 . ?
O27 Fe4 O17 91.00(14) . 1_565 ?
O46 Fe4 O17 95.58(14) 1_565 1_565 ?
O49 Fe4 O17 93.31(15) . 1_565 ?
O27 Fe4 O38 94.58(14) . . ?
O46 Fe4 O38 78.83(14) 1_565 . ?
O49 Fe4 O38 90.09(16) . . ?
O17 Fe4 O38 173.36(14) 1_565 . ?
O27 Fe4 O1 89.63(14) . 3_455 ?
O46 Fe4 O1 91.46(15) 1_565 3_455 ?
O49 Fe4 O1 171.41(15) . 3_455 ?
O17 Fe4 O1 78.22(13) 1_565 3_455 ?
O38 Fe4 O1 98.21(14) . 3_455 ?
O27 Fe4 Fe3 132.25(10) . 4_464 ?
O46 Fe4 Fe3 41.46(10) 1_565 4_464 ?
O49 Fe4 Fe3 76.10(12) . 4_464 ?
O17 Fe4 Fe3 135.01(10) 1_565 4_464 ?
O38 Fe4 Fe3 40.70(9) . 4_464 ?
O1 Fe4 Fe3 108.87(10) 3_455 4_464 ?
O27 Fe4 Na1 43.39(10) . 1_554 ?
O46 Fe4 Na1 142.91(11) 1_565 1_554 ?
O49 Fe4 Na1 103.01(13) . 1_554 ?
O17 Fe4 Na1 49.10(10) 1_565 1_554 ?
O38 Fe4 Na1 135.41(11) . 1_554 ?
O1 Fe4 Na1 72.56(11) 3_455 1_554 ?
Fe3 Fe4 Na1 175.63(5) 4_464 1_554 ?
O27 Fe4 Fe11 121.07(10) . 1_565 ?
O46 Fe4 Fe11 61.74(11) 1_565 1_565 ?
O49 Fe4 Fe11 37.24(10) . 1_565 ?
O17 Fe4 Fe11 71.40(10) 1_565 1_565 ?
O38 Fe4 Fe11 108.48(11) . 1_565 ?
O1 Fe4 Fe11 136.18(10) 3_455 1_565 ?
Fe3 Fe4 Fe11 74.67(3) 4_464 1_565 ?
Na1 Fe4 Fe11 107.30(6) 1_554 1_565 ?
O27 Fe4 O31 40.05(11) . . ?
O46 Fe4 O31 137.58(12) 1_565 . ?
O49 Fe4 O31 53.80(12) . . ?
O17 Fe4 O31 103.40(11) 1_565 . ?
O38 Fe4 O31 83.20(11) . . ?
O1 Fe4 O31 129.20(11) 3_455 . ?
Fe3 Fe4 O31 104.54(6) 4_464 . ?
Na1 Fe4 O31 71.80(7) 1_554 . ?
Fe11 Fe4 O31 88.83(6) 1_565 . ?
O27 Fe4 O30 74.97(11) . 1_464 ?
O46 Fe4 O30 110.15(11) 1_565 1_464 ?
O49 Fe4 O30 128.43(13) . 1_464 ?
O17 Fe4 O30 39.10(10) 1_565 1_464 ?
O38 Fe4 O30 139.64(12) . 1_464 ?
O1 Fe4 O30 44.13(10) 3_455 1_464 ?
Fe3 Fe4 O30 146.69(5) 4_464 1_464 ?
Na1 Fe4 O30 36.70(7) 1_554 1_464 ?
Fe11 Fe4 O30 110.23(5) 1_565 1_464 ?
O31 Fe4 O30 108.43(7) . 1_464 ?
O28 Fe5 O45 175.88(14) 1_565 . ?
O28 Fe5 O50 92.32(14) 1_565 3 ?
O45 Fe5 O50 87.64(15) . 3 ?
O28 Fe5 O37 96.77(14) 1_565 1_565 ?
O45 Fe5 O37 79.10(15) . 1_565 ?
O50 Fe5 O37 88.04(16) 3 1_565 ?
O28 Fe5 O18 89.92(13) 1_565 3 ?
O45 Fe5 O18 94.20(13) . 3 ?
O50 Fe5 O18 88.08(13) 3 3 ?
O37 Fe5 O18 172.39(15) 1_565 3 ?
O28 Fe5 O2 87.57(13) 1_565 . ?
O45 Fe5 O2 93.39(14) . . ?
O50 Fe5 O2 167.18(13) 3 . ?
O37 Fe5 O2 104.71(15) 1_565 . ?
O18 Fe5 O2 79.11(12) 3 . ?
O28 Fe5 Fe2 136.53(10) 1_565 4_565 ?
O45 Fe5 Fe2 39.49(9) . 4_565 ?
O50 Fe5 Fe2 77.68(10) 3 4_565 ?
O37 Fe5 Fe2 41.50(11) 1_565 4_565 ?
O18 Fe5 Fe2 131.09(9) 3 4_565 ?
O2 Fe5 Fe2 110.93(9) . 4_565 ?
O28 Fe5 Na1 41.90(10) 1_565 1_655 ?
O45 Fe5 Na1 142.13(10) . 1_655 ?
O50 Fe5 Na1 100.10(12) 3 1_655 ?
O37 Fe5 Na1 137.65(12) 1_565 1_655 ?
O18 Fe5 Na1 49.64(10) 3 1_655 ?
O2 Fe5 Na1 71.47(10) . 1_655 ?
Fe2 Fe5 Na1 177.46(6) 4_565 1_655 ?
O28 Fe5 Fe13 76.63(10) 1_565 4_565 ?
O45 Fe5 Fe13 101.08(11) . 4_565 ?
O50 Fe5 Fe13 36.06(9) 3 4_565 ?
O37 Fe5 Fe13 58.73(13) 1_565 4_565 ?
O18 Fe5 Fe13 119.86(9) 3 4_565 ?
O2 Fe5 Fe13 154.70(9) . 4_565 ?
Fe2 Fe5 Fe13 70.64(3) 4_565 4_565 ?
Na1 Fe5 Fe13 106.84(5) 1_655 4_565 ?
O28 Fe5 O30 24.98(10) 1_565 1_565 ?
O45 Fe5 O30 157.30(12) . 1_565 ?
O50 Fe5 O30 72.83(11) 3 1_565 ?
O37 Fe5 O30 110.86(12) 1_565 1_565 ?
O18 Fe5 O30 74.14(10) 3 1_565 ?
O2 Fe5 O30 103.13(11) . 1_565 ?
Fe2 Fe5 O30 140.33(6) 4_565 1_565 ?
Na1 Fe5 O30 37.20(7) 1_655 1_565 ?
Fe13 Fe5 O30 69.87(5) 4_565 1_565 ?
O41 Fe6 O18 91.60(14) 1_455 3_455 ?
O41 Fe6 O2 97.10(14) 1_455 1_455 ?
O18 Fe6 O2 83.60(12) 3_455 1_455 ?
O41 Fe6 O13 89.58(14) 1_455 . ?
O18 Fe6 O13 177.16(13) 3_455 . ?
O2 Fe6 O13 98.83(12) 1_455 . ?
O41 Fe6 O9 92.18(14) 1_455 . ?
O18 Fe6 O9 109.01(12) 3_455 . ?
O2 Fe6 O9 164.18(13) 1_455 . ?
O13 Fe6 O9 68.35(12) . . ?
O41 Fe6 O29 170.31(14) 1_455 . ?
O18 Fe6 O29 86.85(13) 3_455 . ?
O2 Fe6 O29 92.23(13) 1_455 . ?
O13 Fe6 O29 91.56(14) . . ?
O9 Fe6 O29 79.32(12) . . ?
O41 Fe6 P3 93.90(10) 1_455 . ?
O18 Fe6 P3 143.05(9) 3_455 . ?
O2 Fe6 P3 131.64(10) 1_455 . ?
O13 Fe6 P3 34.22(9) . . ?
O9 Fe6 P3 34.34(8) . . ?
O29 Fe6 P3 81.73(9) . . ?
O41 Fe6 Na5 53.82(12) 1_455 . ?
O18 Fe6 Na5 112.47(11) 3_455 . ?
O2 Fe6 Na5 53.34(11) 1_455 . ?
O13 Fe6 Na5 70.28(10) . . ?
O9 Fe6 Na5 125.61(10) . . ?
O29 Fe6 Na5 135.35(10) . . ?
P3 Fe6 Na5 100.05(6) . . ?
O41 Fe6 Na1 137.45(12) 1_455 . ?
O18 Fe6 Na1 47.66(11) 3_455 . ?
O2 Fe6 Na1 70.47(10) 1_455 . ?
O13 Fe6 Na1 131.75(11) . . ?
O9 Fe6 Na1 110.53(9) . . ?
O29 Fe6 Na1 44.35(10) . . ?
P3 Fe6 Na1 125.26(5) . . ?
Na5 Fe6 Na1 123.24(7) . . ?
O41 Fe6 Na2 47.14(12) 1_455 1_455 ?
O18 Fe6 Na2 76.01(11) 3_455 1_455 ?
O2 Fe6 Na2 137.02(11) 1_455 1_455 ?
O13 Fe6 Na2 102.98(11) . 1_455 ?
O9 Fe6 Na2 57.61(10) . 1_455 ?
O29 Fe6 Na2 123.34(10) . 1_455 ?
P3 Fe6 Na2 81.27(6) . 1_455 ?
Na5 Fe6 Na2 100.76(7) . 1_455 ?
Na1 Fe6 Na2 116.78(8) . 1_455 ?
O41 Fe6 Fe13 90.27(11) 1_455 2_565 ?
O18 Fe6 Fe13 162.89(9) 3_455 2_565 ?
O2 Fe6 Fe13 79.29(9) 1_455 2_565 ?
O13 Fe6 Fe13 19.61(9) . 2_565 ?
O9 Fe6 Fe13 87.91(8) . 2_565 ?
O29 Fe6 Fe13 94.02(9) . 2_565 ?
P3 Fe6 Fe13 53.64(3) . 2_565 ?
Na5 Fe6 Fe13 56.11(6) . 2_565 ?
Na1 Fe6 Fe13 124.75(6) . 2_565 ?
Na2 Fe6 Fe13 116.94(6) 1_455 2_565 ?
O42 Fe7 O1 95.75(14) 1_655 3_545 ?
O42 Fe7 O14 90.45(14) 1_655 3_545 ?
O1 Fe7 O14 104.38(13) 3_545 3_545 ?
O42 Fe7 O30 167.00(14) 1_655 1_554 ?
O1 Fe7 O30 95.07(14) 3_545 1_554 ?
O14 Fe7 O30 93.82(14) 3_545 1_554 ?
O42 Fe7 O17 87.76(15) 1_655 1_655 ?
O1 Fe7 O17 81.43(13) 3_545 1_655 ?
O14 Fe7 O17 174.07(13) 3_545 1_655 ?
O30 Fe7 O17 86.75(14) 1_554 1_655 ?
O42 Fe7 O10 88.30(13) 1_655 . ?
O1 Fe7 O10 170.50(13) 3_545 . ?
O14 Fe7 O10 66.92(12) 3_545 . ?
O30 Fe7 O10 82.12(12) 1_554 . ?
O17 Fe7 O10 107.36(12) 1_655 . ?
O42 Fe7 P4 91.58(10) 1_655 . ?
O1 Fe7 P4 137.13(10) 3_545 . ?
O14 Fe7 P4 33.22(9) 3_545 . ?
O30 Fe7 P4 85.36(10) 1_554 . ?
O17 Fe7 P4 141.16(9) 1_655 . ?
O10 Fe7 P4 33.84(8) . . ?
O42 Fe7 Na4 41.28(11) 1_655 1_655 ?
O1 Fe7 Na4 131.52(11) 3_545 1_655 ?
O14 Fe7 Na4 98.22(10) 3_545 1_655 ?
O30 Fe7 Na4 125.80(10) 1_554 1_655 ?
O17 Fe7 Na4 76.75(10) 1_655 1_655 ?
O10 Fe7 Na4 55.81(9) . 1_655 ?
P4 Fe7 Na4 77.41(5) . 1_655 ?
O42 Fe7 Na1 132.58(11) 1_655 1_644 ?
O1 Fe7 Na1 70.50(11) 3_545 1_644 ?
O14 Fe7 Na1 136.54(11) 3_545 1_644 ?
O30 Fe7 Na1 45.96(11) 1_554 1_644 ?
O17 Fe7 Na1 46.21(11) 1_655 1_644 ?
O10 Fe7 Na1 112.77(9) . 1_644 ?
P4 Fe7 Na1 129.83(5) . 1_644 ?
Na4 Fe7 Na1 117.68(7) 1_655 1_644 ?
O42 Fe7 Na3 144.76(11) 1_655 3_545 ?
O1 Fe7 Na3 54.17(10) 3_545 3_545 ?
O14 Fe7 Na3 81.48(10) 3_545 3_545 ?
O30 Fe7 Na3 48.20(9) 1_554 3_545 ?
O17 Fe7 Na3 103.17(10) 1_655 3_545 ?
O10 Fe7 Na3 118.87(9) . 3_545 ?
P4 Fe7 Na3 99.51(4) . 3_545 ?
Na4 Fe7 Na3 173.80(5) 1_655 3_545 ?
Na1 Fe7 Na3 60.15(6) 1_644 3_545 ?
O42 Fe7 O31 122.68(11) 1_655 3_545 ?
O1 Fe7 O31 85.86(10) 3_545 3_545 ?
O14 Fe7 O31 35.48(10) 3_545 3_545 ?
O30 Fe7 O31 65.33(11) 1_554 3_545 ?
O17 Fe7 O31 148.12(11) 1_655 3_545 ?
O10 Fe7 O31 84.73(10) . 3_545 ?
P4 Fe7 O31 55.42(5) . 3_545 ?
Na4 Fe7 O31 131.61(6) 1_655 3_545 ?
Na1 Fe7 O31 101.95(7) 1_644 3_545 ?
Na3 Fe7 O31 46.88(6) 3_545 3_545 ?
O34 Fe8 O22 172.27(14) 1_655 3_554 ?
O34 Fe8 O12 88.81(14) 1_655 . ?
O22 Fe8 O12 96.50(14) 3_554 . ?
O34 Fe8 O3 99.14(14) 1_655 3 ?
O22 Fe8 O3 87.36(13) 3_554 3 ?
O12 Fe8 O3 79.72(12) . 3 ?
O34 Fe8 O27 89.40(13) 1_655 1_655 ?
O22 Fe8 O27 84.25(13) 3_554 1_655 ?
O12 Fe8 O27 168.31(12) . 1_655 ?
O3 Fe8 O27 111.97(12) 3 1_655 ?
O34 Fe8 O25 87.35(13) 1_655 1_655 ?
O22 Fe8 O25 85.88(12) 3_554 1_655 ?
O12 Fe8 O25 104.81(12) . 1_655 ?
O3 Fe8 O25 172.24(12) 3 1_655 ?
O27 Fe8 O25 63.56(11) 1_655 1_655 ?
O34 Fe8 Na4 47.31(11) 1_655 1_655 ?
O22 Fe8 Na4 126.89(10) 3_554 1_655 ?
O12 Fe8 Na4 89.21(10) . 1_655 ?
O3 Fe8 Na4 145.19(10) 3 1_655 ?
O27 Fe8 Na4 81.11(9) 1_655 1_655 ?
O25 Fe8 Na4 42.18(9) 1_655 1_655 ?
O34 Fe8 Fe11 93.42(10) 1_655 3 ?
O22 Fe8 Fe11 94.22(10) 3_554 3 ?
O12 Fe8 Fe11 37.66(9) . 3 ?
O3 Fe8 Fe11 42.11(9) 3 3 ?
O27 Fe8 Fe11 154.03(9) 1_655 3 ?
O25 Fe8 Fe11 142.33(8) 1_655 3 ?
Na4 Fe8 Fe11 119.09(5) 1_655 3 ?
O34 Fe8 Na3 144.67(11) 1_655 3 ?
O22 Fe8 Na3 41.91(10) 3_554 3 ?
O12 Fe8 Na3 85.59(10) . 3 ?
O3 Fe8 Na3 45.54(10) 3 3 ?
O27 Fe8 Na3 102.40(10) 1_655 3 ?
O25 Fe8 Na3 127.79(9) 1_655 3 ?
Na4 Fe8 Na3 166.55(6) 1_655 3 ?
Fe11 Fe8 Na3 62.03(4) 3 3 ?
O34 Fe8 O31 72.15(11) 1_655 1_655 ?
O22 Fe8 O31 100.14(11) 3_554 1_655 ?
O12 Fe8 O31 134.08(10) . 1_655 ?
O3 Fe8 O31 143.13(10) 3 1_655 ?
O27 Fe8 O31 34.94(10) 1_655 1_655 ?
O25 Fe8 O31 35.43(9) 1_655 1_655 ?
Na4 Fe8 O31 47.13(7) 1_655 1_655 ?
Fe11 Fe8 O31 164.73(6) 3 1_655 ?
Na3 Fe8 O31 133.06(7) 3 1_655 ?
O34 Fe8 Fe1 137.63(10) 1_655 3_554 ?
O22 Fe8 Fe1 46.83(10) 3_554 3_554 ?
O12 Fe8 Fe1 49.87(9) . 3_554 ?
O3 Fe8 Fe1 83.95(9) 3 3_554 ?
O27 Fe8 Fe1 128.83(9) 1_655 3_554 ?
O25 Fe8 Fe1 94.15(8) 1_655 3_554 ?
Na4 Fe8 Fe1 113.65(4) 1_655 3_554 ?
Fe11 Fe8 Fe1 60.983(18) 3 3_554 ?
Na3 Fe8 Fe1 54.04(5) 3 3_554 ?
O31 Fe8 Fe1 127.05(5) 1_655 3_554 ?
O33 Fe9 O4 97.86(14) 1_455 . ?
O33 Fe9 O11 93.52(14) 1_455 . ?
O4 Fe9 O11 79.44(13) . . ?
O33 Fe9 O21 173.31(15) 1_455 . ?
O4 Fe9 O21 87.28(13) . . ?
O11 Fe9 O21 91.63(14) . . ?
O33 Fe9 O28 91.30(14) 1_455 1_455 ?
O4 Fe9 O28 110.81(12) . 1_455 ?
O11 Fe9 O28 167.97(12) . 1_455 ?
O21 Fe9 O28 82.84(14) . 1_455 ?
O33 Fe9 O26 90.58(14) 1_455 1_455 ?
O4 Fe9 O26 170.02(12) . 1_455 ?
O11 Fe9 O26 105.48(12) . 1_455 ?
O21 Fe9 O26 83.93(12) . 1_455 ?
O28 Fe9 O26 63.42(11) 1_455 1_455 ?
O33 Fe9 Na2 49.33(12) 1_455 1_455 ?
O4 Fe9 Na2 146.43(11) . 1_455 ?
O11 Fe9 Na2 93.99(11) . 1_455 ?
O21 Fe9 Na2 126.03(11) . 1_455 ?
O28 Fe9 Na2 80.84(11) 1_455 1_455 ?
O26 Fe9 Na2 42.99(9) 1_455 1_455 ?
O33 Fe9 Fe1 153.98(11) 1_455 . ?
O4 Fe9 Fe1 56.94(10) . . ?
O11 Fe9 Fe1 76.66(10) . . ?
O21 Fe9 Fe1 32.13(10) . . ?
O28 Fe9 Fe1 103.24(9) 1_455 . ?
O26 Fe9 Fe1 115.16(8) 1_455 . ?
Na2 Fe9 Fe1 153.56(5) 1_455 . ?
O33 Fe9 O30 107.11(12) 1_455 1_455 ?
O4 Fe9 O30 135.07(10) . 1_455 ?
O11 Fe9 O30 133.67(10) . 1_455 ?
O21 Fe9 O30 66.20(11) . 1_455 ?
O28 Fe9 O30 34.34(9) 1_455 1_455 ?
O26 Fe9 O30 35.94(9) 1_455 1_455 ?
Na2 Fe9 O30 71.69(8) 1_455 1_455 ?
Fe1 Fe9 O30 96.75(6) . 1_455 ?
O36 Fe10 O11 101.16(14) 2_565 . ?
O36 Fe10 O50 100.04(15) 2_565 . ?
O11 Fe10 O50 81.71(13) . . ?
O36 Fe10 O24 171.03(14) 2_565 . ?
O11 Fe10 O24 84.64(13) . . ?
O50 Fe10 O24 87.50(13) . . ?
O36 Fe10 O4 89.08(15) 2_565 . ?
O11 Fe10 O4 75.28(12) . . ?
O50 Fe10 O4 156.52(12) . . ?
O24 Fe10 O4 85.77(13) . . ?
O36 Fe10 O47 86.30(14) 2_565 3_445 ?
O11 Fe10 O47 165.22(14) . 3_445 ?
O50 Fe10 O47 109.77(13) . 3_445 ?
O24 Fe10 O47 86.56(13) . 3_445 ?
O4 Fe10 O47 92.26(13) . 3_445 ?
O36 Fe10 Fe1 144.54(12) 2_565 . ?
O11 Fe10 Fe1 75.04(9) . . ?
O50 Fe10 Fe1 113.90(10) . . ?
O24 Fe10 Fe1 30.37(9) . . ?
O4 Fe10 Fe1 55.61(9) . . ?
O47 Fe10 Fe1 91.44(10) 3_445 . ?
O36 Fe10 Fe3 69.04(10) 2_565 3_445 ?
O11 Fe10 Fe3 140.75(9) . 3_445 ?
O50 Fe10 Fe3 136.59(10) . 3_445 ?
O24 Fe10 Fe3 102.13(9) . 3_445 ?
O4 Fe10 Fe3 66.88(8) . 3_445 ?
O47 Fe10 Fe3 31.26(10) 3_445 3_445 ?
Fe1 Fe10 Fe3 91.41(2) . 3_445 ?
O36 Fe10 Fe13 82.12(11) 2_565 2_565 ?
O11 Fe10 Fe13 68.22(9) . 2_565 ?
O50 Fe10 Fe13 25.05(9) . 2_565 ?
O24 Fe10 Fe13 106.51(9) . 2_565 ?
O4 Fe10 Fe13 139.79(9) . 2_565 ?
O47 Fe10 Fe13 125.90(10) 3_445 2_565 ?
Fe1 Fe10 Fe13 125.90(2) . 2_565 ?
Fe3 Fe10 Fe13 141.36(2) 3_445 2_565 ?
O36 Fe10 Fe2 55.02(11) 2_565 2_565 ?
O11 Fe10 Fe2 122.20(9) . 2_565 ?
O50 Fe10 Fe2 57.73(9) . 2_565 ?
O24 Fe10 Fe2 127.37(9) . 2_565 ?
O4 Fe10 Fe2 140.94(9) . 2_565 ?
O47 Fe10 Fe2 72.52(9) 3_445 2_565 ?
Fe1 Fe10 Fe2 155.40(3) . 2_565 ?
Fe3 Fe10 Fe2 84.35(2) 3_445 2_565 ?
Fe13 Fe10 Fe2 57.677(17) 2_565 2_565 ?
O35 Fe11 O23 172.84(15) 3_445 . ?
O35 Fe11 O12 97.99(14) 3_445 3_445 ?
O23 Fe11 O12 85.84(13) . 3_445 ?
O35 Fe11 O49 98.26(16) 3_445 1_545 ?
O23 Fe11 O49 88.24(15) . 1_545 ?
O12 Fe11 O49 82.16(13) 3_445 1_545 ?
O35 Fe11 O3 89.29(14) 3_445 . ?
O23 Fe11 O3 85.83(13) . . ?
O12 Fe11 O3 75.22(12) 3_445 . ?
O49 Fe11 O3 156.95(12) 1_545 . ?
O35 Fe11 O48 85.71(14) 3_445 . ?
O23 Fe11 O48 89.19(13) . . ?
O12 Fe11 O48 166.24(13) 3_445 . ?
O49 Fe11 O48 110.54(13) 1_545 . ?
O3 Fe11 O48 91.64(12) . . ?
O35 Fe11 O46 81.05(13) 3_445 . ?
O23 Fe11 O46 99.68(11) . . ?
O12 Fe11 O46 141.99(11) 3_445 . ?
O49 Fe11 O46 60.66(11) 1_545 . ?
O3 Fe11 O46 142.35(10) . . ?
O48 Fe11 O46 51.59(11) . . ?
O35 Fe11 P5 158.71(11) 3_445 . ?
O23 Fe11 P5 20.73(9) . . ?
O12 Fe11 P5 102.25(9) 3_445 . ?
O49 Fe11 P5 78.20(11) 1_545 . ?
O3 Fe11 P5 102.14(9) . . ?
O48 Fe11 P5 76.17(10) . . ?
O46 Fe11 P5 78.96(7) . . ?
O35 Fe11 P9 16.67(10) 3_445 4_454 ?
O23 Fe11 P9 158.06(10) . 4_454 ?
O12 Fe11 P9 114.49(10) 3_445 4_454 ?
O49 Fe11 P9 102.10(11) 1_545 4_454 ?
O3 Fe11 P9 91.37(9) . 4_454 ?
O48 Fe11 P9 69.12(10) . 4_454 ?
O46 Fe11 P9 69.83(7) . 4_454 ?
P5 Fe11 P9 143.03(4) . 4_454 ?
O35 Fe11 P4 104.64(11) 3_445 3_445 ?
O23 Fe11 P4 80.99(10) . 3_445 ?
O12 Fe11 P4 20.00(9) 3_445 3_445 ?
O49 Fe11 P4 62.79(10) 1_545 3_445 ?
O3 Fe11 P4 94.26(8) . 3_445 ?
O48 Fe11 P4 168.13(10) . 3_445 ?
O46 Fe11 P4 123.38(7) . 3_445 ?
P5 Fe11 P4 92.50(3) . 3_445 ?
P9 Fe11 P4 120.94(4) 4_454 3_445 ?
O35 Fe11 P12 85.15(11) 3_445 . ?
O23 Fe11 P12 92.34(10) . . ?
O12 Fe11 P12 167.96(10) 3_445 . ?
O49 Fe11 P12 85.89(10) 1_545 . ?
O3 Fe11 P12 116.56(9) . . ?
O48 Fe11 P12 24.96(9) . . ?
O46 Fe11 P12 26.85(7) . . ?
P5 Fe11 P12 73.69(3) . . ?
P9 Fe11 P12 69.50(3) 4_454 . ?
P4 Fe11 P12 148.01(4) 3_445 . ?
O35 Fe11 Fe8 93.36(11) 3_445 3_445 ?
O23 Fe11 Fe8 86.08(10) . 3_445 ?
O12 Fe11 Fe8 36.80(9) 3_445 3_445 ?
O49 Fe11 Fe8 118.92(10) 1_545 3_445 ?
O3 Fe11 Fe8 38.46(8) . 3_445 ?
O48 Fe11 Fe8 130.08(9) . 3_445 ?
O46 Fe11 Fe8 174.15(7) . 3_445 ?
P5 Fe11 Fe8 106.80(3) . 3_445 ?
P9 Fe11 Fe8 105.08(3) 4_454 3_445 ?
P4 Fe11 Fe8 56.25(3) 3_445 3_445 ?
P12 Fe11 Fe8 155.02(4) . 3_445 ?
O35 Fe11 O17 136.35(12) 3_445 . ?
O23 Fe11 O17 45.45(11) . . ?
O12 Fe11 O17 113.55(11) 3_445 . ?
O49 Fe11 O17 59.54(12) 1_545 . ?
O3 Fe11 O17 126.47(10) . . ?
O48 Fe11 O17 70.88(11) . . ?
O46 Fe11 O17 55.45(8) . . ?
P5 Fe11 O17 25.62(6) . . ?
P9 Fe11 O17 124.62(6) 4_454 . ?
P4 Fe11 O17 97.37(6) 3_445 . ?
P12 Fe11 O17 58.22(6) . . ?
Fe8 Fe11 O17 129.98(6) 3_445 . ?
O35 Fe11 Fe4 105.06(12) 3_445 1_545 ?
O23 Fe11 Fe4 78.79(10) . 1_545 ?
O12 Fe11 Fe4 112.71(9) 3_445 1_545 ?
O49 Fe11 Fe4 33.02(10) 1_545 1_545 ?
O3 Fe11 Fe4 161.89(9) . 1_545 ?
O48 Fe11 Fe4 78.75(9) . 1_545 ?
O46 Fe11 Fe4 34.76(6) . 1_545 ?
P5 Fe11 Fe4 60.83(3) . 1_545 ?
P9 Fe11 Fe4 99.32(3) 4_454 1_545 ?
P4 Fe11 Fe4 92.72(3) 3_445 1_545 ?
P12 Fe11 Fe4 55.31(3) . 1_545 ?
Fe8 Fe11 Fe4 147.45(3) 3_445 1_545 ?
O17 Fe11 Fe4 35.80(5) . 1_545 ?
O35 Fe11 Na3 132.14(12) 3_445 . ?
O23 Fe11 Na3 42.09(10) . . ?
O12 Fe11 Na3 82.97(10) 3_445 . ?
O49 Fe11 Na3 128.92(12) 1_545 . ?
O3 Fe11 Na3 44.37(9) . . ?
O48 Fe11 Na3 84.74(10) . . ?
O46 Fe11 Na3 125.60(8) . . ?
P5 Fe11 Na3 57.92(5) . . ?
P9 Fe11 Na3 128.45(5) 4_454 . ?
P4 Fe11 Na3 92.29(5) 3_445 . ?
P12 Fe11 Na3 103.60(5) . . ?
Fe8 Fe11 Na3 59.67(4) 3_445 . ?
O17 Fe11 Na3 83.00(7) . . ?
Fe4 Fe11 Na3 118.69(5) 1_545 . ?
O35 Fe11 P2 79.93(12) 3_445 . ?
O23 Fe11 P2 94.01(10) . . ?
O12 Fe11 P2 90.88(9) 3_445 . ?
O49 Fe11 P2 172.52(10) 1_545 . ?
O3 Fe11 P2 17.20(8) . . ?
O48 Fe11 P2 76.65(9) . . ?
O46 Fe11 P2 125.75(7) . . ?
P5 Fe11 P2 106.11(4) . . ?
P9 Fe11 P2 78.25(3) 4_454 . ?
P4 Fe11 P2 110.49(3) 3_445 . ?
P12 Fe11 P2 101.12(3) . . ?
Fe8 Fe11 P2 54.25(2) 3_445 . ?
O17 Fe11 P2 126.47(6) . . ?
Fe4 Fe11 P2 154.46(3) 1_545 . ?
Na3 Fe11 P2 52.23(5) . . ?
O43 Fe12 O14 97.66(17) 3_455 . ?
O43 Fe12 O40 88.15(16) 3_455 . ?
O14 Fe12 O40 162.10(14) . . ?
O43 Fe12 O31 171.4(2) 3_455 . ?
O14 Fe12 O31 89.34(13) . . ?
O40 Fe12 O31 86.64(14) . . ?
O43 Fe12 O49 88.10(18) 3_455 . ?
O14 Fe12 O49 85.76(14) . . ?
O40 Fe12 O49 111.45(14) . . ?
O31 Fe12 O49 87.45(14) . . ?
O43 Fe12 O8 91.8(2) 3_455 . ?
O14 Fe12 O8 87.61(13) . . ?
O40 Fe12 O8 75.24(14) . . ?
O31 Fe12 O8 93.43(16) . . ?
O49 Fe12 O8 173.30(14) . . ?
O43 Fe12 Fe2 76.82(12) 3_455 . ?
O14 Fe12 Fe2 126.10(10) . . ?
O40 Fe12 Fe2 38.89(10) . . ?
O31 Fe12 Fe2 103.07(10) . . ?
O49 Fe12 Fe2 145.88(10) . . ?
O8 Fe12 Fe2 40.17(10) . . ?
O43 Fe12 Fe3 47.64(18) 3_455 4_464 ?
O14 Fe12 Fe3 124.27(9) . 4_464 ?
O40 Fe12 Fe3 71.73(10) . 4_464 ?
O31 Fe12 Fe3 124.00(10) . 4_464 ?
O49 Fe12 Fe3 56.89(10) . 4_464 ?
O8 Fe12 Fe3 127.07(12) . 4_464 ?
Fe2 Fe12 Fe3 91.40(3) . 4_464 ?
O43 Fe12 Fe11 74.01(13) 3_455 1_565 ?
O14 Fe12 Fe11 69.55(9) . 1_565 ?
O40 Fe12 Fe11 128.33(10) . 1_565 ?
O31 Fe12 Fe11 104.07(10) . 1_565 ?
O49 Fe12 Fe11 23.72(10) . 1_565 ?
O8 Fe12 Fe11 150.68(11) . 1_565 ?
Fe2 Fe12 Fe11 148.69(3) . 1_565 ?
Fe3 Fe12 Fe11 60.327(18) 4_464 1_565 ?
O43 Fe12 Na3 136.27(16) 3_455 . ?
O14 Fe12 Na3 77.14(10) . . ?
O40 Fe12 Na3 86.94(10) . . ?
O31 Fe12 Na3 50.21(10) . . ?
O49 Fe12 Na3 133.69(11) . . ?
O8 Fe12 Na3 45.05(12) . . ?
Fe2 Fe12 Na3 72.39(3) . . ?
Fe3 Fe12 Na3 158.56(4) 4_464 . ?
Fe11 Fe12 Na3 138.29(4) 1_565 . ?
O43 Fe12 O30 125.79(18) 3_455 3_454 ?
O14 Fe12 O30 35.78(10) . 3_454 ?
O40 Fe12 O30 128.97(11) . 3_454 ?
O31 Fe12 O30 62.65(10) . 3_454 ?
O49 Fe12 O30 106.98(11) . 3_454 ?
O8 Fe12 O30 67.74(12) . 3_454 ?
Fe2 Fe12 O30 106.66(5) . 3_454 ?
Fe3 Fe12 O30 159.21(5) 4_464 3_454 ?
Fe11 Fe12 O30 99.50(4) 1_565 3_454 ?
Na3 Fe12 O30 42.03(5) . 3_454 ?
O44 Fe13 O13 93.67(16) . 2_564 ?
O44 Fe13 O39 91.96(15) . 4_454 ?
O13 Fe13 O39 151.87(14) 2_564 4_454 ?
O44 Fe13 O50 98.16(16) . 2_564 ?
O13 Fe13 O50 87.97(13) 2_564 2_564 ?
O39 Fe13 O50 118.45(13) 4_454 2_564 ?
O44 Fe13 O32 175.00(15) . 4_454 ?
O13 Fe13 O32 89.44(14) 2_564 4_454 ?
O39 Fe13 O32 83.48(14) 4_454 4_454 ?
O50 Fe13 O32 85.85(13) 2_564 4_454 ?
O44 Fe13 O5 81.33(15) . 4_454 ?
O13 Fe13 O5 82.86(12) 2_564 4_454 ?
O39 Fe13 O5 70.78(12) 4_454 4_454 ?
O50 Fe13 O5 170.76(12) 2_564 4_454 ?
O32 Fe13 O5 95.19(12) 4_454 4_454 ?
O44 Fe13 O37 84.54(16) . 4_454 ?
O13 Fe13 O37 153.48(12) 2_564 4_454 ?
O39 Fe13 O37 54.57(12) 4_454 4_454 ?
O50 Fe13 O37 66.22(12) 2_564 4_454 ?
O32 Fe13 O37 94.42(12) 4_454 4_454 ?
O5 Fe13 O37 122.74(11) 4_454 4_454 ?
O44 Fe13 P9 90.72(13) . 4_454 ?
O13 Fe13 P9 175.35(10) 2_564 4_454 ?
O39 Fe13 P9 26.07(9) 4_454 4_454 ?
O50 Fe13 P9 92.92(10) 2_564 4_454 ?
O32 Fe13 P9 86.08(10) 4_454 4_454 ?
O5 Fe13 P9 96.31(8) 4_454 4_454 ?
O37 Fe13 P9 28.71(8) 4_454 4_454 ?
O44 Fe13 P3 101.62(12) . 2_564 ?
O13 Fe13 P3 23.42(9) 2_564 2_564 ?
O39 Fe13 P3 165.43(11) 4_454 2_564 ?
O50 Fe13 P3 65.20(9) 2_564 2_564 ?
O32 Fe13 P3 82.75(10) 4_454 2_564 ?
O5 Fe13 P3 105.78(8) 4_454 2_564 ?
O37 Fe13 P3 131.42(8) 4_454 2_564 ?
P9 Fe13 P3 156.00(4) 4_454 2_564 ?
O44 Fe13 P12 20.00(11) . . ?
O13 Fe13 P12 111.30(10) 2_564 . ?
O39 Fe13 P12 71.95(10) 4_454 . ?
O50 Fe13 P12 107.28(10) 2_564 . ?
O32 Fe13 P12 155.35(10) 4_454 . ?
O5 Fe13 P12 75.23(8) 4_454 . ?
O37 Fe13 P12 73.14(8) 4_454 . ?
P9 Fe13 P12 72.78(3) 4_454 . ?
P3 Fe13 P12 121.53(4) 2_564 . ?
O44 Fe13 Fe3 76.23(11) . 4_454 ?
O13 Fe13 Fe3 119.69(9) 2_564 4_454 ?
O39 Fe13 Fe3 36.06(9) 4_454 4_454 ?
O50 Fe13 Fe3 151.81(10) 2_564 4_454 ?
O32 Fe13 Fe3 98.83(10) 4_454 4_454 ?
O5 Fe13 Fe3 37.08(7) 4_454 4_454 ?
O37 Fe13 Fe3 85.66(7) 4_454 4_454 ?
P9 Fe13 Fe3 59.98(3) 4_454 4_454 ?
P3 Fe13 Fe3 142.84(3) 2_564 4_454 ?
P12 Fe13 Fe3 59.83(3) . 4_454 ?
O44 Fe13 P8 161.58(15) . 4_454 ?
O13 Fe13 P8 101.44(10) 2_564 4_454 ?
O39 Fe13 P8 79.69(10) 4_454 4_454 ?
O50 Fe13 P8 72.17(10) 2_564 4_454 ?
O32 Fe13 P8 18.76(9) 4_454 4_454 ?
O5 Fe13 P8 110.75(8) 4_454 4_454 ?
O37 Fe13 P8 77.23(8) 4_454 4_454 ?
P9 Fe13 P8 74.54(3) 4_454 4_454 ?
P3 Fe13 P8 88.71(3) 2_564 4_454 ?
P12 Fe13 P8 147.24(4) . 4_454 ?
Fe3 Fe13 P8 104.66(3) 4_454 4_454 ?
O44 Fe13 O6 122.62(15) . 2_564 ?
O13 Fe13 O6 64.90(11) 2_564 2_564 ?
O39 Fe13 O6 88.98(11) 4_454 2_564 ?
O50 Fe13 O6 130.67(11) 2_564 2_564 ?
O32 Fe13 O6 55.47(11) 4_454 2_564 ?
O5 Fe13 O6 45.40(9) 4_454 2_564 ?
O37 Fe13 O6 136.97(9) 4_454 2_564 ?
P9 Fe13 O6 111.32(6) 4_454 2_564 ?
P3 Fe13 O6 79.30(6) 2_564 2_564 ?
P12 Fe13 O6 120.51(6) . 2_564 ?
Fe3 Fe13 O6 71.72(6) 4_454 2_564 ?
P8 Fe13 O6 74.00(6) 4_454 2_564 ?
O44 Fe13 Mn 144.81(14) . 2_564 ?
O13 Fe13 Mn 53.35(10) 2_564 2_564 ?
O39 Fe13 Mn 111.71(10) 4_454 2_564 ?
O50 Fe13 Mn 93.02(10) 2_564 2_564 ?
O32 Fe13 Mn 37.13(9) 4_454 2_564 ?
O5 Fe13 Mn 82.45(7) 4_454 2_564 ?
O37 Fe13 Mn 130.25(8) 4_454 2_564 ?
P9 Fe13 Mn 122.02(3) 4_454 2_564 ?
P3 Fe13 Mn 53.79(3) 2_564 2_564 ?
P12 Fe13 Mn 154.77(4) . 2_564 ?
Fe3 Fe13 Mn 107.51(3) 4_454 2_564 ?
P8 Fe13 Mn 53.10(2) 4_454 2_564 ?
O6 Fe13 Mn 37.65(5) 2_564 2_564 ?
O44 Fe13 Na5 49.28(15) . 2_564 ?
O13 Fe13 Na5 65.03(11) 2_564 2_564 ?
O39 Fe13 Na5 99.03(11) 4_454 2_564 ?
O50 Fe13 Na5 132.28(11) 2_564 2_564 ?
O32 Fe13 Na5 129.35(11) 4_454 2_564 ?
O5 Fe13 Na5 41.66(9) 4_454 2_564 ?
O37 Fe13 Na5 128.18(9) 4_454 2_564 ?
P9 Fe13 Na5 117.18(6) 4_454 2_564 ?
P3 Fe13 Na5 86.10(6) 2_564 2_564 ?
P12 Fe13 Na5 55.53(5) . 2_564 ?
Fe3 Fe13 Na5 64.09(5) 4_454 2_564 ?
P8 Fe13 Na5 147.93(6) 4_454 2_564 ?
O6 Fe13 Na5 73.94(7) 2_564 2_564 ?
Mn Fe13 Na5 99.71(5) 2_564 2_564 ?
O44 Fe13 Fe5 105.31(14) . 4_464 ?
O13 Fe13 Fe5 120.12(9) 2_564 4_464 ?
O39 Fe13 Fe5 84.64(10) 4_454 4_464 ?
O50 Fe13 Fe5 34.13(9) 2_564 4_464 ?
O32 Fe13 Fe5 76.37(9) 4_454 4_464 ?
O5 Fe13 Fe5 154.87(8) 4_454 4_464 ?
O37 Fe13 Fe5 36.95(7) 4_454 4_464 ?
P9 Fe13 Fe5 59.92(3) 4_454 4_464 ?
P3 Fe13 Fe5 96.70(3) 2_564 4_464 ?
P12 Fe13 Fe5 102.60(3) . 4_464 ?
Fe3 Fe13 Fe5 119.90(3) 4_454 4_464 ?
P8 Fe13 Fe5 57.87(3) 4_454 4_464 ?
O6 Fe13 Fe5 131.83(6) 2_564 4_464 ?
Mn Fe13 Fe5 102.60(3) 2_564 4_464 ?
Na5 Fe13 Fe5 154.19(6) 2_564 4_464 ?
O9 Al1 O10 178.02(19) . 1_456 ?
O9 Al1 O26 88.73(15) . 1_455 ?
O10 Al1 O26 90.86(15) 1_456 1_455 ?
O9 Al1 O25 92.64(15) . 1_556 ?
O10 Al1 O25 87.83(15) 1_456 1_556 ?
O26 Al1 O25 177.73(19) 1_455 1_556 ?
O9 Al1 O20 87.15(15) . 1_455 ?
O10 Al1 O20 90.93(15) 1_456 1_455 ?
O26 Al1 O20 90.41(16) 1_455 1_455 ?
O25 Al1 O20 91.46(15) 1_556 1_455 ?
O9 Al1 O19 93.72(16) . 1_556 ?
O10 Al1 O19 88.21(15) 1_456 1_556 ?
O26 Al1 O19 91.01(15) 1_455 1_556 ?
O25 Al1 O19 87.11(16) 1_556 1_556 ?
O20 Al1 O19 178.35(19) 1_455 1_556 ?
O9 Al1 Na4 115.67(13) . 1_556 ?
O10 Al1 Na4 65.97(12) 1_456 1_556 ?
O26 Al1 Na4 131.18(12) 1_455 1_556 ?
O25 Al1 Na4 46.56(11) 1_556 1_556 ?
O20 Al1 Na4 129.85(12) 1_455 1_556 ?
O19 Al1 Na4 48.50(11) 1_556 1_556 ?
O9 Al1 Na2 68.34(14) . 1_455 ?
O10 Al1 Na2 110.01(14) 1_456 1_455 ?
O26 Al1 Na2 48.11(11) 1_455 1_455 ?
O25 Al1 Na2 134.13(13) 1_556 1_455 ?
O20 Al1 Na2 48.19(12) 1_455 1_455 ?
O19 Al1 Na2 133.45(13) 1_556 1_455 ?
Na4 Al1 Na2 175.91(13) 1_556 1_455 ?
O9 Al1 O30 129.09(13) . 1_455 ?
O10 Al1 O30 50.94(12) 1_456 1_455 ?
O26 Al1 O30 41.87(11) 1_455 1_455 ?
O25 Al1 O30 136.34(13) 1_556 1_455 ?
O20 Al1 O30 101.57(13) 1_455 1_455 ?
O19 Al1 O30 78.96(13) 1_556 1_455 ?
Na4 Al1 O30 96.74(8) 1_556 1_455 ?
Na2 Al1 O30 80.73(9) 1_455 1_455 ?
O9 Al1 O31 72.10(12) . 1_556 ?
O10 Al1 O31 109.01(13) 1_456 1_556 ?
O26 Al1 O31 150.60(13) 1_455 1_556 ?
O25 Al1 O31 29.05(11) 1_556 1_556 ?
O20 Al1 O31 110.08(12) 1_455 1_556 ?
O19 Al1 O31 68.91(12) 1_556 1_556 ?
Na4 Al1 O31 48.24(7) 1_556 1_556 ?
Na2 Al1 O31 134.89(10) 1_455 1_556 ?
O30 Al1 O31 143.17(9) 1_455 1_556 ?
O9 Al1 Fe1 116.04(11) . 3_455 ?
O10 Al1 Fe1 61.99(11) 1_456 3_455 ?
O26 Al1 Fe1 83.69(11) 1_455 3_455 ?
O25 Al1 Fe1 97.31(11) 1_556 3_455 ?
O20 Al1 Fe1 29.95(10) 1_455 3_455 ?
O19 Al1 Fe1 149.53(12) 1_556 3_455 ?
Na4 Al1 Fe1 116.38(7) 1_556 3_455 ?
Na2 Al1 Fe1 60.01(8) 1_455 3_455 ?
O30 Al1 Fe1 77.15(7) 1_455 3_455 ?
O31 Al1 Fe1 124.49(6) 1_556 3_455 ?
O9 Al1 Na3 65.97(11) . 1_556 ?
O10 Al1 Na3 115.99(12) 1_456 1_556 ?
O26 Al1 Na3 106.16(12) 1_455 1_556 ?
O25 Al1 Na3 72.82(12) 1_556 1_556 ?
O20 Al1 Na3 147.48(12) 1_455 1_556 ?
O19 Al1 Na3 32.52(11) 1_556 1_556 ?
Na4 Al1 Na3 56.48(7) 1_556 1_556 ?
Na2 Al1 Na3 127.36(10) 1_455 1_556 ?
O30 Al1 Na3 109.48(8) 1_455 1_556 ?
O31 Al1 Na3 45.96(6) 1_556 1_556 ?
Fe1 Al1 Na3 170.12(5) 3_455 1_556 ?
O5 P1 O6 107.49(19) 3_455 . ?
O5 P1 O4 112.58(19) 3_455 1_565 ?
O6 P1 O4 107.98(19) . 1_565 ?
O5 P1 O2 108.4(2) 3_455 1_455 ?
O6 P1 O2 110.61(18) . 1_455 ?
O4 P1 O2 109.74(19) 1_565 1_455 ?
O5 P1 Na5 49.08(15) 3_455 . ?
O6 P1 Na5 130.88(14) . . ?
O4 P1 Na5 120.71(15) 1_565 . ?
O2 P1 Na5 60.05(14) 1_455 . ?
O5 P1 Fe1 128.56(15) 3_455 1_565 ?
O6 P1 Fe1 36.91(12) . 1_565 ?
O4 P1 Fe1 71.62(14) 1_565 1_565 ?
O2 P1 Fe1 118.17(13) 1_455 1_565 ?
Na5 P1 Fe1 167.67(7) . 1_565 ?
O5 P1 Fe3 27.89(14) 3_455 3_455 ?
O6 P1 Fe3 107.68(13) . 3_455 ?
O4 P1 Fe3 86.82(13) 1_565 3_455 ?
O2 P1 Fe3 130.19(13) 1_455 3_455 ?
Na5 P1 Fe3 70.98(6) . 3_455 ?
Fe1 P1 Fe3 111.61(4) 1_565 3_455 ?
O5 P1 Fe13 39.43(14) 3_455 2_565 ?
O6 P1 Fe13 73.74(12) . 2_565 ?
O4 P1 Fe13 144.09(14) 1_565 2_565 ?
O2 P1 Fe13 102.47(13) 1_455 2_565 ?
Na5 P1 Fe13 63.48(6) . 2_565 ?
Fe1 P1 Fe13 106.76(3) 1_565 2_565 ?
Fe3 P1 Fe13 59.80(2) 3_455 2_565 ?
O8 P2 O3 110.4(2) . . ?
O8 P2 O1 114.8(2) . . ?
O3 P2 O1 109.87(19) . . ?
O8 P2 O7 106.2(3) . . ?
O3 P2 O7 110.4(2) . . ?
O1 P2 O7 104.9(2) . . ?
O8 P2 Fe2 40.50(17) . . ?
O3 P2 Fe2 94.61(13) . . ?
O1 P2 Fe2 151.95(14) . . ?
O7 P2 Fe2 77.87(18) . . ?
O8 P2 Na3 79.6(2) . . ?
O3 P2 Na3 51.42(14) . . ?
O1 P2 Na3 88.23(15) . . ?
O7 P2 Na3 161.13(17) . . ?
Fe2 P2 Na3 97.04(6) . . ?
O8 P2 Na5 81.62(19) . 4_564 ?
O3 P2 Na5 152.65(15) . 4_564 ?
O1 P2 Na5 85.01(15) . 4_564 ?
O7 P2 Na5 42.36(16) . 4_564 ?
Fe2 P2 Na5 78.66(6) . 4_564 ?
Na3 P2 Na5 155.09(8) . 4_564 ?
O8 P2 Fe11 92.62(16) . . ?
O3 P2 Fe11 26.81(13) . . ?
O1 P2 Fe11 136.67(14) . . ?
O7 P2 Fe11 98.07(16) . . ?
Fe2 P2 Fe11 68.47(3) . . ?
Na3 P2 Fe11 63.39(5) . . ?
Na5 P2 Fe11 133.94(6) 4_564 . ?
O8 P2 O30 86.69(19) . 3_454 ?
O3 P2 O30 93.73(14) . 3_454 ?
O1 P2 O30 42.03(15) . 3_454 ?
O7 P2 O30 145.59(17) . 3_454 ?
Fe2 P2 O30 125.63(6) . 3_454 ?
Na3 P2 O30 51.03(7) . 3_454 ?
Na5 P2 O30 111.84(7) 4_564 3_454 ?
Fe11 P2 O30 113.38(6) . 3_454 ?
O8 P2 O31 32.98(19) . . ?
O3 P2 O31 96.44(14) . . ?
O1 P2 O31 94.23(15) . . ?
O7 P2 O31 138.60(18) . . ?
Fe2 P2 O31 68.83(5) . . ?
Na3 P2 O31 51.15(6) . . ?
Na5 P2 O31 105.45(7) 4_564 . ?
Fe11 P2 O31 92.07(5) . . ?
O30 P2 O31 56.86(7) 3_454 . ?
O15 P3 O11 114.7(2) . . ?
O15 P3 O13 105.6(2) . . ?
O11 P3 O13 113.5(2) . . ?
O15 P3 O9 112.73(18) . . ?
O11 P3 O9 107.32(19) . . ?
O13 P3 O9 102.37(18) . . ?
O15 P3 Fe6 116.26(15) . . ?
O11 P3 Fe6 129.02(15) . . ?
O13 P3 Fe6 50.64(13) . . ?
O9 P3 Fe6 52.10(12) . . ?
O15 P3 Fe13 88.48(14) . 2_565 ?
O11 P3 Fe13 97.14(13) . 2_565 ?
O13 P3 Fe13 33.07(12) . 2_565 ?
O9 P3 Fe13 135.43(13) . 2_565 ?
Fe6 P3 Fe13 83.52(4) . 2_565 ?
O15 P3 Na3 24.22(15) . 1_556 ?
O11 P3 Na3 95.65(15) . 1_556 ?
O13 P3 Na3 129.00(15) . 1_556 ?
O9 P3 Na3 107.69(13) . 1_556 ?
Fe6 P3 Na3 133.33(6) . 1_556 ?
Fe13 P3 Na3 106.23(5) 2_565 1_556 ?
O15 P3 O31 42.37(14) . 1_556 ?
O11 P3 O31 146.21(15) . 1_556 ?
O13 P3 O31 98.62(15) . 1_556 ?
O9 P3 O31 73.95(13) . 1_556 ?
Fe6 P3 O31 79.40(6) . 1_556 ?
Fe13 P3 O31 104.93(6) 2_565 1_556 ?
Na3 P3 O31 53.94(7) 1_556 1_556 ?
O15 P3 Fe1 75.16(15) . . ?
O11 P3 Fe1 44.82(14) . . ?
O13 P3 Fe1 148.55(13) . . ?
O9 P3 Fe1 106.18(13) . . ?
Fe6 P3 Fe1 157.49(4) . . ?
Fe13 P3 Fe1 117.28(3) 2_565 . ?
Na3 P3 Fe1 52.52(5) 1_556 . ?
O31 P3 Fe1 101.67(6) 1_556 . ?
O12 P4 O14 114.05(19) . 3_545 ?
O12 P4 O16 110.3(2) . 3_545 ?
O14 P4 O16 109.05(19) 3_545 3_545 ?
O12 P4 O10 109.03(19) . . ?
O14 P4 O10 102.23(19) 3_545 . ?
O16 P4 O10 111.97(18) 3_545 . ?
O12 P4 Fe7 130.19(15) . . ?
O14 P4 Fe7 49.64(13) 3_545 . ?
O16 P4 Fe7 119.49(14) 3_545 . ?
O10 P4 Fe7 52.86(13) . . ?
O12 P4 Fe1 85.82(14) . 3_554 ?
O14 P4 Fe1 133.93(14) 3_545 3_554 ?
O16 P4 Fe1 27.95(13) 3_545 3_554 ?
O10 P4 Fe1 109.93(12) . 3_554 ?
Fe7 P4 Fe1 142.03(4) . 3_554 ?
O12 P4 Fe11 29.34(13) . 3 ?
O14 P4 Fe11 100.40(13) 3_545 3 ?
O16 P4 Fe11 92.67(14) 3_545 3 ?
O10 P4 Fe11 138.37(14) . 3 ?
Fe7 P4 Fe11 140.30(5) . 3 ?
Fe1 P4 Fe11 76.58(3) 3_554 3 ?
O12 P4 O30 166.04(16) . 1_554 ?
O14 P4 O30 67.54(14) 3_545 1_554 ?
O16 P4 O30 81.05(14) 3_545 1_554 ?
O10 P4 O30 57.95(14) . 1_554 ?
Fe7 P4 O30 39.33(6) . 1_554 ?
Fe1 P4 O30 102.96(7) 3_554 1_554 ?
Fe11 P4 O30 163.22(7) 3 1_554 ?
O12 P4 Ca 140.95(15) . 3_544 ?
O14 P4 Ca 82.95(14) 3_545 3_544 ?
O16 P4 Ca 32.40(13) 3_545 3_544 ?
O10 P4 Ca 100.41(13) . 3_544 ?
Fe7 P4 Ca 88.06(4) . 3_544 ?
Fe1 P4 Ca 59.83(3) 3_554 3_544 ?
Fe11 P4 Ca 116.75(4) 3 3_544 ?
O30 P4 Ca 52.11(7) 1_554 3_544 ?
O12 P4 O31 122.37(15) . 3_545 ?
O14 P4 O31 51.94(14) 3_545 3_545 ?
O16 P4 O31 57.96(14) 3_545 3_545 ?
O10 P4 O31 128.09(14) . 3_545 ?
Fe7 P4 O31 86.09(6) . 3_545 ?
Fe1 P4 O31 82.10(6) 3_554 3_545 ?
Fe11 P4 O31 93.27(6) 3 3_545 ?
O30 P4 O31 70.18(8) 1_554 3_545 ?
Ca P4 O31 41.21(6) 3_544 3_545 ?
O17 P5 O23 111.3(2) . . ?
O17 P5 O19 111.06(19) . . ?
O23 P5 O19 110.07(19) . . ?
O17 P5 O21 107.9(2) . 1_554 ?
O23 P5 O21 105.2(2) . 1_554 ?
O19 P5 O21 111.19(18) . 1_554 ?
O17 P5 Fe1 116.75(14) . 1_554 ?
O23 P5 Fe1 60.96(14) . 1_554 ?
O19 P5 Fe1 131.17(13) . 1_554 ?
O21 P5 Fe1 44.72(14) 1_554 1_554 ?
O17 P5 Na1 50.03(15) . 1_544 ?
O23 P5 Na1 126.07(15) . 1_544 ?
O19 P5 Na1 123.85(14) . 1_544 ?
O21 P5 Na1 58.04(15) 1_554 1_544 ?
Fe1 P5 Na1 82.75(6) 1_554 1_544 ?
O17 P5 Fe11 83.88(14) . . ?
O23 P5 Fe11 29.65(13) . . ?
O19 P5 Fe11 112.24(13) . . ?
O21 P5 Fe11 126.46(14) 1_554 . ?
Fe1 P5 Fe11 82.79(3) 1_554 . ?
Na1 P5 Fe11 115.78(6) 1_544 . ?
O17 P5 Na3 145.68(16) . . ?
O23 P5 Na3 42.05(14) . . ?
O19 P5 Na3 72.96(14) . . ?
O21 P5 Na3 101.48(15) 1_554 . ?
Fe1 P5 Na3 73.39(5) 1_554 . ?
Na1 P5 Na3 156.02(8) 1_544 . ?
Fe11 P5 Na3 64.22(5) . . ?
O17 P5 Na4 89.98(15) . . ?
O23 P5 Na4 89.89(15) . . ?
O19 P5 Na4 38.62(13) . . ?
O21 P5 Na4 149.80(14) 1_554 . ?
Fe1 P5 Na4 145.36(7) 1_554 . ?
Na1 P5 Na4 131.69(8) 1_544 . ?
Fe11 P5 Na4 78.44(5) . . ?
Na3 P5 Na4 72.27(7) . . ?
O17 P5 O30 51.04(15) . 1_454 ?
O23 P5 O30 162.08(15) . 1_454 ?
O19 P5 O30 82.41(14) . 1_454 ?
O21 P5 O30 80.90(15) 1_554 1_454 ?
Fe1 P5 O30 120.86(7) 1_554 1_454 ?
Na1 P5 O30 43.02(8) 1_544 1_454 ?
Fe11 P5 O30 134.30(6) . 1_454 ?
Na3 P5 O30 154.45(8) . 1_454 ?
Na4 P5 O30 92.76(8) . 1_454 ?
O22 P6 O20 111.83(19) . 3_445 ?
O22 P6 O18 109.5(2) . . ?
O20 P6 O18 110.49(18) 3_445 . ?
O22 P6 O24 108.8(2) . . ?
O20 P6 O24 106.44(19) 3_445 . ?
O18 P6 O24 109.73(19) . . ?
O22 P6 Fe1 93.36(14) . . ?
O20 P6 Fe1 80.49(13) 3_445 . ?
O18 P6 Fe1 147.23(15) . . ?
O24 P6 Fe1 38.59(12) . . ?
O22 P6 Na1 55.30(15) . 3_545 ?
O20 P6 Na1 123.04(14) 3_445 3_545 ?
O18 P6 Na1 54.58(14) . 3_545 ?
O24 P6 Na1 130.52(15) . 3_545 ?
Fe1 P6 Na1 144.91(7) . 3_545 ?
O22 P6 Na2 150.86(15) . 3_445 ?
O20 P6 Na2 39.19(13) 3_445 3_445 ?
O18 P6 Na2 89.45(14) . 3_445 ?
O24 P6 Na2 83.85(15) . 3_445 ?
Fe1 P6 Na2 80.29(8) . 3_445 ?
Na1 P6 Na2 134.69(10) 3_545 3_445 ?
O22 P6 Na3 38.47(14) . 1_556 ?
O20 P6 Na3 134.67(14) 3_445 1_556 ?
O18 P6 Na3 112.34(13) . 1_556 ?
O24 P6 Na3 72.11(14) . 1_556 ?
Fe1 P6 Na3 71.60(5) . 1_556 ?
Na1 P6 Na3 73.58(8) 3_545 1_556 ?
Na2 P6 Na3 151.68(10) 3_445 1_556 ?
O22 P6 O30 49.19(14) . 3_455 ?
O20 P6 O30 153.62(14) 3_445 3_455 ?
O18 P6 O30 68.72(13) . 3_455 ?
O24 P6 O30 98.10(14) . 3_455 ?
Fe1 P6 O30 115.02(6) . 3_455 ?
Na1 P6 O30 33.73(7) 3_545 3_455 ?
Na2 P6 O30 157.51(8) 3_445 3_455 ?
Na3 P6 O30 45.44(6) 1_556 3_455 ?
O31 P7 O29 107.9(2) . 1_554 ?
O31 P7 O27 113.24(19) . . ?
O29 P7 O27 109.30(19) 1_554 . ?
O31 P7 O25 112.31(19) . . ?
O29 P7 O25 111.25(18) 1_554 . ?
O27 P7 O25 102.79(18) . . ?
O31 P7 Mn 58.28(14) . 1_554 ?
O29 P7 Mn 49.81(14) 1_554 1_554 ?
O27 P7 Mn 131.30(14) . 1_554 ?
O25 P7 Mn 125.30(13) . 1_554 ?
O31 P7 Na1 137.25(16) . 1_554 ?
O29 P7 Na1 57.18(15) 1_554 1_554 ?
O27 P7 Na1 53.29(14) . 1_554 ?
O25 P7 Na1 110.37(14) . 1_554 ?
Mn P7 Na1 98.15(8) 1_554 1_554 ?
O31 P7 Na4 72.66(15) . . ?
O29 P7 Na4 144.30(14) 1_554 . ?
O27 P7 Na4 102.43(14) . . ?
O25 P7 Na4 43.99(13) . . ?
Mn P7 Na4 116.67(6) 1_554 . ?
Na1 P7 Na4 144.53(9) 1_554 . ?
O31 P7 Na3 40.75(14) . . ?
O29 P7 Na3 96.86(14) 1_554 . ?
O27 P7 Na3 149.37(14) . . ?
O25 P7 Na3 81.36(13) . . ?
Mn P7 Na3 57.30(4) 1_554 . ?
Na1 P7 Na3 153.70(8) 1_554 . ?
Na4 P7 Na3 59.45(6) . . ?
O31 P7 Fe1 79.48(14) . 1_564 ?
O29 P7 Fe1 48.91(13) 1_554 1_564 ?
O27 P7 Fe1 85.86(13) . 1_564 ?
O25 P7 Fe1 160.14(13) . 1_564 ?
Mn P7 Fe1 46.22(2) 1_554 1_564 ?
Na1 P7 Fe1 60.56(7) 1_554 1_564 ?
Na4 P7 Fe1 152.01(6) . 1_564 ?
Na3 P7 Fe1 100.38(4) . 1_564 ?
O30 P8 O32 109.6(2) . . ?
O30 P8 O28 111.32(19) . . ?
O32 P8 O28 111.93(19) . . ?
O30 P8 O26 112.98(19) . . ?
O32 P8 O26 108.72(19) . . ?
O28 P8 O26 102.10(18) . . ?
O30 P8 Na1 60.32(16) . 1_645 ?
O32 P8 Na1 139.62(16) . 1_645 ?
O28 P8 Na1 52.36(14) . 1_645 ?
O26 P8 Na1 110.98(14) . 1_645 ?
O30 P8 Na2 142.35(15) . . ?
O32 P8 Na2 63.69(16) . . ?
O28 P8 Na2 104.95(14) . . ?
O26 P8 Na2 47.52(14) . . ?
Na1 P8 Na2 149.02(11) 1_645 . ?
O30 P8 Fe13 123.42(15) . 4 ?
O32 P8 Fe13 27.82(13) . 4 ?
O28 P8 Fe13 84.11(13) . 4 ?
O26 P8 Fe13 116.15(13) . 4 ?
Na1 P8 Fe13 121.00(7) 1_645 4 ?
Na2 P8 Fe13 69.24(7) . 4 ?
O30 P8 Na3 37.81(14) . 3_546 ?
O32 P8 Na3 85.72(15) . 3_546 ?
O28 P8 Na3 95.52(13) . 3_546 ?
O26 P8 Na3 150.57(13) . 3_546 ?
Na1 P8 Na3 62.73(8) 1_645 3_546 ?
Na2 P8 Na3 147.72(9) . 3_546 ?
Fe13 P8 Na3 88.75(4) 4 3_546 ?
O35 P9 O33 109.7(2) 2_565 . ?
O35 P9 O37 111.5(2) 2_565 . ?
O33 P9 O37 110.3(2) . . ?
O35 P9 O39 110.2(2) 2_565 . ?
O33 P9 O39 108.0(2) . . ?
O37 P9 O39 107.1(2) . . ?
O35 P9 Na2 119.34(17) 2_565 . ?
O33 P9 Na2 58.03(16) . . ?
O37 P9 Na2 128.81(17) . . ?
O39 P9 Na2 50.39(16) . . ?
O35 P9 Fe13 130.70(16) 2_565 4 ?
O33 P9 Fe13 115.76(14) . 4 ?
O37 P9 Fe13 69.72(18) . 4 ?
O39 P9 Fe13 37.90(14) . 4 ?
Na2 P9 Fe13 73.25(8) . 4 ?
O35 P9 Fe3 81.04(16) 2_565 . ?
O33 P9 Fe3 114.29(15) . . ?
O37 P9 Fe3 125.64(18) . . ?
O39 P9 Fe3 29.80(14) . . ?
Na2 P9 Fe3 60.79(7) . . ?
Fe13 P9 Fe3 63.87(3) 4 . ?
O35 P9 Fe2 87.02(15) 2_565 4 ?
O33 P9 Fe2 136.69(15) . 4 ?
O37 P9 Fe2 29.41(14) . 4 ?
O39 P9 Fe2 102.50(15) . 4 ?
Na2 P9 Fe2 145.97(9) . 4 ?
Fe13 P9 Fe2 73.10(3) 4 4 ?
Fe3 P9 Fe2 107.52(4) . 4 ?
O35 P9 Fe11 22.54(14) 2_565 4 ?
O33 P9 Fe11 132.02(14) . 4 ?
O37 P9 Fe11 96.54(15) . 4 ?
O39 P9 Fe11 100.63(14) . 4 ?
Na2 P9 Fe11 129.40(6) . 4 ?
Fe13 P9 Fe11 110.57(4) 4 4 ?
Fe3 P9 Fe11 75.62(3) . 4 ?
Fe2 P9 Fe11 68.64(3) 4 4 ?
O35 P9 K1 50.92(15) 2_565 2_565 ?
O33 P9 K1 59.63(14) . 2_565 ?
O37 P9 K1 136.64(18) . 2_565 ?
O39 P9 K1 116.15(15) . 2_565 ?
Na2 P9 K1 84.19(9) . 2_565 ?
Fe13 P9 K1 153.58(5) 4 2_565 ?
Fe3 P9 K1 93.33(4) . 2_565 ?
Fe2 P9 K1 129.68(5) 4 2_565 ?
Fe11 P9 K1 73.42(5) 4 2_565 ?
O36 P10 O34 110.1(2) . . ?
O36 P10 O38 111.3(2) . . ?
O34 P10 O38 109.4(2) . . ?
O36 P10 O40 109.7(2) . . ?
O34 P10 O40 107.1(2) . . ?
O38 P10 O40 109.1(2) . . ?
O36 P10 Na4 114.04(16) . . ?
O34 P10 Na4 55.69(15) . . ?
O38 P10 Na4 134.60(15) . . ?
O40 P10 Na4 52.94(15) . . ?
O36 P10 Fe3 89.33(15) . 4_464 ?
O34 P10 Fe3 137.39(14) . 4_464 ?
O38 P10 Fe3 29.25(13) . 4_464 ?
O40 P10 Fe3 100.72(15) . 4_464 ?
Na4 P10 Fe3 148.61(7) . 4_464 ?
O36 P10 Fe2 77.96(16) . . ?
O34 P10 Fe2 114.69(14) . . ?
O38 P10 Fe2 128.04(16) . . ?
O40 P10 Fe2 32.15(14) . . ?
Na4 P10 Fe2 62.08(6) . . ?
Fe3 P10 Fe2 106.12(4) 4_464 . ?
O36 P10 K1 53.46(15) . 1_455 ?
O34 P10 K1 56.98(13) . 1_455 ?
O38 P10 K1 132.47(16) . 1_455 ?
O40 P10 K1 118.38(16) . 1_455 ?
Na4 P10 K1 79.18(7) . 1_455 ?
Fe3 P10 K1 132.13(5) 4_464 1_455 ?
Fe2 P10 K1 95.17(4) . 1_455 ?
O36 P10 O31 152.38(17) . . ?
O34 P10 O31 80.84(14) . . ?
O38 P10 O31 87.10(15) . . ?
O40 P10 O31 43.09(15) . . ?
Na4 P10 O31 50.36(7) . . ?
Fe3 P10 O31 99.39(6) 4_464 . ?
Fe2 P10 O31 74.44(6) . . ?
K1 P10 O31 127.80(7) 1_455 . ?
O43 P11 O41 109.2(2) 2_565 . ?
O43 P11 O45 111.9(2) 2_565 . ?
O41 P11 O45 107.8(2) . . ?
O43 P11 O47 109.4(3) 2_565 . ?
O41 P11 O47 110.4(2) . . ?
O45 P11 O47 108.1(2) . . ?
O43 P11 Na2 112.1(2) 2_565 . ?
O41 P11 Na2 60.34(17) . . ?
O45 P11 Na2 135.78(15) . . ?
O47 P11 Na2 52.16(16) . . ?
O43 P11 Na5 81.9(3) 2_565 1_655 ?
O41 P11 Na5 58.32(17) . 1_655 ?
O45 P11 Na5 72.15(16) . 1_655 ?
O47 P11 Na5 166.94(17) . 1_655 ?
Na2 P11 Na5 118.20(11) . 1_655 ?
O43 P11 Fe3 71.3(2) 2_565 . ?
O41 P11 Fe3 118.81(16) . . ?
O45 P11 Fe3 129.34(16) . . ?
O47 P11 Fe3 38.57(16) . . ?
Na2 P11 Fe3 63.69(7) . . ?
Na5 P11 Fe3 150.36(7) 1_655 . ?
O43 P11 Fe2 85.99(18) 2_565 4_565 ?
O41 P11 Fe2 130.85(16) . 4_565 ?
O45 P11 Fe2 28.75(14) . 4_565 ?
O47 P11 Fe2 107.37(15) . 4_565 ?
Na2 P11 Fe2 155.52(9) . 4_565 ?
Na5 P11 Fe2 79.30(7) 1_655 4_565 ?
Fe3 P11 Fe2 110.34(4) . 4_565 ?
O43 P11 K1 52.23(18) 2_565 2_565 ?
O41 P11 K1 57.22(14) . 2_565 ?
O45 P11 K1 130.36(16) . 2_565 ?
O47 P11 K1 121.52(16) . 2_565 ?
Na2 P11 K1 81.81(8) . 2_565 ?
Na5 P11 K1 59.83(6) 1_655 2_565 ?
Fe3 P11 K1 92.94(4) . 2_565 ?
Fe2 P11 K1 122.67(5) 4_565 2_565 ?
O44 P12 O42 108.9(2) . . ?
O44 P12 O46 109.7(2) . . ?
O42 P12 O46 110.6(2) . . ?
O44 P12 O48 110.6(3) . . ?
O42 P12 O48 108.3(2) . . ?
O46 P12 O48 108.5(2) . . ?
O44 P12 Na4 113.13(17) . . ?
O42 P12 Na4 54.65(15) . . ?
O46 P12 Na4 137.14(15) . . ?
O48 P12 Na4 55.54(15) . . ?
O44 P12 Na5 56.9(2) . 2_564 ?
O42 P12 Na5 82.13(15) . 2_564 ?
O46 P12 Na5 74.17(16) . 2_564 ?
O48 P12 Na5 166.59(17) . 2_564 ?
Na4 P12 Na5 131.38(9) . 2_564 ?
O44 P12 Fe2 77.3(2) . . ?
O42 P12 Fe2 116.20(14) . . ?
O46 P12 Fe2 127.02(16) . . ?
O48 P12 Fe2 33.77(16) . . ?
Na4 P12 Fe2 64.56(6) . . ?
Na5 P12 Fe2 134.21(7) 2_564 . ?
O44 P12 Fe13 27.61(15) . . ?
O42 P12 Fe13 135.66(15) . . ?
O46 P12 Fe13 89.77(13) . . ?
O48 P12 Fe13 101.01(15) . . ?
Na4 P12 Fe13 130.09(6) . . ?
Na5 P12 Fe13 65.67(6) 2_564 . ?
Fe2 P12 Fe13 73.70(3) . . ?
O44 P12 Fe3 85.01(16) . 4_454 ?
O42 P12 Fe3 133.41(14) . 4_454 ?
O46 P12 Fe3 27.87(13) . 4_454 ?
O48 P12 Fe3 107.31(15) . 4_454 ?
Na4 P12 Fe3 157.87(7) . 4_454 ?
Na5 P12 Fe3 68.65(6) 2_564 4_454 ?
Fe2 P12 Fe3 110.16(4) . 4_454 ?
Fe13 P12 Fe3 62.30(3) . 4_454 ?
O44 P12 Fe11 131.60(18) . . ?
O42 P12 Fe11 117.06(14) . . ?
O46 P12 Fe11 67.74(15) . . ?
O48 P12 Fe11 41.37(16) . . ?
Na4 P12 Fe11 83.68(6) . . ?
Na5 P12 Fe11 141.34(7) 2_564 . ?
Fe2 P12 Fe11 69.88(3) . . ?
Fe13 P12 Fe11 106.99(4) . . ?
Fe3 P12 Fe11 74.54(3) 4_454 . ?
O44 P12 K1 51.55(16) . 1_455 ?
O42 P12 K1 57.93(14) . 1_455 ?
O46 P12 K1 132.86(16) . 1_455 ?
O48 P12 K1 118.51(16) . 1_455 ?
Na4 P12 K1 77.59(7) . 1_455 ?
Na5 P12 K1 59.42(6) 2_564 1_455 ?
Fe2 P12 K1 93.69(4) . 1_455 ?
Fe13 P12 K1 79.10(5) . 1_455 ?
Fe3 P12 K1 124.54(5) 4_454 1_455 ?
Fe11 P12 K1 159.21(5) . 1_455 ?
P2 O1 Fe7 131.2(2) . 3_455 ?
P2 O1 Fe4 129.4(2) . 3_545 ?
Fe7 O1 Fe4 96.97(13) 3_455 3_545 ?
P2 O1 O30 118.82(19) . 3_454 ?
Fe7 O1 O30 43.16(9) 3_455 3_454 ?
Fe4 O1 O30 106.34(14) 3_545 3_454 ?
P2 O1 Na3 65.50(13) . . ?
Fe7 O1 Na3 96.49(13) 3_455 . ?
Fe4 O1 Na3 131.90(14) 3_545 . ?
O30 O1 Na3 58.53(9) 3_454 . ?
P1 O2 Fe6 118.54(18) 1_655 1_655 ?
P1 O2 Fe5 146.6(2) 1_655 . ?
Fe6 O2 Fe5 93.64(12) 1_655 . ?
P1 O2 Na5 89.04(16) 1_655 1_655 ?
Fe6 O2 Na5 86.64(14) 1_655 1_655 ?
Fe5 O2 Na5 102.47(14) . 1_655 ?
P1 O2 Fe1 42.02(10) 1_655 1_665 ?
Fe6 O2 Fe1 104.87(11) 1_655 1_665 ?
Fe5 O2 Fe1 124.87(12) . 1_665 ?
Na5 O2 Fe1 129.58(12) 1_655 1_665 ?
P2 O3 Fe8 119.48(19) . 3_445 ?
P2 O3 Fe11 135.99(19) . . ?
Fe8 O3 Fe11 99.43(13) 3_445 . ?
P2 O3 Na3 100.02(17) . . ?
Fe8 O3 Na3 96.31(13) 3_445 . ?
Fe11 O3 Na3 94.92(13) . . ?
P2 O3 Fe2 60.07(11) . . ?
Fe8 O3 Fe2 163.92(14) 3_445 . ?
Fe11 O3 Fe2 76.78(9) . . ?
Na3 O3 Fe2 99.57(11) . . ?
P1 O4 Fe9 120.05(19) 1_545 . ?
P1 O4 Fe10 134.5(2) 1_545 . ?
Fe9 O4 Fe10 100.77(13) . . ?
P1 O4 Fe1 78.90(14) 1_545 . ?
Fe9 O4 Fe1 86.17(11) . . ?
Fe10 O4 Fe1 85.13(11) . . ?
P1 O4 Fe3 67.67(12) 1_545 3_445 ?
Fe9 O4 Fe3 166.06(15) . 3_445 ?
Fe10 O4 Fe3 77.21(9) . 3_445 ?
Fe1 O4 Fe3 107.25(10) . 3_445 ?
P1 O5 Fe3 131.9(2) 3_545 . ?
P1 O5 Na5 101.07(19) 3_545 3_545 ?
Fe3 O5 Na5 113.22(16) . 3_545 ?
P1 O5 Fe13 118.38(19) 3_545 4 ?
Fe3 O5 Fe13 94.49(13) . 4 ?
Na5 O5 Fe13 90.90(14) 3_545 4 ?
P1 O6 Fe1 116.45(18) . 1_565 ?
P1 O6 Mn 140.48(19) . . ?
Fe1 O6 Mn 101.29(13) 1_565 . ?
P1 O6 Fe13 81.11(13) . 2_565 ?
Fe1 O6 Fe13 148.72(14) 1_565 2_565 ?
Mn O6 Fe13 71.53(8) . 2_565 ?
P1 O6 Fe3 51.11(10) . 3_455 ?
Fe1 O6 Fe3 115.63(12) 1_565 3_455 ?
Mn O6 Fe3 122.46(11) . 3_455 ?
Fe13 O6 Fe3 53.74(5) 2_565 3_455 ?
P2 O7 Na5 111.0(2) . 4_564 ?
P2 O7 Fe2 72.44(18) . . ?
Na5 O7 Fe2 92.99(16) 4_564 . ?
P2 O7 Fe3 122.2(2) . 2_564 ?
Na5 O7 Fe3 68.56(13) 4_564 2_564 ?
Fe2 O7 Fe3 159.21(13) . 2_564 ?
P2 O7 Fe11 59.28(14) . . ?
Na5 O7 Fe11 153.3(2) 4_564 . ?
Fe2 O7 Fe11 60.67(8) . . ?
Fe3 O7 Fe11 138.17(13) 2_564 . ?
P2 O8 Fe2 112.9(2) . . ?
P2 O8 Fe12 148.1(2) . . ?
Fe2 O8 Fe12 96.51(15) . . ?
P2 O8 Na3 73.19(18) . . ?
Fe2 O8 Na3 118.17(17) . . ?
Fe12 O8 Na3 104.40(17) . . ?
P2 O8 O31 132.5(3) . . ?
Fe2 O8 O31 105.61(16) . . ?
Fe12 O8 O31 41.36(10) . . ?
Na3 O8 O31 64.45(12) . . ?
P2 O8 Fe11 65.04(14) . . ?
Fe2 O8 Fe11 69.32(10) . . ?
Fe12 O8 Fe11 141.64(17) . . ?
Na3 O8 Fe11 58.33(8) . . ?
O31 O8 Fe11 106.39(13) . . ?
P3 O9 Al1 139.9(2) . . ?
P3 O9 Fe6 93.56(15) . . ?
Al1 O9 Fe6 122.71(16) . . ?
P3 O9 Na2 127.74(18) . 1_455 ?
Al1 O9 Na2 76.67(13) . 1_455 ?
Fe6 O9 Na2 84.67(11) . 1_455 ?
P3 O9 O31 83.36(14) . 1_556 ?
Al1 O9 O31 80.84(12) . 1_556 ?
Fe6 O9 O31 89.35(11) . 1_556 ?
Na2 O9 O31 148.56(13) 1_455 1_556 ?
P4 O10 Al1 142.1(2) . 1_654 ?
P4 O10 Fe7 93.30(15) . . ?
Al1 O10 Fe7 121.63(16) 1_654 . ?
P4 O10 O30 94.75(17) . 1_554 ?
Al1 O10 O30 98.47(15) 1_654 1_554 ?
Fe7 O10 O30 47.78(9) . 1_554 ?
P4 O10 Na4 122.82(17) . 1_655 ?
Al1 O10 Na4 78.08(13) 1_654 1_655 ?
Fe7 O10 Na4 85.25(11) . 1_655 ?
O30 O10 Na4 122.73(14) 1_554 1_655 ?
P4 O10 Fe1 49.18(10) . 3_554 ?
Al1 O10 Fe1 94.08(12) 1_654 3_554 ?
Fe7 O10 Fe1 128.68(12) . 3_554 ?
O30 O10 Fe1 95.47(11) 1_554 3_554 ?
Na4 O10 Fe1 141.64(11) 1_655 3_554 ?
P3 O11 Fe9 122.63(19) . . ?
P3 O11 Fe10 132.56(19) . . ?
Fe9 O11 Fe10 104.30(14) . . ?
P3 O11 Fe1 118.18(17) . . ?
Fe9 O11 Fe1 69.14(9) . . ?
Fe10 O11 Fe1 70.22(9) . . ?
P3 O11 Fe13 59.25(11) . 2_565 ?
Fe9 O11 Fe13 159.46(15) . 2_565 ?
Fe10 O11 Fe13 79.56(9) . 2_565 ?
Fe1 O11 Fe13 129.97(9) . 2_565 ?
P3 O11 Na3 61.93(13) . 1_556 ?
Fe9 O11 Na3 110.06(13) . 1_556 ?
Fe10 O11 Na3 97.72(12) . 1_556 ?
Fe1 O11 Na3 58.00(6) . 1_556 ?
Fe13 O11 Na3 89.05(8) 2_565 1_556 ?
P4 O12 Fe8 121.85(19) . . ?
P4 O12 Fe11 130.7(2) . 3 ?
Fe8 O12 Fe11 105.55(14) . 3 ?
P4 O12 Fe1 68.74(13) . 3_554 ?
Fe8 O12 Fe1 102.59(12) . 3_554 ?
Fe11 O12 Fe1 89.56(11) 3 3_554 ?
P4 O12 Na3 126.76(17) . 3 ?
Fe8 O12 Na3 61.75(9) . 3 ?
Fe11 O12 Na3 63.80(9) 3 3 ?
Fe1 O12 Na3 59.79(7) 3_554 3 ?
P3 O13 Fe13 123.51(19) . 2_565 ?
P3 O13 Fe6 95.14(16) . . ?
Fe13 O13 Fe6 140.75(17) 2_565 . ?
P4 O14 Fe12 128.2(2) 3_455 . ?
P4 O14 Fe7 97.15(16) 3_455 3_455 ?
Fe12 O14 Fe7 133.43(16) . 3_455 ?
P4 O14 O31 104.19(18) 3_455 . ?
Fe12 O14 O31 46.30(10) . . ?
Fe7 O14 O31 120.02(15) 3_455 . ?
P4 O14 O30 85.46(15) 3_455 3_454 ?
Fe12 O14 O30 121.21(15) . 3_454 ?
Fe7 O14 O30 43.19(9) 3_455 3_454 ?
O31 O14 O30 83.22(12) . 3_454 ?
P4 O14 Fe11 57.07(11) 3_455 1_565 ?
Fe12 O14 Fe11 80.68(10) . 1_565 ?
Fe7 O14 Fe11 142.44(13) 3_455 1_565 ?
O31 O14 Fe11 94.38(11) . 1_565 ?
O30 O14 Fe11 140.79(12) 3_454 1_565 ?
P3 O15 Na3 139.6(2) . 1_556 ?
P3 O15 Mn 105.14(19) . . ?
Na3 O15 Mn 113.70(15) 1_556 . ?
P3 O15 O31 118.19(19) . 1_556 ?
Na3 O15 O31 79.40(13) 1_556 1_556 ?
Mn O15 O31 53.06(10) . 1_556 ?
P3 O15 O30 147.3(2) . 3_455 ?
Na3 O15 O30 67.55(12) 1_556 3_455 ?
Mn O15 O30 60.54(10) . 3_455 ?
O31 O15 O30 78.41(12) 1_556 3_455 ?
P3 O15 Fe13 66.37(13) . 2_565 ?
Na3 O15 Fe13 138.16(15) 1_556 2_565 ?
Mn O15 Fe13 69.02(9) . 2_565 ?
O31 O15 Fe13 121.44(13) 1_556 2_565 ?
O30 O15 Fe13 80.93(10) 3_455 2_565 ?
P4 O16 Fe1 131.4(2) 3_455 1_564 ?
P4 O16 Mn 126.01(19) 3_455 1_554 ?
Fe1 O16 Mn 101.48(13) 1_564 1_554 ?
P4 O16 O31 97.39(16) 3_455 . ?
Fe1 O16 O31 122.36(15) 1_564 . ?
Mn O16 O31 52.19(9) 1_554 . ?
P4 O16 O30 72.92(14) 3_455 3_454 ?
Fe1 O16 O30 138.97(15) 1_564 3_454 ?
Mn O16 O30 57.82(9) 1_554 3_454 ?
O31 O16 O30 75.36(11) . 3_454 ?
P4 O16 Fe11 63.10(12) 3_455 1_565 ?
Fe1 O16 Fe11 84.75(10) 1_564 1_565 ?
Mn O16 Fe11 145.04(13) 1_554 1_565 ?
O31 O16 Fe11 95.28(10) . 1_565 ?
O30 O16 Fe11 133.48(11) 3_454 1_565 ?
P5 O17 Fe7 118.34(19) . 1_455 ?
P5 O17 Fe4 140.4(2) . 1_545 ?
Fe7 O17 Fe4 95.99(13) 1_455 1_545 ?
P5 O17 Na1 102.86(18) . 1_544 ?
Fe7 O17 Na1 96.72(15) 1_455 1_544 ?
Fe4 O17 Na1 91.26(13) 1_545 1_544 ?
P5 O17 O30 105.12(18) . 1_454 ?
Fe7 O17 O30 46.48(10) 1_455 1_454 ?
Fe4 O17 O30 113.17(15) 1_545 1_454 ?
Na1 O17 O30 54.91(12) 1_544 1_454 ?
P5 O17 Fe11 70.50(14) . . ?
Fe7 O17 Fe11 128.14(14) 1_455 . ?
Fe4 O17 Fe11 72.81(10) 1_545 . ?
Na1 O17 Fe11 132.97(14) 1_544 . ?
O30 O17 Fe11 171.15(14) 1_454 . ?
P5 O17 Fe1 42.19(10) . 1_554 ?
Fe7 O17 Fe1 153.96(14) 1_455 1_554 ?
Fe4 O17 Fe1 109.14(12) 1_545 1_554 ?
Na1 O17 Fe1 76.56(11) 1_544 1_554 ?
O30 O17 Fe1 114.07(12) 1_454 1_554 ?
Fe11 O17 Fe1 68.22(6) . 1_554 ?
P6 O18 Fe6 117.30(18) . 3_545 ?
P6 O18 Fe5 145.2(2) . 3_445 ?
Fe6 O18 Fe5 95.19(13) 3_545 3_445 ?
P6 O18 Na1 96.96(17) . 3_545 ?
Fe6 O18 Na1 96.24(15) 3_545 3_545 ?
Fe5 O18 Na1 91.24(12) 3_445 3_545 ?
P5 O19 Al1 139.3(2) . 1_554 ?
P5 O19 Na4 117.26(18) . . ?
Al1 O19 Na4 94.06(15) 1_554 . ?
P5 O19 Na3 80.11(14) . . ?
Al1 O19 Na3 129.07(16) 1_554 . ?
Na4 O19 Na3 88.16(13) . . ?
P5 O19 O30 73.81(14) . 1_454 ?
Al1 O19 O30 71.36(12) 1_554 1_454 ?
Na4 O19 O30 109.66(14) . 1_454 ?
Na3 O19 O30 153.04(13) . 1_454 ?
P5 O19 O31 135.86(17) . . ?
Al1 O19 O31 83.19(13) 1_554 . ?
Na4 O19 O31 53.30(10) . . ?
Na3 O19 O31 58.17(9) . . ?
O30 O19 O31 148.79(12) 1_454 . ?
P5 O19 Fe1 32.21(9) . 1_554 ?
Al1 O19 Fe1 131.19(14) 1_554 1_554 ?
Na4 O19 Fe1 134.32(13) . 1_554 ?
Na3 O19 Fe1 60.36(7) . 1_554 ?
O30 O19 Fe1 93.22(9) 1_454 1_554 ?
O31 O19 Fe1 117.44(10) . 1_554 ?
P6 O20 Al1 140.6(2) 3 1_655 ?
P6 O20 Na2 116.64(18) 3 . ?
Al1 O20 Na2 95.03(16) 1_655 . ?
P6 O20 Fe1 70.47(12) 3 3 ?
Al1 O20 Fe1 132.32(15) 1_655 3 ?
Na2 O20 Fe1 95.46(14) . 3 ?
P5 O21 Fe1 103.24(19) 1_556 . ?
P5 O21 Fe9 131.0(2) 1_556 . ?
Fe1 O21 Fe9 114.65(16) . . ?
P5 O21 Na1 93.58(17) 1_556 1_545 ?
Fe1 O21 Na1 113.11(15) . 1_545 ?
Fe9 O21 Na1 98.61(15) . 1_545 ?
P5 O21 O30 74.80(15) 1_556 1_455 ?
Fe1 O21 O30 154.88(16) . 1_455 ?
Fe9 O21 O30 82.39(12) . 1_455 ?
Na1 O21 O30 43.29(10) 1_545 1_455 ?
P5 O21 Na3 55.80(13) 1_556 1_556 ?
Fe1 O21 Na3 68.27(11) . 1_556 ?
Fe9 O21 Na3 110.87(13) . 1_556 ?
Na1 O21 Na3 146.90(13) 1_545 1_556 ?
O30 O21 Na3 124.81(11) 1_455 1_556 ?
P6 O22 Fe8 130.9(2) . 3_446 ?
P6 O22 Na3 117.9(2) . 1_556 ?
Fe8 O22 Na3 102.54(14) 3_446 1_556 ?
P6 O22 Na1 96.33(17) . 3_545 ?
Fe8 O22 Na1 100.55(15) 3_446 3_545 ?
Na3 O22 Na1 103.20(15) 1_556 3_545 ?
P6 O22 Fe1 60.16(12) . . ?
Fe8 O22 Fe1 107.04(13) 3_446 . ?
Na3 O22 Fe1 77.69(11) 1_556 . ?
Na1 O22 Fe1 151.56(14) 3_545 . ?
P6 O22 O30 112.59(16) . 3_455 ?
Fe8 O22 O30 111.51(13) 3_446 3_455 ?
Na3 O22 O30 59.40(11) 1_556 3_455 ?
Na1 O22 O30 43.94(10) 3_545 3_455 ?
Fe1 O22 O30 126.78(11) . 3_455 ?
P6 O22 Fe11 123.83(17) . 1_556 ?
Fe8 O22 Fe11 55.80(8) 3_446 1_556 ?
Na3 O22 Fe11 59.16(9) 1_556 1_556 ?
Na1 O22 Fe11 139.82(13) 3_545 1_556 ?
Fe1 O22 Fe11 65.34(6) . 1_556 ?
O30 O22 Fe11 109.82(9) 3_455 1_556 ?
P5 O23 Fe11 129.6(2) . . ?
P5 O23 Na3 112.93(19) . . ?
Fe11 O23 Na3 101.65(15) . . ?
P5 O23 Fe1 86.70(16) . 1_554 ?
Fe11 O23 Fe1 124.32(15) . 1_554 ?
Na3 O23 Fe1 98.03(14) . 1_554 ?
P6 O24 Fe1 112.49(18) . . ?
P6 O24 Fe10 127.86(19) . . ?
Fe1 O24 Fe10 115.43(16) . . ?
P6 O24 Na3 80.78(15) . 1_556 ?
Fe1 O24 Na3 86.86(12) . 1_556 ?
Fe10 O24 Na3 120.52(13) . 1_556 ?
P7 O25 Al1 137.4(2) . 1_554 ?
P7 O25 Na4 107.79(18) . . ?
Al1 O25 Na4 96.43(15) 1_554 . ?
P7 O25 Fe8 95.48(15) . 1_455 ?
Al1 O25 Fe8 117.34(16) 1_554 1_455 ?
Na4 O25 Fe8 94.64(13) . 1_455 ?
P7 O25 O31 33.49(11) . . ?
Al1 O25 O31 129.89(18) 1_554 . ?
Na4 O25 O31 77.76(14) . . ?
Fe8 O25 O31 112.74(14) 1_455 . ?
P8 O26 Al1 139.8(2) . 1_655 ?
P8 O26 Fe9 95.96(15) . 1_655 ?
Al1 O26 Fe9 117.58(15) 1_655 1_655 ?
P8 O26 Na2 103.41(18) . . ?
Al1 O26 Na2 95.39(15) 1_655 . ?
Fe9 O26 Na2 95.11(14) 1_655 . ?
P8 O26 O30 33.11(11) . . ?
Al1 O26 O30 108.77(16) 1_655 . ?
Fe9 O26 O30 112.13(15) 1_655 . ?
Na2 O26 O30 127.41(19) . . ?
P7 O27 Fe4 141.7(2) . . ?
P7 O27 Fe8 98.13(16) . 1_455 ?
Fe4 O27 Fe8 111.32(15) . 1_455 ?
P7 O27 Na1 95.43(17) . 1_554 ?
Fe4 O27 Na1 100.96(15) . 1_554 ?
Fe8 O27 Na1 103.04(15) 1_455 1_554 ?
P7 O27 O31 33.15(11) . . ?
Fe4 O27 O31 109.44(16) . . ?
Fe8 O27 O31 114.60(15) 1_455 . ?
Na1 O27 O31 116.58(17) 1_554 . ?
P8 O28 Fe5 138.5(2) . 1_545 ?
P8 O28 Fe9 98.43(16) . 1_655 ?
Fe5 O28 Fe9 109.80(14) 1_545 1_655 ?
P8 O28 Na1 96.44(17) . 1_645 ?
Fe5 O28 Na1 102.32(15) 1_545 1_645 ?
Fe9 O28 Na1 108.58(16) 1_655 1_645 ?
P8 O28 O30 34.14(11) . . ?
Fe5 O28 O30 134.89(17) 1_545 . ?
Fe9 O28 O30 115.30(15) 1_655 . ?
Na1 O28 O30 63.29(14) 1_645 . ?
P8 O28 Fe13 70.99(13) . 4 ?
Fe5 O28 Fe13 69.92(9) 1_545 4 ?
Fe9 O28 Fe13 114.30(12) 1_655 4 ?
Na1 O28 Fe13 136.52(15) 1_645 4 ?
O30 O28 Fe13 91.40(13) . 4 ?
P7 O29 Fe6 135.6(2) 1_556 . ?
P7 O29 Mn 99.09(17) 1_556 . ?
Fe6 O29 Mn 102.18(13) . . ?
P7 O29 O31 35.87(12) 1_556 1_556 ?
Fe6 O29 O31 143.20(17) . 1_556 ?
Mn O29 O31 63.35(12) . 1_556 ?
P7 O29 Na1 91.52(17) 1_556 . ?
Fe6 O29 Na1 97.31(14) . . ?
Mn O29 Na1 138.71(16) . . ?
O31 O29 Na1 115.93(16) 1_556 . ?
P7 O29 Fe1 113.20(16) 1_556 1_565 ?
Fe6 O29 Fe1 111.17(11) . 1_565 ?
Mn O29 Fe1 61.03(8) . 1_565 ?
O31 O29 Fe1 91.74(13) 1_556 1_565 ?
Na1 O29 Fe1 78.07(11) . 1_565 ?
P8 O30 Fe7 132.5(2) . 1_556 ?
P8 O30 O32 35.28(12) . . ?
Fe7 O30 O32 142.61(18) 1_556 . ?
P8 O30 O28 34.54(12) . . ?
Fe7 O30 O28 134.88(18) 1_556 . ?
O32 O30 O28 60.82(14) . . ?
P8 O30 Na1 88.63(17) . 1_645 ?
Fe7 O30 Na1 97.23(15) 1_556 1_645 ?
O32 O30 Na1 113.62(16) . 1_645 ?
O28 O30 Na1 55.00(13) . 1_645 ?
P8 O30 O26 33.91(11) . . ?
Fe7 O30 O26 98.67(14) 1_556 . ?
O32 O30 O26 59.37(13) . . ?
O28 O30 O26 56.36(12) . . ?
Na1 O30 O26 95.45(15) 1_645 . ?
P8 O30 O10 89.27(16) . 1_556 ?
Fe7 O30 O10 50.10(9) 1_556 1_556 ?
O32 O30 O10 93.25(15) . 1_556 ?
O28 O30 O10 114.65(15) . 1_556 ?
Na1 O30 O10 126.60(16) 1_645 1_556 ?
O26 O30 O10 58.86(11) . 1_556 ?
P8 O30 O17 106.33(18) . 1_656 ?
Fe7 O30 O17 46.77(10) 1_556 1_656 ?
O32 O30 O17 140.89(17) . 1_656 ?
O28 O30 O17 90.23(15) . 1_656 ?
Na1 O30 O17 55.17(12) 1_645 1_656 ?
O26 O30 O17 83.19(14) . 1_656 ?
O10 O30 O17 74.56(12) 1_556 1_656 ?
P8 O30 Mn 80.48(15) . 3_545 ?
Fe7 O30 Mn 114.16(14) 1_556 3_545 ?
O32 O30 Mn 45.99(11) . 3_545 ?
O28 O30 Mn 105.01(14) . 3_545 ?
Na1 O30 Mn 145.65(15) 1_645 3_545 ?
O26 O30 Mn 93.35(13) . 3_545 ?
O10 O30 Mn 86.02(12) 1_556 3_545 ?
O17 O30 Mn 159.14(15) 1_656 3_545 ?
P8 O30 O1 159.2(2) . 3_546 ?
Fe7 O30 O1 41.77(9) 1_556 3_546 ?
O32 O30 O1 164.97(18) . 3_546 ?
O28 O30 O1 129.17(17) . 3_546 ?
Na1 O30 O1 74.28(13) 1_645 3_546 ?
O26 O30 O1 134.43(16) . 3_546 ?
O10 O30 O1 91.50(13) 1_556 3_546 ?
O17 O30 O1 54.13(11) 1_656 3_546 ?
Mn O30 O1 120.32(13) 3_545 3_546 ?
P8 O30 O14 127.96(19) . 3_546 ?
Fe7 O30 O14 42.99(9) 1_556 3_546 ?
O32 O30 O14 109.22(16) . 3_546 ?
O28 O30 O14 160.72(16) . 3_546 ?
Na1 O30 O14 137.12(16) 1_645 3_546 ?
O26 O30 O14 104.51(14) . 3_546 ?
O10 O30 O14 47.03(10) 1_556 3_546 ?
O17 O30 O14 89.61(13) 1_656 3_546 ?
Mn O30 O14 71.28(10) 3_545 3_546 ?
O1 O30 O14 64.57(11) 3_546 3_546 ?
P8 O30 Na3 125.33(18) . 3_546 ?
Fe7 O30 Na3 102.13(12) 1_556 3_546 ?
O32 O30 Na3 101.22(15) . 3_546 ?
O28 O30 Na3 108.76(14) . 3_546 ?
Na1 O30 Na3 84.91(12) 1_645 3_546 ?
O26 O30 Na3 159.00(15) . 3_546 ?
O10 O30 Na3 135.89(14) 1_556 3_546 ?
O17 O30 Na3 113.47(13) 1_656 3_546 ?
Mn O30 Na3 75.48(9) 3_545 3_546 ?
O1 O30 Na3 65.90(10) 3_546 3_546 ?
O14 O30 Na3 88.92(11) 3_546 3_546 ?
P8 O30 O15 91.98(17) . 3_545 ?
Fe7 O30 O15 130.11(15) 1_556 3_545 ?
O32 O30 O15 61.96(13) . 3_545 ?
O28 O30 O15 93.95(14) . 3_545 ?
Na1 O30 O15 106.44(14) 1_645 3_545 ?
O26 O30 O15 121.31(15) . 3_545 ?
O10 O30 O15 126.97(15) 1_556 3_545 ?
O17 O30 O15 152.60(15) 1_656 3_545 ?
Mn O30 O15 42.31(8) 3_545 3_545 ?
O1 O30 O15 104.04(13) 3_546 3_545 ?
O14 O30 O15 95.03(13) 3_546 3_545 ?
Na3 O30 O15 39.91(8) 3_546 3_545 ?
P8 O30 P4 101.24(16) . 1_556 ?
Fe7 O30 P4 55.31(8) 1_556 1_556 ?
O32 O30 P4 89.08(13) . 1_556 ?
O28 O30 P4 133.96(14) . 1_556 ?
Na1 O30 P4 149.87(15) 1_645 1_556 ?
O26 O30 P4 78.81(11) . 1_556 ?
O10 O30 P4 27.30(7) 1_556 1_556 ?
O17 O30 P4 94.70(11) 1_656 1_556 ?
Mn O30 P4 64.48(7) 3_545 1_556 ?
O1 O30 P4 88.62(10) 3_546 1_556 ?
O14 O30 P4 27.00(7) 3_546 1_556 ?
Na3 O30 P4 110.89(11) 3_546 1_556 ?
O15 O30 P4 101.64(12) 3_545 1_556 ?
P8 O30 O16 86.77(16) . 3_546 ?
Fe7 O30 O16 80.89(12) 1_556 3_546 ?
O32 O30 O16 65.50(13) . 3_546 ?
O28 O30 O16 121.14(15) . 3_546 ?
Na1 O30 O16 171.68(16) 1_645 3_546 ?
O26 O30 O16 76.91(12) . 3_546 ?
O10 O30 O16 46.47(10) 1_556 3_546 ?
O17 O30 O16 119.76(14) 1_656 3_546 ?
Mn O30 O16 39.87(7) 3_545 3_546 ?
O1 O30 O16 108.62(13) 3_546 3_546 ?
O14 O30 O16 44.24(9) 3_546 3_546 ?
Na3 O30 O16 103.40(12) 3_546 3_546 ?
O15 O30 O16 80.67(11) 3_545 3_546 ?
P4 O30 O16 26.03(6) 1_556 3_546 ?
P8 O30 Al1 62.50(12) . 1_655 ?
Fe7 O30 Al1 71.00(9) 1_556 1_655 ?
O32 O30 Al1 79.39(12) . 1_655 ?
O28 O30 Al1 84.11(11) . 1_655 ?
Na1 O30 Al1 108.05(13) 1_645 1_655 ?
O26 O30 Al1 29.37(8) . 1_655 ?
O10 O30 Al1 30.58(7) 1_556 1_655 ?
O17 O30 Al1 71.44(10) 1_656 1_655 ?
Mn O30 Al1 95.64(10) 3_545 1_655 ?
O1 O30 Al1 111.10(12) 3_546 1_655 ?
O14 O30 Al1 77.56(10) 3_546 1_655 ?
Na3 O30 Al1 165.75(13) 3_546 1_655 ?
O15 O30 Al1 135.91(13) 3_545 1_655 ?
P4 O30 Al1 54.87(6) 1_556 1_655 ?
O16 O30 Al1 63.66(8) 3_546 1_655 ?
P7 O31 Fe12 130.2(2) . . ?
P7 O31 O29 36.21(12) . 1_554 ?
Fe12 O31 O29 146.30(18) . 1_554 ?
P7 O31 Mn 90.47(16) . 1_554 ?
Fe12 O31 Mn 124.17(15) . 1_554 ?
O29 O31 Mn 54.37(11) 1_554 1_554 ?
P7 O31 O25 34.21(11) . . ?
Fe12 O31 O25 129.26(17) . . ?
O29 O31 O25 60.89(13) 1_554 . ?
Mn O31 O25 106.08(14) 1_554 . ?
P7 O31 O27 33.60(11) . . ?
Fe12 O31 O27 97.14(14) . . ?
O29 O31 O27 59.80(13) 1_554 . ?
Mn O31 O27 109.10(15) 1_554 . ?
O25 O31 O27 56.43(12) . . ?
P7 O31 O40 101.12(18) . . ?
Fe12 O31 O40 46.59(10) . . ?
O29 O31 O40 137.15(17) 1_554 . ?
Mn O31 O40 168.39(16) 1_554 . ?
O25 O31 O40 84.30(14) . . ?
O27 O31 O40 80.83(14) . . ?
P7 O31 O14 146.5(2) . . ?
Fe12 O31 O14 44.35(9) . . ?
O29 O31 O14 123.59(16) 1_554 . ?
Mn O31 O14 80.18(11) 1_554 . ?
O25 O31 O14 173.59(17) . . ?
O27 O31 O14 120.62(16) . . ?
O40 O31 O14 89.61(13) . . ?
P7 O31 O49 93.70(17) . . ?
Fe12 O31 O49 47.34(11) . . ?
O29 O31 O49 98.97(16) 1_554 . ?
Mn O31 O49 104.35(14) 1_554 . ?
O25 O31 O49 117.56(16) . . ?
O27 O31 O49 62.49(13) . . ?
O40 O31 O49 74.43(13) . . ?
O14 O31 O49 58.51(11) . . ?
P7 O31 Na4 78.78(15) . . ?
Fe12 O31 Na4 92.62(13) . . ?
O29 O31 Na4 107.61(14) 1_554 . ?
Mn O31 Na4 137.14(14) 1_554 . ?
O25 O31 Na4 47.09(10) . . ?
O27 O31 Na4 84.17(13) . . ?
O40 O31 Na4 47.79(10) . . ?
O14 O31 Na4 128.79(14) . . ?
O49 O31 Na4 117.55(14) . . ?
P7 O31 O15 93.03(16) . 1_554 ?
Fe12 O31 O15 136.56(16) . 1_554 ?
O29 O31 O15 71.02(13) 1_554 1_554 ?
Mn O31 O15 47.20(9) 1_554 1_554 ?
O25 O31 O15 82.31(13) . 1_554 ?
O27 O31 O15 126.30(15) . 1_554 ?
O40 O31 O15 131.70(16) . 1_554 ?
O14 O31 O15 103.33(13) . 1_554 ?
O49 O31 O15 150.80(16) . 1_554 ?
Na4 O31 O15 91.63(12) . 1_554 ?
P7 O31 O16 103.64(18) . . ?
Fe12 O31 O16 84.33(12) . . ?
O29 O31 O16 75.37(13) 1_554 . ?
Mn O31 O16 45.29(9) 1_554 . ?
O25 O31 O16 135.73(16) . . ?
O27 O31 O16 96.77(15) . . ?
O40 O31 O16 129.38(15) . . ?
O14 O31 O16 48.25(10) . . ?
O49 O31 O16 60.61(12) . . ?
Na4 O31 O16 176.89(14) . . ?
O15 O31 O16 90.20(13) 1_554 . ?
P7 O31 O8 149.2(2) . . ?
Fe12 O31 O8 45.21(10) . . ?
O29 O31 O8 167.28(17) 1_554 . ?
Mn O31 O8 117.17(14) 1_554 . ?
O25 O31 O8 118.48(16) . . ?
O27 O31 O8 131.71(16) . . ?
O40 O31 O8 51.85(11) . . ?
O14 O31 O8 58.35(11) . . ?
O49 O31 O8 92.35(14) . . ?
Na4 O31 O8 71.64(11) . . ?
O15 O31 O8 96.27(13) 1_554 . ?
O16 O31 O8 105.66(13) . . ?
P7 O31 Na3 122.51(17) . . ?
Fe12 O31 Na3 101.15(13) . . ?
O29 O31 Na3 110.03(14) 1_554 . ?
Mn O31 Na3 77.30(9) 1_554 . ?
O25 O31 Na3 95.78(13) . . ?
O27 O31 Na3 152.20(15) . . ?
O40 O31 Na3 96.78(13) . . ?
O14 O31 Na3 86.91(11) . . ?
O49 O31 Na3 143.79(14) . . ?
Na4 O31 Na3 74.30(10) . . ?
O15 O31 Na3 39.49(8) 1_554 . ?
O16 O31 Na3 105.68(12) . . ?
O8 O31 Na3 57.32(10) . . ?
P8 O32 Mn 112.48(19) . 3_545 ?
P8 O32 Fe13 133.4(2) . 4 ?
Mn O32 Fe13 104.89(15) 3_545 4 ?
P8 O32 O30 35.10(12) . . ?
Mn O32 O30 78.52(14) 3_545 . ?
Fe13 O32 O30 143.46(18) 4 . ?
P8 O32 Na2 86.93(17) . . ?
Mn O32 Na2 122.52(16) 3_545 . ?
Fe13 O32 Na2 95.85(14) 4 . ?
O30 O32 Na2 113.16(16) . . ?
P8 O32 Fe1 113.51(16) . 3 ?
Mn O32 Fe1 53.43(8) 3_545 3 ?
Fe13 O32 Fe1 110.78(12) 4 3 ?
O30 O32 Fe1 100.41(13) . 3 ?
Na2 O32 Fe1 69.12(10) . 3 ?
P9 O33 Fe9 139.4(2) . 1_655 ?
P9 O33 Na2 92.40(18) . . ?
Fe9 O33 Na2 95.33(15) 1_655 . ?
P9 O33 K1 93.57(16) . 2_565 ?
Fe9 O33 K1 123.04(16) 1_655 2_565 ?
Na2 O33 K1 102.95(14) . 2_565 ?
P9 O33 Fe13 44.54(11) . 4 ?
Fe9 O33 Fe13 105.75(13) 1_655 4 ?
Na2 O33 Fe13 63.54(11) . 4 ?
K1 O33 Fe13 130.78(11) 2_565 4 ?
P10 O34 Fe8 137.5(2) . 1_455 ?
P10 O34 Na4 94.01(18) . . ?
Fe8 O34 Na4 96.45(14) 1_455 . ?
P10 O34 K1 96.30(15) . 1_455 ?
Fe8 O34 K1 122.22(16) 1_455 1_455 ?
Na4 O34 K1 99.41(13) . 1_455 ?
P10 O34 O31 76.64(14) . . ?
Fe8 O34 O31 78.78(11) 1_455 . ?
Na4 O34 O31 50.48(10) . . ?
K1 O34 O31 147.42(13) 1_455 . ?
P10 O34 Fe11 139.62(17) . 3_455 ?
Fe8 O34 Fe11 56.97(9) 1_455 3_455 ?
Na4 O34 Fe11 124.57(13) . 3_455 ?
K1 O34 Fe11 68.46(8) 1_455 3_455 ?
O31 O34 Fe11 135.48(10) . 3_455 ?
P9 O35 Fe11 140.8(2) 2_564 3 ?
P9 O35 K1 103.16(18) 2_564 . ?
Fe11 O35 K1 115.94(16) 3 . ?
P9 O35 Fe3 72.99(15) 2_564 2_564 ?
Fe11 O35 Fe3 93.43(14) 3 2_564 ?
K1 O35 Fe3 104.85(12) . 2_564 ?
P9 O35 Fe2 68.07(14) 2_564 3 ?
Fe11 O35 Fe2 78.75(11) 3 3 ?
K1 O35 Fe2 150.13(15) . 3 ?
Fe3 O35 Fe2 99.71(9) 2_564 3 ?
P10 O36 Fe10 141.1(2) . 2_564 ?
P10 O36 K1 100.48(17) . 1_455 ?
Fe10 O36 K1 118.24(15) 2_564 1_455 ?
P10 O36 Fe2 75.71(15) . . ?
Fe10 O36 Fe2 94.77(14) 2_564 . ?
K1 O36 Fe2 107.74(12) 1_455 . ?
P10 O36 Fe3 65.86(13) . 4_464 ?
Fe10 O36 Fe3 78.90(11) 2_564 4_464 ?
K1 O36 Fe3 146.25(14) 1_455 4_464 ?
Fe2 O36 Fe3 98.76(9) . 4_464 ?
P9 O37 Fe5 131.8(2) . 1_545 ?
P9 O37 Fe2 129.8(2) . 4 ?
Fe5 O37 Fe2 97.40(16) 1_545 4 ?
P9 O37 Fe13 81.57(18) . 4 ?
Fe5 O37 Fe13 84.31(14) 1_545 4 ?
Fe2 O37 Fe13 96.45(16) 4 4 ?
P9 O37 Fe11 59.92(13) . 4 ?
Fe5 O37 Fe11 167.84(17) 1_545 4 ?
Fe2 O37 Fe11 71.90(10) 4 4 ?
Fe13 O37 Fe11 102.29(11) 4 4 ?
P10 O38 Fe3 129.4(2) . 4_464 ?
P10 O38 Fe4 128.8(2) . . ?
Fe3 O38 Fe4 96.01(14) 4_464 . ?
P10 O38 O31 70.78(14) . . ?
Fe3 O38 O31 121.25(15) 4_464 . ?
Fe4 O38 O31 64.97(10) . . ?
P9 O39 Fe3 128.7(2) . . ?
P9 O39 Fe13 116.0(2) . 4 ?
Fe3 O39 Fe13 106.65(16) . 4 ?
P9 O39 Na2 99.9(2) . . ?
Fe3 O39 Na2 91.32(15) . . ?
Fe13 O39 Na2 109.04(17) 4 . ?
P9 O39 Fe11 56.55(12) . 4 ?
Fe3 O39 Fe11 78.50(10) . 4 ?
Fe13 O39 Fe11 119.83(14) 4 4 ?
Na2 O39 Fe11 131.02(16) . 4 ?
P9 O39 Fe2 55.08(13) . 4 ?
Fe3 O39 Fe2 120.49(14) . 4 ?
Fe13 O39 Fe2 71.59(10) 4 4 ?
Na2 O39 Fe2 147.19(15) . 4 ?
Fe11 O39 Fe2 56.85(5) 4 4 ?
P10 O40 Fe12 123.7(2) . . ?
P10 O40 Fe2 125.3(2) . . ?
Fe12 O40 Fe2 102.33(15) . . ?
P10 O40 Na4 96.42(18) . . ?
Fe12 O40 Na4 112.42(16) . . ?
Fe2 O40 Na4 90.89(15) . . ?
P10 O40 O31 115.9(2) . . ?
Fe12 O40 O31 46.76(10) . . ?
Fe2 O40 O31 117.06(15) . . ?
Na4 O40 O31 68.08(12) . . ?
P10 O40 Fe3 56.19(12) . 4_464 ?
Fe12 O40 Fe3 76.61(11) . 4_464 ?
Fe2 O40 Fe3 118.52(13) . 4_464 ?
Na4 O40 Fe3 147.47(15) . 4_464 ?
O31 O40 Fe3 105.85(13) . 4_464 ?
P11 O41 Fe6 131.7(2) . 1_655 ?
P11 O41 Na2 89.19(19) . . ?
Fe6 O41 Na2 97.94(15) 1_655 . ?
P11 O41 Na5 91.94(18) . 1_655 ?
Fe6 O41 Na5 87.17(15) 1_655 1_655 ?
Na2 O41 Na5 172.06(18) . 1_655 ?
P11 O41 K1 97.60(16) . 2_565 ?
Fe6 O41 K1 127.50(16) 1_655 2_565 ?
Na2 O41 K1 99.91(13) . 2_565 ?
Na5 O41 K1 72.15(11) 1_655 2_565 ?
P11 O41 Fe3 41.99(12) . . ?
Fe6 O41 Fe3 142.22(16) 1_655 . ?
Na2 O41 Fe3 52.44(9) . . ?
Na5 O41 Fe3 125.28(13) 1_655 . ?
K1 O41 Fe3 84.81(9) 2_565 . ?
P12 O42 Fe7 133.9(2) . 1_455 ?
P12 O42 Na4 93.95(18) . . ?
Fe7 O42 Na4 103.90(15) 1_455 . ?
P12 O42 K1 96.96(15) . 1_455 ?
Fe7 O42 K1 121.79(16) 1_455 1_455 ?
Na4 O42 K1 97.12(12) . 1_455 ?
P12 O42 Fe2 44.31(11) . . ?
Fe7 O42 Fe2 147.93(15) 1_455 . ?
Na4 O42 Fe2 52.91(9) . . ?
K1 O42 Fe2 86.08(8) 1_455 . ?
P11 O43 Fe12 135.2(3) 2_564 3_545 ?
P11 O43 K1 103.7(2) 2_564 . ?
Fe12 O43 K1 116.5(2) 3_545 . ?
P11 O43 Fe3 80.4(2) 2_564 2_564 ?
Fe12 O43 Fe3 101.5(2) 3_545 2_564 ?
K1 O43 Fe3 110.88(16) . 2_564 ?
P11 O43 Fe2 68.81(16) 2_564 3_545 ?
Fe12 O43 Fe2 68.01(12) 3_545 3_545 ?
K1 O43 Fe2 139.0(2) . 3_545 ?
Fe3 O43 Fe2 107.45(14) 2_564 3_545 ?
P11 O43 Fe11 140.3(3) 2_564 3 ?
Fe12 O43 Fe11 76.70(12) 3_545 3 ?
K1 O43 Fe11 67.72(9) . 3 ?
Fe3 O43 Fe11 68.33(10) 2_564 3 ?
Fe2 O43 Fe11 142.95(12) 3_545 3 ?
P12 O44 Fe13 132.4(2) . . ?
P12 O44 Na5 94.4(2) . 2_564 ?
Fe13 O44 Na5 94.78(18) . 2_564 ?
P12 O44 K1 103.97(19) . 1_455 ?
Fe13 O44 K1 123.51(17) . 1_455 ?
Na5 O44 K1 74.42(14) 2_564 1_455 ?
P12 O44 Fe2 75.26(19) . . ?
Fe13 O44 Fe2 92.09(16) . . ?
Na5 O44 Fe2 169.70(15) 2_564 . ?
K1 O44 Fe2 107.98(14) 1_455 . ?
P12 O44 Fe3 69.79(15) . 4_454 ?
Fe13 O44 Fe3 69.56(11) . 4_454 ?
Na5 O44 Fe3 70.85(11) 2_564 4_454 ?
K1 O44 Fe3 143.92(17) 1_455 4_454 ?
Fe2 O44 Fe3 104.58(12) . 4_454 ?
P11 O45 Fe5 128.4(2) . . ?
P11 O45 Fe2 130.3(2) . 4_565 ?
Fe5 O45 Fe2 101.04(14) . 4_565 ?
P11 O45 Na5 78.57(16) . 1_655 ?
Fe5 O45 Na5 94.39(15) . 1_655 ?
Fe2 O45 Na5 105.30(15) 4_565 1_655 ?
P12 O46 Fe4 128.4(2) . 1_545 ?
P12 O46 Fe3 132.4(2) . 4_454 ?
Fe4 O46 Fe3 99.17(15) 1_545 4_454 ?
P12 O46 Fe11 85.41(16) . . ?
Fe4 O46 Fe11 83.50(12) 1_545 . ?
Fe3 O46 Fe11 99.80(13) 4_454 . ?
P12 O46 Fe13 65.17(12) . . ?
Fe4 O46 Fe13 165.37(15) 1_545 . ?
Fe3 O46 Fe13 67.78(9) 4_454 . ?
Fe11 O46 Fe13 104.68(10) . . ?
P11 O47 Fe3 114.4(2) . . ?
P11 O47 Fe10 116.7(2) . 3 ?
Fe3 O47 Fe10 113.45(17) . 3 ?
P11 O47 Na2 97.1(2) . . ?
Fe3 O47 Na2 90.90(16) . . ?
Fe10 O47 Na2 120.94(19) 3 . ?
P11 O47 Fe2 51.00(12) . 4_565 ?
Fe3 O47 Fe2 113.32(14) . 4_565 ?
Fe10 O47 Fe2 73.23(10) 3 4_565 ?
Na2 O47 Fe2 145.26(17) . 4_565 ?
P12 O48 Fe2 121.6(2) . . ?
P12 O48 Na4 92.17(19) . . ?
Fe2 O48 Na4 93.21(16) . . ?
P12 O48 Fe11 113.7(2) . . ?
Fe2 O48 Fe11 112.54(17) . . ?
Na4 O48 Fe11 120.87(18) . . ?
P12 O48 Fe13 55.86(13) . . ?
Fe2 O48 Fe13 74.16(11) . . ?
Na4 O48 Fe13 124.68(16) . . ?
Fe11 O48 Fe13 113.54(12) . . ?
P12 O48 Fe3 51.39(12) . 4_454 ?
Fe2 O48 Fe3 116.70(14) . 4_454 ?
Na4 O48 Fe3 140.84(15) . 4_454 ?
Fe11 O48 Fe3 72.24(9) . 4_454 ?
Fe13 O48 Fe3 50.82(5) . 4_454 ?
P12 O48 Na3 143.3(2) . . ?
Fe2 O48 Na3 91.41(12) . . ?
Na4 O48 Na3 68.53(11) . . ?
Fe11 O48 Na3 59.05(9) . . ?
Fe13 O48 Na3 160.19(11) . . ?
Fe3 O48 Na3 130.42(11) 4_454 . ?
Fe4 O49 Fe12 113.42(17) . . ?
Fe4 O49 Fe11 109.74(16) . 1_565 ?
Fe12 O49 Fe11 133.09(19) . 1_565 ?
Fe4 O49 O31 93.08(15) . . ?
Fe12 O49 O31 45.21(9) . . ?
Fe11 O49 O31 147.93(18) 1_565 . ?
Fe4 O49 Fe3 67.20(11) . 4_464 ?
Fe12 O49 Fe3 89.01(13) . 4_464 ?
Fe11 O49 Fe3 91.30(12) 1_565 4_464 ?
O31 O49 Fe3 118.86(14) . 4_464 ?
Fe4 O49 Fe1 102.91(15) . 1_564 ?
Fe12 O49 Fe1 111.62(13) . 1_564 ?
Fe11 O49 Fe1 74.66(10) 1_565 1_564 ?
O31 O49 Fe1 78.55(11) . 1_564 ?
Fe3 O49 Fe1 159.37(12) 4_464 1_564 ?
Fe5 O50 Fe13 109.81(15) 3_445 2_565 ?
Fe5 O50 Fe10 112.55(15) 3_445 . ?
Fe13 O50 Fe10 129.47(17) 2_565 . ?
Fe5 O50 Fe2 65.70(9) 3_445 2_565 ?
Fe13 O50 Fe2 84.39(11) 2_565 2_565 ?
Fe10 O50 Fe2 88.89(11) . 2_565 ?
Fe5 O50 O30 78.27(11) 3_445 3_455 ?
Fe13 O50 O30 84.04(11) 2_565 3_455 ?
Fe10 O50 O30 130.34(14) . 3_455 ?
Fe2 O50 O30 135.43(11) 2_565 3_455 ?
 
_refine_diff_density_max    1.878
_refine_diff_density_min   -0.876
_refine_diff_density_rms    0.123
